This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!
(1.4)
where A is introduced to distinguish operators from oneparticle states. Here (• • •) denotes the statistical average, and g(x — xf) is the short range correlation within the de Broglie wavelength at a temperature T. It is assumed that the wave function \po(x) of the condensate changes only over a macroscopic scale. In the high temperature phase there is only short range order. In the state with the BE condensate, p(x,x!) remains finite and of the order of the particle density, however large \x — xf\ is. Moreover, its dependence on x and xr is given, so to speak, independently by the wave function xpQ. This implies that there exists a kind of long range order. Since it appears in the offdiagonal component of the density matrix, it is called the ODLRO (oi diagonal long range order). This should be compared with the crystalline order given by (xp^(x)xp(x)xp\xr)xp(xf)) ~ n(x)n(xf), where n(x) is the density variation with lattice periodicity. If we substitute the mass of a 4 He atom into m and the density n of liquid 4 He into N/V in Eq. (1.3), we obtain T BE = 3.13 K, which is not very different from Tx = 2.17 K for actual liquid 4 He. Also entropy at
8
Superconductivity and superfluidity
is not much different from its value at Tx for the actual liquid. For these reasons F. London has proposed that the superfluidity of 4 He is due to the BE condensation.
1.2.1 Dilute Bose gas Let us show that one may explain the facts outlined in Section 1.1 qualitatively if one uses a macroscopic wave function corresponding to the condensate of an ideal Bose gas. To concentrate on the superfluid component our arguments will be limited to the case T = 0. To mimic real liquid 4 He, however, it is assumed that a weak repulsive interaction exists between particles. The Hamiltonian of the system in the secondquantised form is
H = fdxl ^l
+ jJ
(1.5)
where U is a weak repulsive interaction and \x is the chemical potential introduced so that the total particle number is N. The ground state of an ideal Bose gas is ^
(16)
where aj creates a particle in the state xpo(x) of the condensate and 0) is the vacuum state. One may employ the same state as a first order approximation provided that the interaction is sufficiently weak. This yields the lowest order approximation to a dilute Bose gas. The state xpo(x) must be determined by the Hartree approximation, namely the state is obtained by minimising Let us take a potential the energy expectation value £o = (^ONIH^ON)2 U(x) = gd(x) for simplicity. We put g = 4nah /m if U(x) is to represent a hard core with radius a. Then we obtain
The wave function xpo(x) is a complex number and \p$ and \po are regarded as being independent of each other. Thus the wave function ipo(x) is obtained from the condition dEo/dxp^ = 0, that is h2
 2^ v 2 ^o  Wo + glvol V ) = 0
(1.7)
1.2 Bose gas and macroscopic wave function
9
This is a nonlinear Schrodinger equation similar to the GinzburgLandau equation studied in Chapter 5. Since = li/g = ns in a uniform state, where the superfluid particle density ns is given approximately by N/V in the present case, Eq. (1.7) can be rewritten as
j
= 0.
(1.8)
Here we have introduced the healing distance If \xpo\2 deviates from ns at a certain point, it recovers the value ns in about the healing distance. The momentum density g(x) = (fi/2i) • {xp*Vxp — Vxp* • xp} has an expectation value (1.10) in the present state, where xpo and xpy have been written in terms of the amplitude and the phase as
Therefore the velocity field vs = (g)/mns is that of a potential flow whose potential is the phase of the macroscopic wave function and the circulation around a closed loop in the fluid is quantised as pK, p being an integer and K given by Eq. (1.2). The solution of Eq. (1.8) for a vortex line along the zaxis takes the form ipo = yJns(x)Qlp0 and the velocity field is given by VSQ = pKJr. The density ns approaches zero along the zaxis, where vs diverges, and as a result a vortex has a core of radius ~ £. Quantised vortices in superfluid 4 He with p = 1 have been observed by various methods and it is known that £  1 A. 1.2.2 Charged Bose gas We have considered a neutral Bose gas so far. Suppose now that a Bose gas has an electric charge e*. (It is assumed, of course, that charges of an opposite sign are distributed uniformly in space and the screened Coulomb interaction between gas particles is taken into account in the definition of g.) Since particles couple with a magnetic field in this case, one makes the substitution
10
Superconductivity and superfluidity
Id
Fig. 1.7. Penetration of a magnetic field into a superconducting plate.
where ^4 is the vector potential. Note in particular that the current density corresponding to (g) is now
<>•>£*
(1.11)
Where the scale of the spatial variation of the system is larger than £ one may put ns ~ ns. Then, when combined with the Maxwell equation V x B = (4n/c)(js), the following equation is obtained,
V2B 
= 0,
(1.12)
where AL is called the London penetration depth. If the density ~ 1023 cm  3 of conduction electrons in a metal is substituted for nS9 and m* and e* are replaced by m and e of an electron, one obtains X^ ~ 10~5 cm. Let us consider an actual example to see that Eq. (1.12) leads to the Meissner effect. Suppose a superconducting plate of thickness Id is placed in an external magnetic field H parallel to the plate. If Eq. (1.12) is solved in this case with the boundary conditions Bz(±d) = if, one obtains the solution Bz(x) = H
d).
Accordingly, for d > AL? there is a current js along the +ydirections within a thickness AL of the surface of the plate and the magnetic field does not penetrate into the interior of the sample, see Fig. 1.7 Let us show next that this system leads to flux quantisation. Suppose a magnetic flux is trapped in the cavity of a superconducting cylinder as shown in Fig. 1.8. Since B = 0 and (ys) = 0 along the dotted line C provided that
1.3 Symmetry breaking
11
Fig. 1.8. A superconducting cylinder. d > AL, it follows from Eq. (1.11) that c
V<£d/ =
By Stokes theorem, the right hand side of this equation is shown to be equal to (e* /hc) in the left hand side is a phase, its total variation along C must be an integral multiple of In. Thus one is lead to he
(p = integer).
(1.13)
In fact, the observed flux quantisation in a superconductor is obtained if one puts e* = 2e, which suggests that the superfluid consists of pairs of electrons. One reaches the identical conclusion even if an external magnetic flux exists only inside the cavity of the cylinder and the superconductor is not immersed in the field B directly. This is a good example of the AharonovBohm effect, which states that a gauge field A itself has a physical meaning in quantum mechanics.
1.3 Symmetry breaking The properties of a superfluid are best described by the wave function xpo(x) as seen in the previous section. However, in a state with a condensate such as Eq. (1.6), one cannot regard the expectation value of xp(x) as xpo(x) since it vanishes provided the total number of particles is conserved. The density is rather inconvenient. Rather than matrix of the form {X¥ON\W\X)W(X')\ X¥ON) consider the density matrix (1.4), we introduce the matrix elements }.
(1.14)
12
Superconductivity and superfluidity
One may consider, for the same purpose, expectation values with respect to the state m
(1.15) which is an appropriate superposition of states with different N with 1 m
(1.17)
The expectation value itself changes as (xp(x)) —• elcc(\p(x)). The Hamiltonian of a system may be left invariant under various transformations in general and the normal state observes this invariance. Ordering of a system implies that the system undergoes a transition to a state with less symmetries, that is, invariance under some transformations has been lost. The symmetry breaking associated with superconducting and superfluid transitions is gauge symmetry breaking. It should be noted here that if a system has an internal
1.4 Superfluidity
13
structure, such as the superfluid 3 He, the rotational symmetry is broken simultaneously. It is the Josephson effect, explained in Section 3.4, that shows the theory dealing with (xp) or {ipxp) without fixed particle number to be essential in describing superconductivity and superfluidity. (The experiments are not possible for superfluids so far but one expects the same effects exist there.) The effect demonstrates that when two superconductors A and B are weakly coupled through a tunnelling junction so that electrons may be exchanged, the electron numbers N\ and N& of respective superconductors do not take fixed values but the phase difference between the pair wave functions takes a definite value. In contrast to the case, for example, of a ferromagnet accompanied by a magnetic field, in superconductivity and superfluidity there is no symmetry breaking external physical field, that is, an external field that couples to the order parameter directly, To observe (xp(x)) 'directly', therefore, one has to couple the system with another similar system, such as a tunnelling junction, and see the response induced by the coupling. 1.4 Superfluidity
The particle number No of the condensate is less than N in the presence of an interaction even in the ground state at T = 0. Suppose particles form a condensate in the p = 0 state, there are processes in which two particles in the condensate may be scattered into states (/>, —p) for example, which make the expectation value of the particle number np for a finite p nonvanishing. Neutron scattering experiments as well as theoretical estimates in liquid 4 He yield the result No ^ 0.1N. The ODLRO exists, however, since the density matrix is of the form (1.4) so long as No is of the order of JV. The N — No particles in the present system must maintain a certain correlation with the condensate to lower the interaction energy. Therefore when the condensate flows with velocity vs, the system should look like the ground state for vs = 0 if seen by an observer moving with velocity vs. Thus one reaches the conclusion that all the particles, not just No particles, are thought of as the superfluid component. In other words, one has ns = n at T = 0 K. In reality, wall scattering occurs and it is a necessary condition for superfluidity that the flow does not decay by these scattering processes. In order to discuss this one has to know not only the ground state but the excited states. Suppose an elementary excitation with a momentum p has an energy sp. If the superfluid moves with a velocity vS9 an elementary excitation with momentum p in the comoving frame has the energy sp as mentioned above. The elementary excitation energy becomes sp +p • vs if one Galileitransforms
14
Superconductivity and superfluidity
Fig. 1.9. Elementary excitations in superfluid 4 He measured by neutron inelastic scattering. < g The interval p < 0.8 A is called the phonon region while 1.4 A p < 2.4 A is called the roton region. (From [G3].)
to the rest frame of the 'wall'. Therefore all the excitations should satisfy the Landau criterion >0
(1.18)
for the flow energy not to be lowered by creating excitations by scattering off a wall, that is, for the superflow to be stable. An ideal Bose gas does not satisfy this condition. Elementary excitations in liquid 4 He are phonons and rotons with the Landau spectrum shown in Fig. 1.9 and satisfy the above condition. The critical velocity vsc of a superflow is the minimal vs for which an equality in Eq. (1.18) is realised for a certain excitation. The critical velocity in the superfluid 4 He is determined in many cases not by the phonon or roton excitations but by quantised vortices. In the presence of an interaction, particlelike excitations with the energy spectrum p2/2m in an ideal Bose gas are absorbed into a collective mode called the sound wave (density wave) with the spectrum pvs. It was shown explicitly by the theory of an interacting dilute Bose gas (N.N. Bogoliubov, 1947, see [F2]) that the existence of a condensate is indispensable for this mechanism. Bogoliubov's theory starts with the mean field associated with the condensate. The Bogoliubov transformation employed in the theory of superconductivity first appeared in this context. In a dilute Bose gas considered in the previous section a fluctuation with wave number p around the condensate ipo = Jn~s has a spectrum of the phonon type. In order to see
1.4 Superfluidity
15
this, one considers the equation of motion corresponding to Eq. (1.7)
substitutes \p = ^Jf^ + 8\p and then linearises the resulting equation in dip. One finds as a result the eigenfrequency a>2 = (nsg/m)p2 + (p2/2m)2 which becomes a sound wave with dispersion vs = \/%g/m as p —• 0. At finite temperature there are phonon and roton excitations according to the equilibrium distribution in the rest frame of a 'wall'. Landau constructed the theory of superfluid 4 He from the viewpoint that these thermal excitations constitute the normal component, and successfully treated the thermodynamic properties and transport phenomena quantitatively. We also note R.P. Feynman's unique theory concerning the phonon and roton spectrum of the elementary excitations in superfluid 4 He (see [F2]).
2 Meanfield theory of pair condensation
The microscopic theory of superconductivity of metals was discovered by J. Bardeen, L.N. Cooper, and J.R. Schrieffer (BCS) in 1957. The key concept of the BCS theory is pair condensation. In the present chapter, the meanfield theory of superfluidity and superconductivity is developed for ordinary superconductors of singlet swave pairing and superfluid 3 He with triplet pwave pairing. Our formalism is applicable to such systems as neutron stars and heavy fermion superconductors where pairs have internal degrees of freedom.
2.1 Interactions and twoparticle bound states Bound state formation by two particles on the Fermi surface is called pairing. Before we discuss pairing in manybody systems, let us consider interaction between two fermions with spin 1/2 and their bound states. Suppose there exists an interaction Jffi between two particles, whose matrix element is given by (k+*9kP\Hi\*f+<J,*'P')
= VaPjp(k,k!)9
(2.1)
where \k+a9 —kfi) denotes a state vector of two fermions with momenta k+ = k + q/2 and — k = — k + q/2 and spins a and /?. This vector is also written in the secondquantised form as
where 0) indicates vacuum 1. a\a is an operator which creates a particle of momentum k and spin a. It is assumed, for simplicity, that the matrix 1
Vectorial subscripts will be denoted by ordinary italic letters hereafter if there is no risk of confusion. Accordingly a* is simply denoted by %.
16
2.1 Interactions and twoparticle bound states
17
element (2.1) is independent of q. It follows from the antisymmetry of fermionic operators that ^pKkr).
(2.2)
The matrix elements also satisfy the Hermiticity condition V^fi,(k,k') = Va!M(k',k).
(2.3)
Suppose the interaction H\ leaves the spin invariant. Then it follows from Eq. (2.2) that V(e\k,k')
* W ( * ' * ' ) = \ (<5a«'%  W )
+\ (<5a«'% +
(2.4)
Here k, k') = V{eUo\k, k') = ±V{e)'i0)(k, k'),
(2.5)
where (e) and (o) represent the even and the odd part of the interaction, respectively. If the interaction Hamiltonian is given by
for example, one obtains [7(*  k'\) ± V(\k + k'\)}.
(2.6)
Now let us consider a twoparticle system. The energy eigenstate with centre of mass momentum q can be written as
The coefficient Cap(k, q) is the wave function in the momentum representation and satisfies the antisymmetry ).
(2.7)
The Schrodinger equation in this representation is \±{k\
+ k2_) E)
CaP(k,q) + J2 VaWp>(k,k')C^ik\q) = 0.
(2.8)
When the interaction is spinindependent and hence satisfies Eq. (2.4) it
18
Meanfield theory of pair condensation
immediately follows that there are two classes of eigenfunctions, namely the spinsinglet state satisfying Cap(k, q) = CaP(k, q) = CPa(k, q)
(2.9)
and the spintriplet state satisfying CaP(k9 q) = Cafi(k,
q) = Cpa(k, q).
(2.10)
The spin indices and the symmetry indices (e) and (o) will be omitted and q = 0 will be taken, for simplicity, in the following. Then Eq. (2.8) is rewritten as A(*) =
Suppose the interaction is invariant under rotations in momentum space. Then the matrix element can be expanded as
V{k,kr) = V(k,k',k • k) = J^(2l + l)Vi(k,k')Pi(k • k) i i
where k = k/\k\ and Q^ is the solid angle. In this case, Eq. (2.11) can be written in terms of the partial wave component as 1
4
dW V k
r00
where A(k) has been decomposed as
**
1
A bound state corresponds to the solution with E < 0. It is not easy to find the solution to Eq. (2.13) due to a generally nontrivial dependence of V(k,kf) on k and k!. It can be shown, however, that if V\ is negative, bound states with an angular momentum / may exist. It can be seen from Eqs. (2.8) and (2.9) that a bound state with / even (odd) must be a spinsinglet (triplet) state. For example, the potential of a hydrogen atom is V\w = 4ne2/\k — k'\2 and the lsground state wave function is given by (see [G4])
n(l+k2)2'
2.2 Cooper pairs and the BCS ground state
19
Let us take an swave (/ = 0) interaction of a d function type such that the potential is given by Vo(k9k') ~ — X = const, for k,k f < Kc and = 0 otherwise. For an attractive potential (X > 0), solutions with E < 0 are determined by the condition
* £ ( * L y
v (2.14)
The above equation also gives the bound state condition for a threedimensional square well potential of depth U and width a if the parameters are chosen to be X = Ua3 and Kc = a~l. Note that there are no bound states unless 4nmKcX > 1. It should be also noted that Eq. (2.11) always has a bound state solution for a onedimensional problem however small X may be. 2.2 Cooper pairs and the BCS ground state
Due to the Pauli principle, not only an ideal Fermi gas, but an interacting Fermi system such as electrons in a metal and liquid 3 He, can, at low enough temperatures, be regarded as a system of quasiparticles obeying Fermi statistics; called the Fermi liquid. If there are no phase transitions, the ground state at T = 0 K is a Fermi sphere of quasiparticles. Let aj a be an operator which creates a quasiparticle (which we simply call a particle hereafter) of momentum k and spin a. Then the Fermi sphere is written as
where 0) is the vacuum state and the product is over the states inside the Fermi sphere. Let us recall that the number density n is given, in terms of the Fermi momentum k?, as n = /C/3TT2 and that the density of states on the Fermi surface, namely the number of oneparticle states per unit volume and unit energy, is mfcS dn(kF) d(k2F/2m)
n2 * '
where N(0) is the density of states for a fixed spin direction. The effective mass of the quasiparticle has been written simply as m. The importance in the physics of a Fermi system that all the states on the Fermi surface are degenerate should also be stressed. Let Tj
XJ.
—
V~^ *
/
t
j_
CVUi.Client "T" 7T"
\~^
/
7/
(u
uf\
' aR ct*R*'!•*•> •* /**
f t
7^ R^lh
m^lh^ n^Cl fc' /?/
c~) i H\
\^.L/l
20
Meanfield theory of pair condensation kfk
Fig. 2.1. be the Hamiltonian of the system. Here the matrix element V is given by Eq. (2.1) and, if fi denotes the chemical potential,
is the particle energy measured from the Fermi surface. One may put /a = kp/2m in an equilibrium state. Now let us show that where the interaction is negative, however small it may be, there exists a state whose energy is lower than that of the Fermi sphere ground state. As an example, consider a state with a spinsinglet pair with centre of mass momentum zero outside the Fermi sphere (Fig. 2.1),
W = E Qa^al^l^),
(2.18)
k>kF
where C^(k) = —C^(k) = Q. Let us consider an approximation in which the only role of the interaction is to scatter the pair (fcf, —k{) into another pair (kf\,—k f[\ both pairs being outside the Fermi sphere. Then this problem becomes analogous to the twoparticle problem studied in the previous section, except that the present pair is interacting in the presence of the background Fermi sphere and hence the fc'integration in (2.13) is over the range k! > kf. Let us take an swave (/ = 0) interaction of the form 8
0
(
"*>&{">0) (otherwise).
,2,9)
where it is assumed that coc
2.2 Cooper pairs and the BCS ground state
21
JV(O) / d£, one obtains an equation which determines the eigenvalue — JE,
1 = N(0)g r d £ — ^ —
= N(O)gIn  £  ,t, 2 Q ) c .
(2.20)
Note that there always exists a solution \E\ to this equation. Since the Fermi sphere ground state gives E = 0, the result above implies that the Fermi sphere state is unstable against the formation of the pair introduced above however small the attractive interaction may be and hence that the Fermi sphere state cannot be the true ground state. This fermion pair is called a Cooper pair. For N(0)g
(2.21)
The singular dependence of £ on g indicates that this result cannot be obtained by a perturbative expansion with respect to g. The wave function of a Cooper pair Q oc ( I E I + 2 ^ ) " 1 in the krepresentation corresponds to the real space wave function  + i
;
t K
,
<*,<*<«
(2.22)
where JC is the relative coordinate of the pair, r = JC, and kc is fixed by the relation ^ c ~ (kc — kp)vf = coc. The function ^(r) varies as r~l coskpr for small r and approaches zero faster than r~l for r ^ VF/\E\. Accordingly one can take the size of the pair to be roughly vp/\E\. Since a Cooper pair is formed above the Fermi sphere, the size of the pair is larger than that of a pair of the same binding energy in vacuum by a factor y/ep/\E\.
2.2.1 The BCS ground state When a Cooper pair exists due to an attractive interaction, it is expected that all the particles in the vicinity of the Fermi surface should form pairs of some kind to lower the total energy. To make our discussion simple, let us assume for the moment that the Cooper pair is a spin singlet as before. Then the pair wave function in the fcrepresentation is given by Cn(k,q) = Cu(k,q) = Q , CTT = C u = 0, see Eq. (2.9). It would be natural to expect that the particles all form identical pairs with the largest binding energy to minimise the system energy, just like the BoseEinstein condensation in a Bose system. It should be noted in particular that the centre of mass momentum q must be the same for all the pairs, to take advantage of the attractive matrix
22
Meanfield theory of pair condensation
elements. Let us take q = 0 here. Then the ground state is given by xiV/2
where N is the total number of particles. Written in the coordinate representation, this becomes a product of twobody wave functions:
where s/ is the antisymmetrisation operator and sy denotes that the pair ij is in the spinsinglet state. Equation (2.23) being a product of N/2 pairs of a\^a_k^ the wave function is a superposition of a state with a pair and a state without a pair, for any particular k. Accordingly, *F#) can also be written as
where PN is the projection operator onto the states with N particles. Let us normalise the wave function as
(uk + i ^ I A  ) 10) = ^ivl^o).
\VN) =PNU
(2.24)
k
Here the coefficients uk and Vk are given by 2
(
)"1/2.
(2.25)
The condition that the total particle number be N is not imposed on For this wave function one has k,a
k
\vk\2 (l  N 2 ) = 0(N). k
Therefore *Fo) may be employed instead of *F#) for large N provided that N = N is satisfied. This approximate ground state *Fo) was first introduced in the BCS theory. We note en passant that ^o) becomes the Fermi sphere I^V) if one puts vk = 1, (k < kp) and Vk = 0 , (k > kp). We will see in the next section that, in a superconducting state, \vk\ takes a value between 0 and 1 in the vicinity of the Fermi surface, where the attractive interaction is at work. The expectation values (^ol^Zci^/ctl^o) and (¥oflLaLju l*Fo) do not vanish
2.3 The meanfield theory of pair condensation
23
in the state *Fo). Therefore, as remarked in Section 1.3, the state *Fo) violates symmetry under gauge transformations. It will become clear in the following discussions that *Fo) is much simpler than *Fjy) and, moreover, manifestly shows essential features of superconductivity. It should be kept in mind that *Fo) is not the exact ground state but a variational wave function, so to speak, in which the parameters Uk and Vk are fixed such that the expectation value E = (^FQI^I^O) of the Hamiltonian (2.17) takes an extremum.
2.3 The meanfield theory of pair condensation Although the BCS theory has started with the ground state l^o), it is a meanfield theory based on the assumption that the expectation value of the pair is finite and hence is most clearly explained from that point of view. Here we discuss, for later convenience, the most general pairing state at finite temperatures. Thus, instead of the above expectation values, the statistical averages ^ajff(*) = {akaakp)
(2.26) are assumed finite. These averages are called the pair amplitudes. Fermi statistics imposes a condition, similar to Eq. (2.7), ¥/?«(*) = V*p(k)
(2.27)
on the pair amplitude. The meanfield approximation amounts to keeping only the interaction terms which induce the transition between as considered in the Hamiltonian (2.17). The ^summation may be dropped since all the pairs are assumed to have vanishing centre of mass momentum. In the meanfield approximation, one rewrites the interaction as
\
0
and drops the second term in the square brackets assuming that the fluctuations of aa and a W from the mean values are small. Let us introduce the mean fields
(2.28)
24
Meanfield theory of pair condensation
associated with the pair amplitudes (2.26). It follows from Eq. (2.2) that the mean field A satisfies relations similar to Eq. (2.27), Aap(k) = APa(k).
(2.29)
Now the meanfield Hamiltonian Jf m f is given by
Yl £ka4aaka + 2 k,oc
l l
l
}
(2.30)
The mean fields create or annihilate particle pairs. In the meanfield theory, the statistical averages such as (2.26) are obtained in terms of Jf mf as 1 Z = Tr ( e " ^ m f ) .
(2.31)
2.4 Representation of the mean field A^ Before we diagonalise Eq. (2.30), let us look at the representation of the pair amplitudes and the mean field Ak. The pair spin state is classified into either a spinsinglet state or a spintriplet state, as with twoparticle bound state considered in Section 2.1. Let us see how the pair amplitude (2.26) transforms under spinspace rotations. For a spin 1/2 particle, the unitary matrix which rotates the spin state by an infinitesimal angle 39 around an axis specified by a unit vector n is R = 1 + ld9n  a.
(2.32)
Here a = (ou<J2,o?>) are the Pauli matrices,
*i = ( i o j '
a2
=[i
0y
G
" = {O  i j 
(133)
The amplitude Y ^ transforms as ^ap
=
RayRp^yrj
= Rxy^\r\ Ryj p
under this rotation. Since —02002 = <xT, one finds that '
l
{a'V 
X
¥O 1GO2)
((7^02  ^(72(7) (72. 1
(2.34)
The symbols T and /? = 1/k^T will be used to denote the absolute temperature and its inverse, respectively.
2.4 Representation of the mean field A^
25
Accordingly, one finds a spinsinglet representation V F^, which is invariant under spinspace rotations, and a spintriplet representation x¥^\ which transforms as a vector: = A(k)i
(2.35) (2.36)
If the latter equation is substituted into Eq. (2.34), one obtains *¥' = (A + 5dnxA)'(ioo2) and hence finds that A transforms as a vector under rotations. The ^dependence of A (A) represents the orbital state of the singlet (triplet) pair. From antisymmetry (2.27), these quantities must satisfy (singlet state) A(k) = A(k) (triplet state) A(k) = A(k).
( [
, }
Therefore the most general form of the pair amplitude takes the form xp = y d ) + ^(3)
=
t M + ^ y A3A
A3 +A \ A\ +iA2 J
It is also possible to obtain similar representations for the mean field A(k). Provided that the interaction is of the form (2.4), the singlet mean field is A(k) = A(k)i
A(Jfc) = J2 v(Q)(k> V)Mk!)
(2.39)
k'
while the triplet mean field is A(k) = A(k)  ia<j2
\(k) = J2 V(°\k,kf)A{kr).
(2.40)
The vector A{k) is also called a d vector and, like the vector A, transforms as a vector under spinspace rotations. It can be shown easily that A U = A* • A + i(A* x A) • a.
(2.41)
Accordingly, if the spin quantisation axis is rotated so that A* x A  z, the above equation is diagonahsed and the eigenvalues are easily found to be A* • A+1 A* x A. A pair with A* x A = 0 (^ 0) is called a unitary (nonunitary) pair. The fields A(k) and A(k) are complex numbers in general and their kdependence represents the orbital state of the pair. The orbital state is
26
Meanfield theory of pair condensation
classified according to the partial wave analysis introduced in Section 2.1. Examples will be analysed in detail in the following chapters. The kind of pairs which appear in a given system depends on which state minimises the free energy of the system. Coexistence of the singlet pairing and the triplet pairing is not usually considered since in general this raises the free energy. There is, however, no a priori reason to exclude this possibility. 2.5 Bogoliubov transformation The meanfield Hamiltonian Jf mf of the previous section is quadratic in a and cfl and hence may be diagonalised by the Bogoliubov transformation
}
(2'42)
The new operators y and y^ are required to satisfy the anticommutation relations for fermions. This condition is satisfied if one takes
u[ = uk, vl = vk uku\ + vkvl = 1, ukvk  vkuk = 0.
(2.43)
Here uk and vk are 2 x 2 matrices whose components are Ukap and v^p, respectively. One may always impose the Hermiticity condition u\ = uk
(2.44)
on the matrix u without loss of generality in the cases under consideration. If one writes J>fmf in terms of y and y^ defined by the Bogoliubov transformation
ak =
ukyk+vky\
ah = u[yk  v£yl that satisfies Eqs. (2.43) and (2.44), and requires that terms yy and y"^ do not appear in JfW, one obtains the condition Uk€kVk + vk\kuk
 ukAkuk + vkk\vk = 0.
(2.45)
Here Ak denotes the matrix {Aap(k)} and (2.46) If Eq. (2.45) is satisfied, the Hamiltonian Jf mf becomes (2.47)
2.5 Bogoliubov transformation
27
fife = uklkuk  vk\kv\ + ukAkv\ + vkk\uk
(2.48)
where
and
\E {
&
\\
AJ}
(2.49)
denotes the pair condensation energy. (In the above equation, tr denotes the trace over the spin indices.) The matrix sk is Hermitian and hence can be considered as a diagonal matrix. Accordingly, it describes the excitation energy of the quasiparticles described by y and y^. The ground state of the Hamiltonian is the Fock vacuum of these quasiparticles. Henceforward, the term quasiparticles implies these excitations in a superconducting state, unless otherwise stated. Let us write down the solution of the above problem. General pairings being rather complicated, let us assume that the normal state electron energy is independent of the spin (^ka = &) and A is unitary, that is, either the pair A 4 A
A
is singlet or AkAk = A£At • 1. If one employs an Ansatz ukap = Ukdap/Dk9
vkap =
the condition (2.45) becomes 2£kuk—ul+\A k\2 From this and Eq. (2.48) one obtains
+Akap/Dk
= 0, where \Ak\2 = ^tr
(2.50)
After some algebra, one finally obtains the Bogoliubov transformation matrices L
?
1
/1
1, i>fc =  7 = W l
J2 V
&
Afc • 7T—.
(2.51)
£k A fc 
Therefore, J f mf is diagonalised by a transformation of the above form for a spinsinglet pairing as well as a spintriplet pairing provided it is unitary. (See [E9] for diagonalisation in general cases.) The final step in the meanfield approximation is to find the pair amplitude ^F/c and hence the mean field Ak. The statistical average (2.26) for the pair amplitude is easily obtained from J»f mf of the form (2.47) and the fact that y and y^ satisfy the Fermionic anticommutation relations. If the result is
28
Meanfield theory of pair condensation
substituted into Eq. (2.28), one obtains
—Vk'dy'Uk'y'P'fdZk'y 1)} •
(2.52)
Here
f(x) = (J* + l)" 1 = \ (l  tanh ?f)
(2.53)
is the Fermi distribution function. Equation (2.52) gives the mean field A^ in a selfconsistent manner and is often called the gap equation. Before we close this section, let us write down the free energy. This is given by F(T9 V,n) =  r
1
inTr ( e " ^ ) =  j T 1 E
l n
(l + e" fe «) + Jf c.
(2.54)
The symbol Tr stands for the trace over all possible states of the system. If Eqs. (2.50) and (2.51) are applicable, Eq. (2.54) becomes In (l + e" f e a )  E (£ka  &« + tvA^k)
.
(2.55)
Let us note that the gap equation (2.52) is equivalent to the condition that A/c minimises the free energy, namely •^7=0.
(2.56)
The matrix elements of A/c and A^ are assumed to be independent when the above variation is taken. The free energy F may be rewritten as F=
ETS (2.57)
where / = /(fifca) S is the entropy of thermally excited quasiparticles and E is the internal energy, the first term of which is the quasiparticle excitation energy while the second term is the condensation energy. When the interaction is of the form (2.4) and hence conserves the total spin, Eq. (2.52) (for unitary states) takes the same form, ]
(2.58)
2.5 Bogoliubov transformation
1
0
M I
v
1
/
\
29
0
1
/ (a)
\/ /
(b)
Fig. 2.2. (a) An example of V(/i) which leads to swave pairing, (b) An example of V(fi) which leads to pwave (solid line) or dwave (broken line) pairing.
for both spinsinglet pairing and spintriplet pairing. This can be easily shown when Eqs. (2.50) and (2.51) are applicable. The gap Akap takes a nonvanishing value at the critical temperature T c. Tc is obtained by putting fy = & in Eq. (2.58). When the interaction is of the form (2.12) and, furthermore, V\ is regarded as constant in the vicinity of the Fermi surface, that is Vi =
constant 0
(2.59)
then the integration over the direction of kf may be carried out. Finally one obtains the following equation for each /, which determines the critical temperature Tc = 1//CBJ?C> = N(0)Vt
(2.60)
/
Jo Therefore, in this simplified model, the equation which determines Tc takes the same form irrespective of the type of pair formation. Therefore it is expected that condensation takes place in the /channel which has the largest attractive \Vi\ and hence has the highest T c. Since the gap equation (2.58) is nonlinear in A ^ at T < Tc, in general, there may appear several components with different /. However, in practice, the proportion of components other than the dominant one is small. To find the values of V\ and, in particular, which V\ is negative and most attractive, one has to know the effective interaction between particles. This is generally a difficult problem. Just as an example, suppose the interaction V takes the form
V(n) = Vo
5V2P2(fi)
30
Meanfield theory of pair condensation
on the Fermi surface. Here \k\ ~ \k'\ ~ kp and \i — k k . If the interaction is attributed to phonon exchanges or spin fluctuation exchanges, its wave number is q = kf — k and \i becomes \i = kk = 1 — (q2/2k^\ see Fig. 2.1. Figure 2.2 shows V(/i) for the cases (a) V\ = V2 = 1 and (b) V\ =  1 , V2 = 1 (solid line) and V\ = 1, V2 = —1 (broken line), with an arbitrary VQ. They lead to condensation with swave, pwave and dwave pairs, respectively.
3 BCS theory
Basic properties of a superconducting state according to the socalled BCS theory will be discussed in the present chapter. According to this theory, an attractive force between electrons in the vicinity of the Fermi surface leads to superconductivity with spinsinglet swave pairing. Our discussion here serves as a basis for the generalisations presented in the following chapters. 3.1 Spinsinglet pairing and the energy gap
The interaction in an ordinary superconductor is thought to be attractive down to the average distance between conduction electrons, see Chapter 4. If this is the case, the amplitude independent of the angle, the swave (/=0) amplitude, is the most important in Eq. (2.12). Therefore, as mentioned in Section 2.2, ordinary superconductivity is caused by the spinsinglet swave pairings. In this case, the mean field A^ takes the form (2.39), namely A
(3J)
o)
and Afc = A_^ is in general a complex number. The Bogoliubov transformation
for the above A^ is already given in Eq. (2.51) as Uk =
—7=
/ 1 i ^ 1 H
i
? 1,
11 V>k =
—7=
^ 1
»
^ 7^~T
a
a\ W~3)
V2V skj 72 V skj Afc As was mentioned in Section 2.2, the BCS theory assumes that there is an 31
32
BCS theory
attractive swave interaction of constant amplitude between electrons near the Fermi surface. That is, it is assumed, as in Eq. (2.59), that l ( m ' > l & ' ' & l ) (3.4) 0 (otherwise) where g is a positive constant and coc is of the order of the Debye frequency if the attractive force is mediated by phonons. For the above interaction, the gap takes a constant value A& = A for  ^  < coc and vanishes otherwise. The constant A is determined by the gap equation (2.58), which takes the form ^ . 2
(3.5)
Here ek is the excitation energy of quasiparticles, ek = y/% + Ap.
(3.6)
Let us consider an excitation on the ground state, that is, the quasiparticle vacuum, to simplify our arguments. The inverse of the Bogoliubov transformation tells us that we need to add an electron to the system or subtract an electron from the system to excite a single quasiparticle. Accordingly, one has to excite a quasiparticle pair if the process is to keep the electron number of the system fixed. Therefore, at least 2Ao of energy is necessary for the excitation to take place, Ao being A at T = 0. In other words, the excitation spectrum has a gap. A pair must be broken to create an excitation in the ground state, where all the electrons are paired to form the condensate. Hence at least the binding energy of the pair is required. At finite temperatures, there already exists a gas of thermally excited quasiparticles and the scattering process of the quasiparticles must also be considered. Quasiparticle creation in this case is the same as that for T = 0, except that there are particles which do not form pairs and hence the mean field is suppressed and the gap A(T) becomes less than Ao. A quasiparticle is specified by the momentum k and the spin a. The density of states of quasiparticles with spin a in the vicinity of the Fermi surface is given by
 M) ~ N(0)J f = JV(O) . ^
N 2
A
2
9(\co\  A).
(3.7)
According to the above equation, the states within the gap are pushed outside
3.1 Spinsinglet pairing and the energy gap
 3  2  1 0 1 2 3
33
co/A
Fig. 3.1. The density of states @(co) in a superconducting state.
the gap as in Fig. 3.1 and the density of states diverges as l/Jco2 — A2 as co —• +A. It will be shown later that the density of states appears in various physical properties of superconductors. It should be noted that Eq. (3.7) is correct only for an isotropic Fermi surface and that @(co) deviates from this equation in an actual metal since the modulus of A varies on the Fermi surface. Note also that the group velocity of the quasiparticle excitation is vg(k) = Vksk = (k/m)(£k/ek).
3.1.1 Energy gap The factor A on both sides of Eq. (3.5) has been retained to show that there always exists a solution A = 0, but it will be dropped hereafter. Since OJC
(3.8)
1 = N(0)g /
Jo
Let us first consider the limit /? = oo, that is, T = 0 and hence find the gap Ao in the ground state. (The absolute value symbol for A will be dropped hereafter.) When coc > Ao, it takes a form identical to Eq. (2.21), that is, (3.9)
= 2co c exp[1/N(0)g].
Next let us consider the critical temperature Tc at which the nonvanishing solution A appears for the first time as the system is cooled down. For calculational convenience, Eq. (3.8) is rewritten using the formula 1
Y
— tanh =
2*
2
> f£^00
z
,.,,
1
2 2
~
{In + l) n + x
(3.10) 2
34
BCS theory
as 1 = 2N(0)gp~
Y
.
2 + Ap
tan" 1
.
c
(3.11)
where co^ = (2n + l)^/?" 1 . Since the gap A vanishes at T = Tc = l//? c , one has an equation that determines /? c: 1 = 4iV(0)g V
7 ^
tan"1 ,/ c < °° (2 + l)
Since /Jccoc > 1, the summation in the right hand side may be approximated by j J2n
(3.12)
where \p(z) is the di Gamma function and use has been made of the formula
m=l
the asymptotic form and the value From these expressions one finally obtains the BCS expression for the critical temperature /cBTc = 1.13a>cexp [l/AT(O)g],
(3.13)
where the numerical value 2ey /n ~ 1.13 has been used. From this expression and Eq. (3.9) one obtains the ratio = 3.53.
(3.14)
It is expected physically that /CB TC is of the order of the pairbreaking energy. The ratio 3.53 is a 'universal' value independent of Tc and other variables. It should be noted, however, that this value is obtained within the socalled weak coupling approximation in the BCS theory. As is shown in Table 3.1, the actual value for ordinary superconducting metals with low Tc is close to this weak coupling value but for metals with higher Tc, this ratio clearly deviates from 3.53. This deviation from the BCS value will be an important point in the following chapters.
3.1 Spinsinglet pairing and the energy gap
35
Table 3.1. Observed values O/2AO//CBT C and AC/C n AC/C n BCS Al Cd Sn Hg Pb Nb
3.53 3.53 3.44 3.61 3.65 3.95 3.65
1.18 0.52 3.72 4.15 7.20 9.25
0
0.2
0.4 0.6 T/Tc
1.43 1.45 1.32 1.60 2.37 2.71 1.87
0.8
1.0
Fig. 3.2. The temperature dependence of the energy gap of Pb. The symbol o denotes values obtained by the tunnelling experiment. The solid line is the prediction of the BCS theory. Figure 3.2 shows the temperature dependence of the energy gap, from which one finds that the meanfield theory reproduces the data very well. At low temperatures T
2TT
1/2
Wo
(3.15)
The behaviour of A(T) in the vicinity of Tc will be given in the next section.
3.1.2 Coherence length The energy scale which characterises a superconducting state is A. The corresponding characteristic length (3.16)
36
BCS theory
called the coherence length, is important in the analysis of superconducting phenomena. Let us write the coherence length at T = 0 as £o. The pair wave function (2.26) of the condensate is ^ = —u^Vk, which is given, in real space, by x f
^(JC) = ^/ i k
exp(i& ' x) = ^2~
1/
I j2
IAI2 V / 2e x 7~2 )
P ( i ^ * *)•
This is a similar form to the Cooper pair wave function considered in Section 2.2 and shows that the coherence length £ represents the spatial extension of a pair. The length £o is of the order of 10~4 cm in an ordinary superconducting metal, which is much larger than the distance between electrons. Accordingly many pairs overlap one another. 3.1.3 Charge density The charge density en is obtained with the help of the Bogoliubov transformation (3.2) as
Qs = 2]T \Vk\\ Q*=2J2 (\uk\2  N 2 ) /(<*). k
(3.17)
k
The first term Qs may be thought of as the contribution of the condensate i.e., the pairs and is given by the number of states n = kp/37r2 with & < 0. The second term Q* is the contribution of the quasiparticle excitations and vanishes for an equilibrium Fermi distribution with particlehole symmetry. If, on the other hand, the system is out of equilibrium and particle excitations (above the Fermi level) and hole excitations (below the Fermi level) obey different distributions, the second term fails to vanish. One may consider, in this case, that a quasiparticle with a momentum k has a charge q k = e (\uk\2 — \vk\2) = e^k/sk It should be noted that by calculating d J2k \vk\2/dji, one finds that Qs changes by SQS = 2eN(0)dfi under an infinitesimal change Sfi of the chemical potential. 3.2 Thermodynamic properties
The thermodynamic properties of a superconductor are derived from the free energy (2.55). Before we do this, however, let us consider the thermodynamic relations relevant to a superconductor in a perfectly diamagnetic state. Consider a long cylinder made of a superconductor and suppose that a
3.2 Thermodynamic properties
37
uniform external magnetic field of strength H is applied parallel to the axis of the cylinder. The magnetic flux density B is also uniform and parallel to the axis of the cylinder. Let us denote the superconducting state and the normal state by the indices s and n respectively, and the free energy and entropy per unit volume by F and S respectively. One has dF = SdT + (l/4n)H • dB since the work required to change the flux density from B to B + dB is (l/4n)H • dB per unit volume. If H is taken to be an independent variable, one should use the free energy G(T,H) = F(T,B) — B • H/4n, instead of F(T,B) (the other variables are omitted). One therefore obtains l rH G(T,H)  G(T,0) =  — / B(H) 4TT JO
• dH\
(3.18)
In the normal state, one may put B = H since the magnetic susceptibility of an ordinary metal is of the order of 10~7 ~ 10~6 emu. One may also take B = 0 in the superconducting state if perfect diamagnetism is assumed. Then one has (3.19)
Let us focus on type 1 superconductors here. (Type 2 superconductors will be studied in Chapter 5.) Since a superconductor becomes normal when the external magnetic field reaches H = HC(T), one has Gs = Gn at that field and hence one finds G s (T,0)  G n (T,0) =  H C 2 ( T ) / 8 T T . This therefore implies that the free energy difference at H = 0 is found by measurement of the critical field. The free energy difference under a magnetic field H is obtained from the above relation and Eq. (3.19) as GS(T,H)  Gn(T,H) = ^{H2H2Q{T)\
(3.20)
from which the entropy difference is found to be
This is negative as it should be. One finds the specific heat jump at Tc by differentiating the above equation with respect to T and using the identity
AC = (Cs  C n ) T = T c =
^
(dHA \dTjTc
(3.21)
38
BCS theory
3.2.1 The free energy according to the BCS theory Let us consider the free energy of the BCS model of the previous section. One has to calculate the difference of the free energy of the superconducting state (A ^ 0) and of the normal state (A = 0), supposing that it should exist. We are interested in this difference because the free energy Fs contains the contribution from the interior of the Fermi sphere, for which  ^  is large, and hence the free energy per particle is a large quantity of the order of £FAccordingly the evaluation of Fs would require the quantitative theory of the normal state of a metal. However the difference of Fs and Fn may be discussed within the present model. Equation (2.55) is given in the present case by
E {
l
ln
[} + e ~ fe ) +*ktk + A ^ }
(3.22)
and one obtains, in the BCS model, k
k POO
1
= ^(OJjB" 1 / d£ ln Jo 1 (3.23) 2N(0) / d£(s  £) + A 2 /g. Jo The amplitude A(T) will be simply written as A in the remainder of this section. If Eq. (3.9) is used, one obtains Fn
ln((l1 + < = —jS~ 14JV(0) jt jT I d£ d£ ln 1
(3.24)
1. T
which is the modified Bessel function Ki(f}A) for j8A > 1. If the asymptotic form of K\ is employed and the second term is evaluated within the lowest order in 1 — (A/Ao), Eq. (3.24) becomes Fs  Fn(T = 0) ~ ^ 2 iV(0)(/T) +yiV(0)(/c B T) .
/
^
A
(3.25)
3.2 Thermo dynamic properties
39
The third term is the contribution from the normal state, from which one obtains the electronic specific heat of the normal state, nN(0)klT.
(3.26)
The coefficient of T on the right hand side is commonly called the Sommerfeld constant and denoted by y. From the second term of Eq. (3.25), the specific heat of the superconducting state can be found:
This specific heat is exponentially small at low temperatures due to the energy gap. From Eqs. (3.20), (3.25) and (3.14), one obtains tfc2(0)/8;i = iV(0)A2/2 (3.28)
It is physically understandable that the condensation energy at T = 0 is of the order of the product of the number of pairs JV(O)Ao/2 and the pair binding energy Ao. We note that the temperature dependence of the critical magnetic field (3.28) is valid over quite a wide temperature range. 2. T <; T c : Let us next consider the temperatures in the vicinity of T c. We will use the results obtained here when we discuss the GinzburgLandau theory later. Since A(T)//c B T c < 1 near T = Tc, the free energy may be expanded in powers of A. Let us recall that A^ is a complex number and hence A& and A£ are independent quantities. For this reason it is easier to compute
by differentiating Eq. (3.22) rather than by evaluating directly F sn Fs — Fn. Hence one finds in the BCS model
Jo
C
40
BCS theory
where conc = (2n + l)n/f}c. Equation (3.11) has been used to obtain the second expression. The first term of the second expression is readily evaluated if one notes that (1 — T/Tc) < 1. The second term is also obtained easily if
a = N(O)(lT/Tc),
b=
where C(3) = Z ^ i n~3 As was noted at the end of Section 2.4, the equilibrium value of the gap A is determined so as to minimise F sn and hence one finds 9
2
a
8TT 2
A =  = —— (/c
9
/
T\
2 BTc) (1  — j .
(3.31)
By making use of the above result, the equilibrum free energy is found to be
(3.32)
It should be noted that Fsn is proportional to (1 — T/Tc)2. It then follows from this result that the jump in the specific heat at Tc is given by AC/Cn = 12/7C(3) = 1.43.
(3.33)
This value is universal in the BCS model. The comparison between the universal number and the measured value is made in Table 3.1. The temperature dependence of Cs in the vicinity of Tc comes from the next order term in the expansion and hence is proportional to T/Tc — 1. Figure 3.3 shows the variation in the specific heat of aluminium, and shows an excellent agreement between experiment and BCS theory.
3.2.2 States carrying supercurrent Pair condensation takes place with the centre of mass momentum q ^ 0 in a state with a superconducting current. Therefore the thermodynamic average ^^(k.q) = (dk+(Xak_p) becomes finite, where k+ = k + q/2. This
41
3.2 Thermodynamic properties
Fig. 3.3. The temperature dependence of the specific heat of aluminium. The specific heat of the normal state is observed to be proportional to T under a magnetic field of 300 G. (From [G5].)
state is an equilibrium state with the specified total momentum. Therefore it is still a thermodynamic state. The real space order parameter in this case, ¥(*) = E/c e i ( *+*)•*(a M a M ), has a phase factor e**"*. Noting that \q\ < fcF, one finds that the electron energies taking part in the pair formation are
(3.34)
Theories developed in Chapter 2 are generalised easily in the present case and one obtains the following results, in which the coefficients of the Bogoliubov transformation (3.35)
are \Ak\'
Formally they take the same form as the case with q = 0. It should be noted,
42
BCS theory
however, that the excitation energies are modified to ^ + k'
(3.36)
ek_i = Skk q/2m. These results are in agreement with those obtained from the Galilei transformation of a system with elementary excitations provided that vs is set equal to q/m in Eq. (1.18). Furthermore the free energy (3.22) is replaced by
l
ln
[1 + exp(j8e*+s)] + efc  & + A ^ } .
(3.37)
k
Let us consider the electrical current density first. Since a uniform electrical current is represented by an operator k,<x
one needs to evaluate the expectation value of this operator in a superconducting state:
isE 171
k
+ §) «T«M> + (* + § {
^
b
k
I
b
k
(3.38) where use has been made of the Bogoliubov transformation (3.35). Some of the spin indices are suppressed for simplicity. To obtain the density ns(T) of the superfluid component, let us keep only terms that are proportional to q. Since only the excitations near the Fermi surface contribute to the current, one may put \k\ ^ fep in the above equation. If ? ^ ( 1 — &/I&D/2 = nq/2 is subtracted from the second term, contributions from the two sides of the Fermi surface (±£) cancel out in this term. Thus one finds Js — neg/2m
1 =—
3m
8sk
q Jo
?lM, ds
,3.39,
where n = 2N(0)k^/3m is the number density. Finally one obtains
n>M). Note that the second term of ns(T) is always negative.
(3.40)
3.2 Thermo dynamic properties
43
Let us consider the case T = 0 first, for which ns(T) = n. That is, all the particles form pairs with vs = q/m and contribute to the supercurrent. For T < Tc, ns becomes n(l — T/Tc) and, of course, vanishes at T = Tc. The difference n — ns(T) is of course the normal fluid component made of thermally excited quasiparticles obeying Fermi statistics. The effect of the centre of mass motion of pairs appears in the gap equation through the distribution function of the excitations. Let us find a term proportional to # 2 A 2 , which adds to the free energy Fsn near Tc. The function for 2/(efe) in Eq. (3.29) should be replaced by f(sk+kq/2ni)+f(£kkq/2rn) 2 1 q ^ 0. Then it follows that the term proportional to q in (dFsn/dA*)A~ is
One may put 8%. = £% at T ~ Tc. After carrying out the ^integration and the ^summation, one obtains
One has to add the above term to the free energy F sn of Eq. (3.30) when q =fc 0. If one substitutes A2 of Eq. (3.31) into the above equation, one finds, from Eq. (3.40), that the coefficient of (q2 /Am) is exactly a half of ns(T), that is, the number of pairs. Problems related to states with superconducting current, such as the critical current in a thin film, will be treated in Chapter 5.
3.2.3 Spin paramagnetism Let us consider the paramagnetism associated with the electron spin, also known as the Pauli paramagnetism. Suppose the system under consideration is a superconductor under a uniform external magnetic field H. Then due to the Meissner effect, the magnetic susceptibility for a uniform B (^ H) is obtained only for a small particle or a thin film whose thickness is less than the penetration depth, or for a type 2 superconductor near HC2. Note also that only spins couple to a magnetic field in a liquid 3 He as we will see in Chapter 6. Let /LLO be the magnetic moment of an electron. Then the electron energies taking part in the pairing are
This is equivalent to simply replacing k • q/2m by ^H in Eq. (3.34) obtained for q 7^= 0. Accordingly the excitation energies are modified as
44
BCS theory
£k + (—)noH. For example the gap equation is now given by
)}.
,3.42,
Let us consider the case of a weak magnetic field pi^H < A, which is analogous to the case of small q. The magnetisation of the system is obtained as M = —dF s/dH from the free energy Fs of Eq. (3.19). In obtaining this, one needs to differentiate the explicit Hdependence of Fs since, although A depends on H, the equality dFs/dA = 0 holds in an equilibrium state. Thus one has M
= «> E (/(* + VoH)  f(sk k
The magnetisation is then given by
If compared with Eq. (3.40), one finds that it is thermally excited quasiparticles that polarise under a magnetic field. It also follows that
{
(T
7C(3) ,2 , 2 Tc). field H, for which It can be easily shown from Eq.^(3.42) that the magnetic A vanishes at T = 0, satisfies fioH/Ao = 1/2. At low temperatures, however, the phase transition between the normal state and the superconducting state is of the first order and it takes place at the Clogston limit H?, also known as the Pauli limit, defined by /iotfp/Ao = 1/V2.
(3.44)
There are some type 2 superconductors whose HC2 obtained in Section 5.3 is larger than ifp. If this is the case, the upper critical field is replaced by ifp. 3.3 Response of a superconducting state to an external field Suppose the system is interacting with a timedependent external field Ft(x, t), which introduces an extra term
= JdxCi(x)Fi(x9t)
(3.45)
in the Hamiltonian Jf. F may be an electromagnetic field or an ultrasound wave and can be treated classically in many cases. The subscript i denotes
3.3 Response of a superconducting state to an external
field
45
the ith component where F is a vector. This index will be dropped where this does not cause confusion. Suppose the interaction is adiabatically applied to a system which is in equilibrium at t = — oo. This may cause a variation proportional to F in an observable Q(x) of the system, which is known as a linear response. This variation is given by the wellknown Kubo formula as
dx'dtf([Q(x,0,Qtf,0])Ft(x\tr).
6Q(x,t) =  i / f J
(3.46)
J— 00
Here operators such as Q(x, t) are in the Heisenberg representation whose time evolution is generated by Jf — ptN, where \x is the chemical potential and N is the total particle number of the system. The operator Q may be the number density n(x, t), the current density j(x, t) and so forth. Define the retarded correlation function
KQC(x x',t
0 = i( [Q(x, t), Qtf, 0 ] )0(t  0
(3.47)
for a spatially uniform system. Corresponding to the Fourier decomposition of the external field
F(x, t) = ^2 F(4> °>)exp(i# • x  icot), q,co
Eqs. (3.46) and (3.47) are decomposed as
SQ(q, co) = KQC(q, co)F{q, co), KQC(q, co) =  ^
uidE
+£
Here Z is the partition function, 5 is an infinitesimal constant related to the adiabatic switching of the field, and \n) is an energy eigenstate with energy En, which is, in the mean field approximation, given by the quasiparticle excitations. In order to find decay or relaxation of the external field due to the interaction with the system, it is necessary to evaluate the time variation of the total energy of the system (3.49) and to average it over one period of the external field. Note that only the explicit time dependence of the external field is to be considered in the derivative
46
BCS theory
The most important cases are those in which C(x) and Q(x) are the same density such as n(x) or j(x). Let the Fourier transform of the density be
Cj(^q)al_Qiak+a.
(3.50)
k,OL
The density C is assumed to be spin independent, although generalisation to a spindependent case is straightforward. To evaluate the matrix elements in Eq. (3.48), Cj(q) must be expressed in terms of y^ and y of the Bogoliubov transformation (3.2). (The centre of mass momentum of the pairs, namely q in the previous section, is assumed to be zero. The vector q here denotes the wave vector of the external field.) One finds
Luk+ + v*k+vk_)yl_ayk+a + (v*k_vk+ + v*k+vk_)5q0 ± u*k+vk_)yl_y_k+i
+ (v*k_uk+ ± v*k+uk_)yk_i (3.51)
The signs are chosen according to the parity Ci(—k,q) = +Ct(k,q)
(3.52)
under k > —k. The coefficients of y^y,y^y\yy in Eq. (3.51) are called coherence factors and produce effects characteristic of a superconducting state with a pair formation. Finally one obtains q,co) = — ^2 Ci(k> 9)Cj(k9 q) k \rs\/ * 7 * M2 J\^k+) ]\fik) x \2\{uk_uk++ vk vk_)\ jj— CU  Id + 6fc+  £fe_ L
+ l("LU/c+ ± 4+Vk_)\2[l  f(£k+)  f(sk_)] .,( ' !____ I (»  i5  8/c +  8/c_
o;  id + 8/c+ + sk_
(3.53) where use has been made of the relation C*(q) = Ct(—q), which follows since C(x) is real. The first term represents processes in which thermally excited quasiparticles are scattered by the external field while the second term corresponds to quasiparticle pair creations/annihilations due to the
3.3 Response of a superconducting state to an external field
47
external field. The coherence factors are obtained, using Eq. (3.3), as u*k_uk+ + v*k+vk_\2 =
(sk_ek+
+ £k£k+ +  A  2 ) (3.54)
2
\u*k_vk+ ± u*k+vk_\\2 =
^k
&k
(ek_ek+  £k£k+ ± A 2 ).
Let us now consider some applications. 3.3.1 Ultrasound absorption The simplest application is to ultrasound absorption. This is because the wave number q is uniquely specified by the given frequency co, once the wave mode is chosen. This is in contrast with the electromagnetic field discussed later. Furthermore the sound velocity vs = co/q is much smaller than the Fermi velocity up. For the longitudinal wave considered in the following, the quantity C(x) in Eq. (3.45) is the particle density n(x) and one has C(k,q) = 1. Let (/>(0Q^q'x~a)^ be the potential for electrons due to the sound wave (a lattice wave of a long wavelength). It can be shown from Eq. (3.49) that the sound wave absorption is given by
Here K(q,co) is given by Eq. (3.53) with the substitution Q = 1. Since an ultrasound frequency is usually much smaller than A(T), only the first term of Eq. (3.53) contributes to the imaginary part and one obtains
ImKfo, a>) = 7c W l +
^
^
Note the appearance of the coherence factor. Let us make the change of variables
which is obtained by using £ + — £_ = k • qv? (note that qvj; > co = qvs) and £ = (^+ + £_)/2. Since co
d e l  ) 1  1 " / .
(3.56)
Note that the density of states and the coherence factor exactly cancel out and the integration simply gives a function /(A). In comparing theory
BCS theory
48 1.0
0
Sn 33.5 MHz
•
Sn 54.0 MHz
X
Sn 28.5 MHz
0.6
_ A
Sn 35.2 MHz
0.4

0.2

0.8
n
1
1 /
A
J" 1
0.2
0.4
0.6 TITc
1
0.8
1
1
1.0
Fig. 3.4. Ultrasound absorption. (From [G6].) with experiment, it turns out to be convenient to normalise the absorption coefficient relative to the normal state value as (3.57) Since v? >> ^s? sound absorption takes place when quasiparticles near the equator of the Fermi surface with momenta perpendicular to q are scattered by the sound wave. Therefore A(T) in Eq. (3.57) is the energy gap averaged over the equator. As is shown in Fig. 3.4, a s /a n directly measures the temperature dependence of the gap. It should be added that in the case of transverse waves the absorption suddenly becomes small as the temperature is reduced below Tc. This is due to the Meissner effect since, in the free electron model, the vector potential appears in the absorption coefficient. In reality, however, one must also take into account the finite electron mean free path / and electron band effect.
3.3.2 Response to electromagnetic field Let A(x, t) be the vector potential of an electromagnetic field. Here the gauge V • A = 0 is chosen for reasons which will become clear later. According to
3.3 Response of a superconducting state to an external
field
49
quantum mechanics, the electronic current density operator is 2 m
a ^
Vl e
C J
\
1
C J
2
_ ; ( x\
n(x)A(x t) (3 58) me Here the first term is called the paramagnetic current and the second term the diamagnetic current. The interaction Hamiltonian which is proportional to A is p
1
r
Let us compute the electronic current density itself as a response to the applied field. Since the second term in Eq. (3.58) is already proportional to A, one may replace n(x) by the mean particle density n. The first term
Mi) = E > L « M k a
is obtained by taking Q(k,q) = ekt/m in Eq. (3.53). Since general cases are complicated, let us concentrate on the case T = 0 here. The response in this case is given by
m2 me
1
+K(q9co)\Ai(q,co)
sk_sk+ \coid
 sk_ sk+
J
co  W + sk_ + sk+ J
(3.60)
Let us consider a static magnetic field, co = 0, first. It can be easily shown that K(q,co) ^ 0{(qv?/'Ao)2) provided that qv?
A
A.
me As was shown in Chapter 1, the Meissner effect can be derived if the above equation is solved simultaneously with the Maxwell equations. Note that if one takes A = 0 in Eq. (3.60), one obtains K = ne2/me, which exactly cancels the first term of (ji(q,co)). In a normal state, no current proportional to the vector potential A exists and, as in the Ohmic law, the lowest order contribution to the current response is from terms proportional to coA.
BCS theory
50
Fig. 3.5. The codependence of G\ for pure lead (•) and lead with a magnetic impurity Gd (•). See Section 4.6 for the AG theory. (From [G7].) Let us next consider the imaginary part of Eq. (3.60). In contrast to ultrasound absorption, electromagnetic wave absorption is quite complicated, since A(q, co) in a sample is obtained by simultaneously solving the Maxwell equations with Eq. (3.60). Accordingly when the incident wave has a finite frequency co, one generally has skin effect. In a superconductor there is also the Meissner effect. Hence the wave penetrates into the sample within a finite depth 8?. Therefore one has to calculate K(q,co) for \q\ ~ dp1. For a thin film with thickness d less than the coherence length (d < £ = I>F/A), however, the ^dependence is negligible, which makes the analysis easier. The imaginary part is obtained by putting Im(co — id — Sk_ — Sk+)~{ = nS(co — 8k_ — £k +) in Eq. (3.60). One may make the replacement (3.55) here as well since qv? > Ao ~ co. The result is the expression for the real part (also known as the resistive part) di(co) of the codependent electrical conductivity o\(co) +102(01) = —i(c/co)K(co). As in ultrasound attenuation, we are interested in the ratio normalised by the normal conductivity,
=i r co JA
— co) —
(3.61)
The value of ais/^in measured with a thin film of lead is in good agreement with this prediction based on the BCS theory. Observe, in particular, that absorption starts when co exceeds the energy gap, see Fig. 3.5. Analogous to the electrical conductivity, the thermal conductivity K is also an important transport coefficient. However, here we are content with the following comments. The contribution to the thermal conductivity in
3.3 Response of a superconducting state to an external
field
51
a normal metal is mainly from the conduction electrons and there exists the WiedemannFranz relation K = (n2/3)(/CB/e)2T'cr between the electrical conductivity o = 1/p and the thermal conductivity K. In a superconducting state, however, a is infinite while K becomes less than that in a normal state. This is because the current is carrie " >y the pair condensate while the entropy is carried by the gas of thermally oxcited quasiparticles only. At a low temperature T
4A
.
(3.62)
In the limit q —> 0, this is simply equivalent to shifting the phase of the pair by a constant amount and the energy remains the same as that of the ground state. It can be shown that the electrical current response against the longitudinal component of the vector potential vanishes if this excitation
52
BCS theory
is taken into account. (One has to use the WardTakahashi relation to construct a rigorous theory with gauge invariance, see [C3].) If the phase x of the pair varies spatially as q • x, there exists a uniform superflow as was shown in Section 3.2. If the phase % changes as eiqx, then the superflow is not uniform and hence there exist density fluctuations. Consequently this collective mode with finite q couples with density fluctuations. In an electron system this excitation becomes a plasma oscillation with a large frequency due to the Coulomb interaction. Accordingly this excitation does not directly influence such phenomena as superconductivity. Collective modes play very interesting roles in a superconductor or a superfluid with a pair condensate with nonvanishing angular momentum (/ ^ 0) that is, other than swave pairing, see Chapter 6.
3.3.3 Nuclear magnetic resonance The nucleus of many metals that show superconductivity has a spin. Let / denote the nuclear spin and m^ = y^I the associated magnetic moment. This moment precesses in a static magnetic field H. The resonance frequency shifts from &>o = 7 N # and, moreover, the precession decays due to interaction with the surroundings. In a metal, the moment interacts with the conduction electrons and information on the latter is obtained through nuclear magnetic resonance. The origin of the interaction is the coupling of the nuclear magnetic moment with the electron magnetic moments associated with the electron spin and the orbital angular momentum. We consider only the electron spins here to simplify the discussion. The magnetic field due to a magnetic moment #WN placed at the origin is given by 3x(x • m N )  x2/ffN , 8TT J \x\ Hence the interaction between #MN and a magnetic moment associated with the electron spin s is ^s/=A
fdxs(x)B(x) J
(3.63)
s(x) = ip*a(x)sapxpp(x).
Suppose the electrons belong to the sband and the probability tp(jc)2 is isotropic around the nucleus. Then only the (5function term contributes to the interaction. Therefore if J?, denotes the lattice points on which the nuclei
3.3 Response of a superconducting state to an external
field
53
sit, the interaction between an electron and a nucleus is given by / d s(x) • £ y^Iid(x  Rt).
(3.64)
Shift of the resonance frequency (Knight shift) Since coo is small compared to the electron spin frequency, the nuclear magnetic moment experiences an averaged electron spin. The spin part of the magnetisation of the electron system in an external magnetic field H is
where x is the magnetic susceptibility. Accordingly each spin is under an extra magnetic field (called the hyperfine field) of (87i/3)t/;(O) 2x// according to Eq. (3.64). Here ip(0) is the electron wave function at the position of the nuclei. Therefore the shift of the resonance frequency is given by K s
a n d is called t h e Knight quantitatively, the ratio
cocoo (Do
=
8* 3
2
shift. A l t h o u g h it is r a t h e r difficult t o fix tp(0) 2
may be compared with the theory. According to Eq. (3.43) the ratio Xs/Zn —• 0 as T —• 0. Figure 3.6 shows the Knight shifts for Al, Hg and Sn. The shift for Al is close to the theoretical curve while those for Sn and Hg do not vanish as T —• 0. This discrepancy is attributed to spinorbit scattering (S — L scattering). The samples consist of fine particles since microwaves are used in actual experiments, for which S — L scattering at the surface is not negligible. The electron spin is no longer a good quantum number in the presence of S — L scattering. Accordingly the pair cannot remain in the pure spinsinglet state. As a result, the Knight shift Xs generally remains finite as T —• 0. The Knight shift tends to vanish as T —• 0 for such metals as Al, for which the contribution from S — L scattering is small. There is an additional contribution /orb to the magnetisation due to the orbital motion of electrons. This may be separated from other contributions since it has minimal temperature dependence. Nuclear spin relaxation time T\ Let us calculate the transition probability with which each nuclear spin undergoes a transition from a state with energy COQ to that with vanishing
BCS theory
54 1
°o o o°o o
1.0 0.8 ; H g •Sn
> 0.6
0
(I)
y
* 0.4 0.2 0
y
c /

o
/ i
1
1
1
1
0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0
Fig. 3.6. The Knight shift of Al. The arrows in the figure depict the shifts for Hg and Sn in the limit T » 0. They do not fall to zero because of S — L scattering. (From [G8].)
energy, induced by spinelectron interaction (3.64), assuming that there are no correlations among motions of different nuclear spins. If one concentrates on a particular nuclear spin, the interaction between the spin and conduction electrons is given by Jdfi oc Ylk,q \al t a M ^ ~ ^ + h.c.j, where 1^ = Ix + \Iy. The second order perturbation in 2tf\ gives the transition probability V*k+Vk_\28(8k+ +CO
Sk_).
Kq
Quasiparticle pair creations are neglected in the above equation since the inequality a> < A holds as before. Note that the coherence factor in Eq. (3.51) is odd in this case and that there is ^summation since the scattering processes occur at a nuclear site. For an isotropic model, one has
r = 4/
ds
e + co 2
A
JA
+
 A2 s(s + co)
(3.66)
The contributions above and below the Fermi surface cancel in the term proportional to £+£_. If one puts A = 0 in the above equation, it reduces to
r
Jo
3.3 Response of a superconducting state to an external field
55
10.0
Fig. 3.7. The temperature dependence of T\ for 27A1. The solid line is the theoretical curve in which the anisotropy of the gap is taken into account. The dotted line denotes T\ for a normal state. (The dots • are taken from [G9], while o are from [G10].) If the proportionality constant is supplied, one obtains the Korringa equation
2 = (y W ) 7 N I V ( 0 )  N ( 0 ) )
nkBT
(3.67)
in the normal state. It should be noted that 7\ * is proportional to T as a result of the Fermi degeneracy. The coherence factor and the density of states, as well as the Fermi distribution functions, appear in Eq. (3.66). As a result, the integrand diverges logarithmically at the lower limit s = A for co ~ 0. Accordingly it is expected that Tf1 becomes very large below Tc. In actual metals, however, the electronphonon interaction, which is the origin of superconductivity, and also the density of states are not isotropic. As a result, the energy gap has an anisotropy of up to 10% on the Fermi surface. The logarithmic divergence is weakened once the gap is averaged over the Fermi surface. Taking this into account, the theoretical prediction agrees with experiment, see Fig. 3.7. It should be added that the strong coupling effect treated in Chapter 4 also tends to weaken the increase of T^ 1 . In any case, the increase of Tj" 1 just below Tc should be contrasted with the simple suppression of the ultrasound absorption coefficient a s. Equation (3.66) becomes exponentially small at low temperatures (A(T) ~ Ao) due to the factors containing the distribution function, which can be seen in Fig. 3.7. (See [El] for a review of nuclear magnetic resonance.)
BCS theory
56
insulator
^substrate
(a)
(b)
Fig. 3.8. Tunnelling junctions. 3.4 Tunnelling junction and Josephson effect
The tunnelling junction is one of the most powerful phenomena for the study of superconducting states. Firstly, it makes possible direct observation of the density of states associated with the energy gap. Similarly, the Josephson effect due to pair tunnelling reveals the role played by the phase of the order parameter, that is, symmetry breaking associated with superconductivity. Secondly, the tunnelling characteristic shows in detail how the electronphonon interaction leads to pair formation in ordinary superconductors. The latter will be studied in Chapter 4. Let us consider here the tunnelling effect in a superconductor within the BCS model. A typical tunnelling junction is made of two metals in contact through a thin insulator (an oxide film in many cases, one can even use a normal metal) as shown in Fig. 3.8. The contact may be a weak one such as a point contact made by a needle. Figure 3.8(b) is a model of a junction in which metals A and B couple through a tunnelling barrier. Let us denote the state of an electron in the side A (B) by k,a (/>,/?)• An electron transfer from one side to the other is possible since there is an overlap of electron wave functions inside the barrier. Let us introduce the tunnelling Hamiltonian kpalcp«
+ h.c,
(3.68)
k,p,<x
which couples A and B, to describe the effect. Here a/ca(cjPa) is an electron operator of the system A (B) and T^v is a matrix element which transfers an electron p,<x in B to an electron A:, a in A, which is assumed to be independent of the spin. The matrix element satisfies Tkp = T^_k due to the timereversal invariance. This is the requirement that the probability amplitude for the timereversed transfer be the same as before the timereversal. Processes accompanying phonons or those mediated by magnetic impurities are of course neglected in Hj of Eq. (3.68). The tunnelling current
3.4 Tunnelling junction and Josephson effect
57
is the derivative of the number of electrons in the system A with respect to time, which is given by the commutation relation of NA = J2k,a alaak<x Hj, namely
lcpah.c.].
(3.69)
k,p,cc
In most cases, a constant voltage V is applied between the two sides of a tunnelling junction. If system A has an electric potential — eV while B has 0 potential, electrons in A have more energy than those in B by — eV. Accordingly the matrix element (m\crk(Xcva\n), which transfers an electron from A to B, has an extra phase t~ieVt in addition to the ordinary phase e i(£ n £ m )t j j e r e  m ^ a n ( j n^ a r e energy eigenstates of the system A + B in the absence of Hj. It is convenient to include this extra phase in Hj from the beginning. Let us define HT(t) = hTe~ieVt + hT1e*Vt,
hT = J2 Tkpalcp*
(3.70)
k,p,a
for this purpose. We need to evaluate the expectation value of the current J in the presence of Hj. The tunnelling junction is assumed to be a weak interaction and hence we may keep lowest order terms, that is, terms of the order of T 2 . This is just the linear response theory introduced in Section 3.3 and we simply adopt the formalism developed there. From Eqs. (3.69) and (3.70) one finds
= i f dtf([J(t\HT(t')]) J —CO
= 2eRe f J—c
(3.71) The second term is characteristic of a superconductor and it yields a finite contribution because the electron number is not a good quantum number in each system, A and B. If Eq. (3.71) is written in the same form as Eq. (3.48), one obtains n,m
'EmEn 2
x{(n/?Tm) + e
i2eVt
+
(n\hT\m)(m\hT\n)}.
eVi5 (3.72)
58
BCS theory
3.4.1 Quasiparticle term The summation over states in Eq. (3.72) is carried out separately for system A and system B. Let us introduce the spectral density of each system as PAa(G\k9CO)= J2
ZA^XpiPEnjKflAlakMA)]2
nA,mA
xS{coEmA+EnA)(l+s^)
(3.73)
and similarly for pQ^G)ip,oi). The contribution from the first term in the curly brackets in Eq. (3.72) can be written in terms of these spectral densities as /7"da>ida>2 nd(a>2  a>i + eV)
k,p (G
\
JJ
W
G )
(3.74)
Suppose \Tkp\2 may be replaced by the averaged value over the states near the Fermi surface, which is a good approximation in most cases. Then the above equation becomes / =4ne{\Tkp\2)
f dco@A(co)3JB(co  eV)\f(co)  f(co  eV)],
(3.75)
where ~
'~
o)
(3.76)
k,(X
is the density of states. Since states in the BCS model are described by quasiparticle excitations, the spectral density Eq. (3.73) is readily obtained as p
(3.77)
If, furthermore, there exists the particlehole symmetry, the coherence factor vanishes upon the summation in Eq. (3.76) and the density of states becomes ®(
M
2
6(\co\ 2
which is the density of states given by Eq. (3.7). 1. / nn  If both A and B are in the normal state, the densities of states are S^A(CO) = NA(0) and similarly for B. Then one readily finds i?i= 4 7r e 2 <T fcp  2 )iV A (0)JVB(0).
("3 78)
3.4 Tunnelling junction and Josephson effect
>
40 20
1
3
0 20 40
59
—r~ 42 0 2 4 Voltage (mV)
Fig. 3.9. The / — V characteristic curve of a NbPb tunnelling junction at T = 1.4 K. Note the Josephson current at V = 0. The tunnelling current obeys Ohm's law and R x is the conductance per unit area. 2. Jsn. Suppose the system B is in the normal state. This case is important in studying the electronphonon interaction for example. To compare theory with experiment, it is convenient to analyse d/ s n /dF: d/sn dV
_i r ° 700
df(coeV) dco
One may measure the density of states ^A(&>) since the derivative of the distribution function is finite with width k^T near co = eV. An explicit example will be given in Chapter 4. 3. Figure 3.9 shows the tunnelling characteristic / s s for which both sides of the junction are superconductors. This case is studied in detail in the next subsection.
3.4.2 Josephson term Let J be the contribution from the second term in the curly brackets in Eq. (3.72). In order to write this term in a form similar to Eq. (3.74), we introduce a new spectral density
piF\k,co) = Y,2l^^{n\ak]\m){m\a.ki\n)d(cD
 Em + £„)(! + e " ^ ) ,
n,m
(3.80) where the subscript A or B has been dropped to simplify the notation. It readily follows from Eq. (3.2) that the new spectral density in the BCS model is given by (F\o)
= +ukvk[5(co  ek)  5(co + sk)].
(3.81)
60
BCS theory
If \Tkp\2 is replaced by the averaged value as before, one has the expression corresponding to Eq. (3.74),
ff dcoidco2lm(( II
J = ^(eRNA(O)NB(O))L
1 ~———e~
i2eVt
/ / dcoidco2 Im V a>2 — coi +• —ev — — id JJ JJ \o)2 — G>i + eV — lc
2
(3.82) Let us recall here that the factor u^k in Eq. (3.81) is proportional to the order parameter. Accordingly Y.k PA^(^> W) i s proportional to the order parameter, that is, the wave function of the condensate, of the system A. In the simple BCS model one therefore has
, co) =
Yl T j
^
A
g(oj2  A2).
(3.83)
Here / is the phase of the order parameter (or A) and is constant in the present case. If the above relation is substituted into Eq. (3.82) one obtains J =
(
A
(
sin B (02 — co\TTT7 + eV ^
+nd(co2 coi+
^F)COS(XB
^A  XA  2eVt)\,
(3.84)
where P stands for the principal part. Note, from Eq. (3.82), that AAAB. Note also that J depends on the phase difference of the pair wave functions and hence oscillates with frequency 2eV in the presence of a potential difference. The second term in the curly brackets of Eq. (3.84) has the same structure as the quasiparticle term and is considered to be a contribution from pair tunnelling. Although the existence of this term has been confirmed experimentally, we do not consider it further here. The first term gives the wellknown Josephson effect. The contribution of this term, denoted by J s i, will be considered in the following. Note first of all that if there exists a phase difference XB — XA between two superconductors A and B, then J s i is finite, even when V = 0. This corresponds to a supercurrent induced by a spatial variation of the order parameter phase in a bulk sample. The current here is carried by pairs keeping coherence while they tunnel. Let us write J s i = J c sin(xB  XA)
(3.85)
3.4 Tunnelling junction and Josephson effect
61
Fig. 3.10. The interference effect due to an external magnetic flux Q> piercing through the ring.
when V = 0. The energy of the tunnelling junction associated with this current is = Jc
COS(XB 
XA\
(3.86)
which takes its minimum when XB = XA Suppose both sides of the junction are made of the same superconducting metal (A = AA = AB). In the BCS model the above coefficient is given by (3.87) In the limit T
v"'
A A + AB
VA A + A B y
where K is a complete elliptic integral of the first kind. Interference effect Suppose there are two Josephson junctions in a loop of superconducting wire and a flux O pierces through the loop as shown in Fig. 3.10. If the effect of the current is negligible except at the junctions, one may invoke the same argument as that for the flux quantisation in Chapter 1 to find
= 2e j Adi =
62
BCS theory
If the two junctions have identical characteristics, the supercurrent flowing from the left side to the right side is given by
where % = XR(XI) ~~ ZL(^I) + ftO/^o The phase of the wave through the two paths changes and interferes as the magnetic flux O varies. The SQUID (superconducting quantum interference device) makes use of this principle to measure a magnetic flux. It can measure a very small magnetic field of the order of 10" 7 G. a.c. Josephson effect It can be seen from Eq. (3.84) that an alternating current of frequency hco = 2eV0
(3.88)
appears when a potential difference Vo is applied to a Josephson junction (we use the subscript 0 to denote an applied direct current voltage). This is called the a.c. Josephson effect. The voltage V = 1 x 10~6 V corresponds to 2nco = 483.6 MHz according to Eq. (3.88). The frequency of an a.c. Josephson current determines the potential difference. As a method to measure this, let us consider the case in which an a.c. voltage of frequency co\ is applied together with a d.c. voltage Fo. The first term of Eq. (3.85) is written as Jsl
=Jcsinx(t)
where %(t) is the phase difference between A and B and it is assumed that V is not very large. Let us recall here that the scalar potential always appears with the timederivative of the phase of the wave function due to the gauge invariance requirement. We have, in the present case, a pair made of two electrons, and hence the relevant combination is 2eV + d%/dt where we have put h = 1. Since V = 0 implies / =constant, the timevariation of x should satisfy dx/dt + 2eV = 0.
(3.89)
If V = Vo, this becomes x = —2eVot + const, and reproduces Eq. (3.84). If the solution of Eq. (3.89) for V = Vo + vcoscoit is substituted into the above expression for J s i, one obtains J(t) = Jcsin[2eFo£ + (2ev/coi) x sincoit + const.]. The Fourier expansion of the above expression reveals the important fact
3.5 Meanfield theory in the presence of spatial variation
63
80 70
400
800
1200
Voltage (jiV)
Fig. 3.11. The steps in the / — V characteristic of an SnSn tunnelling junction (T = 1.2 K) in the presence of a 10 GHz microwave. (From [Gll].)
that J(t) has a d.c. component if = ncoi
(n is an integer)
is satisfied. This effect is observed in an experiment in which the / — V characteristic of a junction is measured while a microwave of frequency co\ is applied. It is seen from Fig. 3.11 that steps are observed at V = n(hco/2e), which are called the Shapiro steps. A quantitative analysis of the characteristics requires a treatment in which the current due to quasiparticles is also considered. Since the microwave frequency measurement can be done with a relative error of the order of 10~12, the ratio 2e/h = 4.8359767 x 1014 Hz/V can be employed as a voltage standard thanks to this effect. There are many topics concerning the Josephson effect which we have left untouched. See [C4] and [Dl] for further information.
3.5 Meanfield theory in the presence of spatial variation
In the presence of an inhomogeneity due to an external field, boundaries or impurities, the energy gap also varies in space, which produces localised excitations and scattering of quasiparticle excitations. It is convenient to
64
BCS theory
introduce real space formalism to treat this kind of problem. Let us write the Hamiltonian in the meanfield approximation as
= I dx t t
l i
+ A(x)Vf (x)y}(*)}
(3.90)
Here H^ is a oneparticle Hamiltonian in which the band effect of the periodic potential is taken into account. This is given by (l/2m*)(V/i — eA/c)2 — ji in the free electron model. The constant A*^ has been dropped here. U(x) is the potential due to impurities and boundaries, and ordinary corrections due to the HartreeFock approximation have been renormalised into the chemical potential fi. The attractive interaction is approximated by —gd(x — x!) as before and the mean field for the superconductivity is A(x) =  g ( v T W v i W > .
(3.91)
The equations of motion for xp and xp^ in the Heisenberg picture are
(3.92)  1  ^ = [H(b) + U(x)]xpl  A (x)v>. They are different from the ordinary HartreeFock equations in that xp^ and xp] couple to each other. We have assumed for simplicity that U(x) is independent of spin. Corresponding to the Bogoliubov transformation (3.2), the fields xp and xp^ are expanded in terms of the creation and annihilation operators yn^ and yL of the quasiparticle in the eigenstate n as
^\
f\Vt
vn (x) un (x) J
\yli
Here (un(x),vn(x)) is the eigenfunction and reduces to the plane wave state (&kxUk,elkxVk) in the homogeneous case. If one substitutes the Ansatz M> yli ^ e~18nt ^ n t 0 Eq (3.92) and sets the coefficient of yn^ (or y^) to 0, one obtains the Bogoliubovde Gennes equation which determines un(x) and I H(b) + U(x)  sn
{
A*(x)
A(x)
H{h)* + U(x) + sn
It can be shown from Eq. (3.94) that if (un,vn) is a solution with the eigenvalue en, then (w*,i;*) is a solution with the eigenvalue —e n. Thus we
3.5 Meanfield theory in the presence of spatial variation
(a)
65
(b)
Fig. 3.12. (a) The spatial variation of the energy gap when a superconductor is in contact with a normal metal, (b) Andreev scattering. The velocity vector of the excitation is reversed. need to consider the quasiparticle excitations with a positive energy only. Note that eigenfunctions with different eigenvalues are orthogonal to each other. The gap A(JC) is determined from Eqs. (3.91) and (3.93) as (3.95)
and it is then left for us is to find the solutions (un,vn) which satisfy both Eqs. (3.94) and (3.95) simultaneously. In the absence of a magnetic field, the assumption of uniformity readily leads to the results of Section 3.1. The Bogoliubovde Gennes equations (3.94) and (3.95) are employed to find the energy gap A(x) and the quasiparticle excitation in the presence of inhomogeneity induced by boundaries or an external magnetic field. For example, when a superconductor is in contact with a normal metal or a different superconductor, the gap A(JC) varies in the vicinity of the contact, see Fig. 3.12(a). A quasiparticle scattering due to the spatial variation of A (the Andreev scattering) takes place in this case as shown in Fig. 3.12(b). Suppose a particle is incoming with momentum k from the normal side (n). On entering the superconducting side (s), the particle forms a pair with a particle with momentum —k and the pair becomes a part of the condensate. Accordingly a hole with momentum —k remains in the n side. The reflected wave in this case propagates in the opposite direction to the incoming wave and this should be compared with ordinary scattering where only the component perpendicular to the reflection plane changes sign. It is known that the magnetic flux quantum penetrates into a type 2 superconductor and there exist localised states in the vicinity of the flux. The Bogoliubovde Gennes equation is used to analyse these states in Chapter 5. (See [Cl].)
66
BCS theory
3.5.1 Effects of defects and boundaries One of the remarkable features of an ordinary superconductor is that Tc is almost independent of such defects as surfaces, boundaries, nonmagnetic impurities or dislocations. Let us assume that the defect potential U(x) is independent of spin. One has H^ = H^) in the absence of an external magnetic field (A = 0). The operator in Eq. (3.94) becomes real if A(x) is taken to be real (a constant phase e1* may be removed since v(x) may be redefined to have the same phase). This implies that there exist real solutions (un,vn) with degenerate eigenvalues ewj = enj = en. Therefore Eq. (3.95) justifies the assumption that A(x) is real. This can also be explained from the viewpoint of pairing. Although U(x) is quite a complicated potential, in general, the eigenvalue equation
always has a set of oneparticle wave functions {(j)n}9 which form a complete orthonormal basis. It is clear that if (j)n^ is a solution with the eigenvalue £n then (/>* is also a solution with the same eigenvalue. Accordingly, the theory becomes identical to that for a uniform case if electrons in the states 0 n j and (/>* are to form a pair. The pair wave function in the present case is (4>n^(x)(j)^(x)) and is real as mentioned above. In a singlet swave superconductor, a oneelectron state \pm, % being the spin, and its timereversed state Rtxpna generally form a pair. Accordingly, the pair is made of the set (xpn^(x),xp^(x)) as above, since angular momentum changes sign under timereversal. In the presence of impurities or boundaries, a pair is made of a oneparticle state (and its timereversal) in which scattering from these defects is already taken into account. Furthermore, if impurity atoms are distributed randomly so that one may assume A(JC) is independent of JC, one obtains from Eqs. (3.94) and (3.95) the gap equation A
=8E A n
ZSn
tanh
^T> Z
8
» = \/tn2 + A\
(3.96)
which is identical to that for a uniform case. Therefore the gap A does not change, unless the density of states near the Fermi surface is modified by impurities. (It should be noted that impurities affect the scattering process if the interaction and the density of states are anisotropic near the Fermi surface.) Although the electron density changes, of course, within the screening distance rs from the boundary or an impurity atom, this effect may be negligible since rs is small. An important example of cases without timereversal symmetry is a magnetic impurity, which leads to depairing. A system carrying a supercurrent
3.6 Gor'kov equations
67
has been treated in Section 3.2, where it was shown that a pair wave function has a phase factor elq x and is no longer real. Then the above argument is not applicable and even nonmagnetic impurities lead to depairing. The Hamiltonian satisfies H(\>) ^ H^ in the presence of an external magnetic field, which necessarily induces spatial variation of the phase. In general the superconducting state is then dramatically altered.
3.6 Gor'kov equations
The Green's function method, which is useful in manybody theory, is an indispensable tool in the theory of superconductivity. This is evident, for example, in the theory of electronphonon interaction which will be treated in the next chapter. In the present section, we formulate the BCS theory in terms of the Green's functions, which will be helpful in the following discussions. (For the generalisation to imaginary time formalism and other topics, see [Al] and [A4] for example.) The oneparticle Green's function is defined by
= i(Tipa(x,t)ipl(x',tf)).
Gap(xj;x\t')
(3.97)
Here tpa(jc, t) is the electron field operator in the Heisenberg representation, T is the timeordering operator (for tr > t, the average becomes i{\pt(xf9tf)\pOL(x9t))) and (• • •) denotes the statistical average. There exists a pair condensate in the superconducting state, where we restrict ourselves within the spinsinglet pairings. Then, in addition to G, one has to introduce F(x,t;xf,1?) =
( p i ( , )
W i
( , ) )
)\{\r))
(3.98)
It is convenient in a uniform system to introduce the Fourier transformed function such as dteimt(Taka(t)al(0))8ali.
Ga/!(*, co) =  i /
J — 00
Let us denote an eigenstate of the total system with the eigenvalue E n by \En). The Green's function G is obtained from the definition of the statistical average as
Re G(k,co) = + f ° Jao
Im G(k,co) =
G
n( \
dxp{G\k,co)P—— ' COX
(3.99)
68
BCS theory
Here p^ is just the spectral density defined by Eq. (3.73). Similarly the Green's function
F(fc,co) = r
dteiM(Tak](t)aki(O))
J—oo
can be written in terms of the spectral density p(F\k,co) of Eq. (3.80). The Green's function above is defined at an arbitrary temperature. At finite temperatures T ^ 0, however, finite temperature Green's functions employing imaginary time must be introduced in order to use perturbation theory based on Wick's theorem. Accordingly we restrict ourselves to the case T = 0; we will be concerned with the ground state Green's functions only. The equations of motion that the Green's functions G and F satisfy are obtained readily from Eq. (3.92) as
i ^  Jfy)  £ / « ] G(x, t; *', tf)  iA(x, t)F\x9 t;x\ tf) = 8(x  x')5(t  tr) l
Jt (3.100)
The mean field A(JC) is obtained from the definition of F as A(x9t) = gF(x,t+;x9t).
(3.101)
Here t + = t + At (At > 0) and At —• 0 is understood. The potential U contains the HartreeFock mean field. Equations (3.100) are called the Gor'kov equations. Gor'kov equations are quite useful in analysing spatially nonuniform superconducting states in the presence of a magnetic field or impurities for example. We note en passant that the nonvanishing matrix elements appearing in the mean field are of the form (N — 2\xp\p\N). Thus A(x,t) has a time dependent factor e~l2/zt. Similarly A*(x,i) is proportional to Ql2fit. The a.c. Josephson effect in the presence of a potential difference, which we studied in Section 3.4.2, is related to this factor. As a preliminary to the next chapter, we calculate the Green's functions G,F and F^ for a uniform case in the absence of an external field. It is also assumed that spinorbit interaction is absent. Let us first introduce the following Nambu formalism to show that FeynmanDyson perturbation theory is applicable to superconducting states. We first note that = ( a\v
akl )
(3.102)
3.6 Gor'kov equations
69
satisfy the fermionic commutation relation
{ak{tla\(t)} = \. F r o m this observation, o n e defines the following 2 x 2 G r e e n ' s function
,t) = i(Tak(t)al(O)) _(
\U«(k,t)
iF(k,t) \ G u(k,t)) )
((
Now the Hamiltonian H^) is written, with the help of Eq. (3.102), as (3.104) k,a
where T^'S are the Pauli matrices and £k is the conduction band energy including the HartreeFock energy. The free particle Green's function without interactions is given by Zk<£3).
(3.105)
The interparticle interaction (2.17) is written in the form of a 2 x 2 matrix as
Hi =   E
l
i
which can also be written as (3.106)
H
Therefore one may regard a/k and ak as twocomponent fermion operators and use Wick's theorem in the perturbation theory, if only one keeps in mind that the Green's functions and the interactions are of matrix form. Therefore one may employ the ordinary Feynman diagram technique. In the meanfield approximation one obtains from Eq. (3.106) the Hamiltonian H
i = H
%W*i + ^2)h
(3.107)
E
(3.108)
k
where we have put q = 0 and
^
70
BCS theory
With these definitions, the meanfield Hamiltonian is written in a compact form as
A = A^i! + Af \ ,
(3.109)
from which one readily obtains the matrix Green's function
G(k, co) = _ J  _ ( o , i + &e3 _A),
(3.110)
where £^ = <^ + Afc2. This result may be derived, of course, from the Gor'kov equations (3.100) directly. The gap equation is just Eq. (3.108) and AJ^ and A^ are determined by similar equations. A^ and iAJ^ are real numbers and the x defined by lA^e1* = AJ^ + A[2^ is the phase of the condensate. It is noted that A^ 2^ are complex numbers for a phononmediated attractive force. Two final remarks are in order. The Gor'kov equations and the Bogoliubovde Gennes equation are equivalent formalisms in the weakcoupling approximation, where there is no time delay in the interaction. In cases in which averages over the impurity positions are involved, however, the Gor'kov equations must be employed since what are to be averaged are not the wave functions but the Green's functions (the correlation functions). It is exceedingly difficult to solve the Gor'kov equations in the presence of a magnetic field or in the analysis of the proximity effect, which appears when a superconducting metal is in contact with a normal metal. The crudest approximation which is useful to treat these systems is the GinzburgLandau theory, which is applicable when the scale of the spatial variation L of the system satisfies L > £o, see Chapter 5. The semiclassical approximation (G. Eilenberger, 1968) is a useful method when £o <: L > fep1, see [C2] for details. It is assumed there that the amplitude of all the quasiparticle momenta k is fep and the energy associated with the spatial variation is approximated by v?k • V. We note that if the pair has an angular momentum other than the swave, the mean field A^ depends on the direction of k (see Chapter 6) and accordingly one has to introduce the xdependent field A^(x). Thus the semiclassical approximation must be introduced from the outset.
Superconductivity due to electronphonon interaction
In most superconducting materials including metals such as Al, Pb and Nb and metallic compounds such as Nb^Sn, the electron pair is induced by the phononmediated interaction between electrons. This interaction is simplified in the BCS theory and is replaced by a direct attractive force between electrons. Here we discuss a theory in which electronphonon interaction is considered from the beginning. In so doing an approximation to the Coulomb repulsion between electrons is also taken into account. In band theory, which serves as the foundation of the theory of electrons in solid state physics, one considers the Schrodinger equation with periodic potential of ions resting on the crystal lattice together with the meanfield potential that incorporates to some extent the Coulomb interaction between electrons. As a result, oneelectron states expressed by Bloch functions are obtained as the eigenfunctions. These states are specified by the band index, the wave number k in the first Brillouin zone and the spin a, and will be denoted simply by k, a. Furthermore, the spin index a is dropped in many cases since we will not treat a system with magnetism unless so stated. It is assumed in the following that the energy eigenvalue ^ is already known through the band theory.
4.1 Electronphonon system The motion of ions is treated as a lattice vibration. The normal mode is specified by the wave number q and the polarisation a, and will be denoted simply by q. Lee bj and bq be the creation and the annihilation operators of a phonon which has been obtained by quantising a mode with frequency coq and wave number q. Then the displacement of the ions associated with a lattice vibration with mode q is given by uq = (2NM(oq)1/2(bq 71
+ blq).
(4.1)
72
Superconductivity due to electronphonon interaction
Here we have assumed for simplicity that there are N ions of a single kind with mass M. There is electron scattering in the presence of a lattice vibration since electrons move in a potential which is not perfectly periodic. The electronphonon interaction that causes scattering is
alaaka
(4.2)
to the first order in the displacement of ions. The matrix element in the above Hamiltonian is given by ^)'x].
(4.3)
Here U is the potential due to ions, /?/ the position of the /th ion in the absence of lattice vibration, cj)k(x)Qlk'x the Bloch function and nq the unit polarisation vector of lattice vibration with wave number vector q. The wave number q is determined by kf — k = q + G, G being the reciprocal lattice vector. In the following, however, the Umklapp processes in which G ^ 0 are not explicitly written. Summarising the above results, one writes the total Hamiltonian of a system of electrons and a lattice as bb
l
Mk+q,k(bq
+ biq)al+qak
+ ^coulomb
(4.4)
The final term is to be considered as a part of the Coulomb interaction between electrons, which has not been taken into account in the band energy &. The method of Green's functions is useful to analyse this system. The electron Green's functions have already been defined in Section 3.6. The phonon Green's function is defined by
2NMcoq
(4.5)
since the phonon operators always appear in the combination uq of Eq. (4.1). Corresponding to Eq. (3.99), it is convenient to express the Fourier
4.2 Electronphonon interaction in the normal state
73
transform D(q,co) in terms of the phonon spectral density pph as
D(q, co) = r d x p ^ , x) ( Jo
l
—rj: 
[co — x + id
* ., }
(4.6)
co + x — id)
n) 2 5(x  En),
(4.7)
where 0) and \n) are the ground state and an excited state with energy En respectively. Here use has been made of the relation a>q = a>q and only the form at T = 0 has been given. When there are no interactions of phonons with each other or with electrons, we have the free phonon spectral density PPh(0)(<7, x) = {2NMcoq)l5{x  coq).
(4.8)
There are three physically important effects of electronphonon interaction: 1. Electron scattering by phonons. This contributes to the lifetime % and manifests itself in transport phenomena such as the electrical resistivity. 2. Renormalisation of the electron energy. In particular this leads to an increase of the effective mass m*, which can be distinguished from the effect of the periodic potential. This may be observed through specific heat data. 3. It leads to the electronelectron interaction. This was first proposed by Frolich as the origin of superconductivity, see [C2] for example. As a preliminary to superconductivity, which is the main theme of the present chapter, in the next section we study the effects of electronphonon interaction in the normal state, that is, the effects 1 and 2 mentioned above.
4.2 Electronphonon interaction in the normal state Important information on the system, such as the density of the excited states, is obtained once the Green's functions are known. Let Go and Do be the electron and the phonon Green's functions, respectively, in the absence of any interaction. In Fig. 4.1 they are represented by thin solid and wavy lines respectively, while those with interaction are thick solid and wavy lines in Fig. 4.2. The interaction is denoted by a vertex which emits or absorbs
74
Superconductivity due to electronphonon interaction
Fig. 4.1. The electronphonon interaction, (a)
(b)
2 =
Fig. 4.2. The Feynman diagrams for (a) the electron Green's function and (b) the selfenergy. a phonon. It is necessary to evaluate the selfenergies E(A;, co) and U(q,co) defined by the FeynmanDyson equations G(k,co) = G0(k,co)[l+i:(k,co)G(k,co)] = [G01(k,aj)X(k,co)]1 D(q, co) = [DoHq, co)  Tl(q, co)]
1
(4.9) (4.10)
to obtain the full Green's functions G and D, see Figs. 4.2 and 4.3. The selfenergies 2,(k,co) and H(q,co) are given by infinite summations of the Feynman diagrams and are shown in Figs. 4.2(b) and 4.3(b), respectively. Corresponding to the direct interaction VIM between electrons, one has the quantity \Mw\2D(k — k',co — co')9 which is one of the fundamental building blocks in the perturbative expansion. It is common to introduce the combination g(k9kf9x) EE N(0)\Mw\2Pph(kkf,x)
(4.11)
since \Mkk'\29 containing all information of the individual system, is always multiplied by the spectral density Pphiq.co) (we note that the symbol <x2F is often used, instead of g, in literature). It is assumed here that the system is of unit volume. It will be shown below that g(&, kf, x) is a dimensionless quantity and will prove to be useful in characterising the strength of the electronphonon interaction. It is important to realise that the phononmediated
4.2 Electronphonon interaction in the normal state
75
* D
Do
Fig. 4.3. The Feynman diagrams for (a) the phonon Green's function and (b) the selfenergy.
u —a = C
i + / > ~ s s + fr\ rv\ + ...
Fig. 4.4. The processes that are considered in the electron selfenergy calculation. interaction depends on the variable x which corresponds to the frequency, in contrast with the direct interaction. In other words, the interaction is timedependent since the action takes time to propagate. The main purpose of this section is to calculate the selfenergy 2 of an electron. As for a phonon, the spectrum coq, at least, is known experimentally through neutron diffraction and other methods, as we will see later. Hence, supposing the effect of the interaction is to renormalise phonon frequency to the actually observed value coq, one can neglect the phonon selfenergy H(q,co) in Eq. (4.10). Note however that such a scheme is not allowed if phonons are 'softened' by an interaction with electrons. Let us assume that the electron selfenergy S is approximately given by the first term of Fig. 4.2(b). That the other terms are negligible is justified by Migdal's theorem, which we will touch upon later. Even in this approximation, all the diagrams in Fig. 4.4 are taken into account. The corresponding expression is
( 2ni \a> — co f — x + id
co — cof + x — id
(4.12) This is an integral equation since G in the right hand side contains 2. Our purpose is to obtain 2(/r,co) for \k\ = fcp and \co\ of the order of the Debye frequency COD "C £F Accordingly most contributions in the a/integration come from the region cof ~ O)D since co, x ^ COD Then it follows that most contributions in the A^summation come from those kf with \kr\ ~ fep. Making use of these facts, one puts \k\ = \kf\ = /cp and replaces the ^summation by
76
Superconductivity due to electronphonon interaction
G>
complex co plane Fig. 4.5. The modification of the integration contour in the selfenergy calculation.
Y,k, ~ N(0)J^Jd^kfHowever the a/integration should be carried out first. In the limit T > 0, Eq. (3.99) becomes /•oc
G(k,a>)=
dx
/ J—o
P(G)(k,x)  x + i(co/M)<5
Thus the function G is defined separately for co > 0 and co < 0 and, if co is continued to the complex plane, these functions are analytic in the upper half plane and the lower half plane, respectively. By making use of this fact, one can change the contour of a/integration to the path shown in Fig. 4.5, which runs slightly below the negative real axis and slightly above the positive real axis. As a result, the &/integration in Eq. (4.12) is rewritten as f ( r°°dco do/
9{cof) — cof — x + iS
7oo 27li
6{cor) 2ilmG(k\cof). co — cor + x — id,
According to Eq. (4.13), ImG(k',cof) is just the spectral density. If written in this form, one easily finds that the ^integration converges in the limit £' —• oo. The selfenergy X(k f,co') is considered to be independent of
ii
/
7—
can simply be obtained by residue calculus. In doing so we must keep in mind that the signature of lmL(co) is co/\co\. Finally we reach the following result, POO
= / h
C
POO
dxg(x) / h
dz [coz —
co — x co + x
1
x + id
+ co + z f+ x 
id J (4.14)
4.2 Electronphonon interaction in the normal state
11
where
J^k',x).
(4.15)
Here the system is assumed isotropic. An important point is that the £'integration can be carried out in Eq. (4.14) owing to the approximation that is applicable when COD < £F Accordingly the result is identical with that obtained by second order perturbation theory. 4.2.1 Effective mass and lifetime When the quasiparticle description is applicable, the Green's function near the Fermi surface is approximated by id) ~ (1 + kk)co — ( = 2 /
dx^.
(4.16)
Here the superscripts (r) and (i) stand for the real and imaginary parts respectively. Since the real part £^(£,0) vanishes within the approximation employed in Eq. (4.14), the peak of the spectral density ImG appears at co = £fc/(l + kk). In the isotropic case (kk = k) the quasiparticle mass becomes The variable k is, therefore, called the mass enhancement parameter. The quasiparticle lifetime T& is given by
One has to know the coupling constant g to evaluate 2 explicitly. The phonon spectrum and the matrix element Mw may be evaluated by the pseudopotential method for a relatively simple metal. We will not persue that here and, instead, use phonons in the socalled jellium model and calculate g. Electrons move in the following screened Coulomb potential of ions U(q) = 4ne2/q28(q) = 4ne2/(q2 + k2)
(4.18)
k2 = 6nne2/s^. We have assumed that the ion is univalent and employed the ThomasFermi permeability. Then Eq. (4.3) becomes \Mk+q,k\2 = [4nne2q/(q2 + k2)]2.
(4.19)
78
Superconductivity due to electronphonon interaction
In this model, phonons consist only of longitudinal mode and their dispersion relation is given by coq2 = 4nne2q2/M(q2
+ k2).
When q
2
2coqd(x
 coq).
From this expression one can get a rough idea of g. In the present approximation, one has q ~ fcp^/1 — \i with ji = kk'lk\. Then the average over the Fermi surface is equivalent to that over \i and one finds
(420)
£a^7r If this expression is used in Eq. (4.14), one obtains
Therefore, when cu < Q p , the imaginary part is given by E^ ~ — no and one finds that the description in terms of particlelike excitations is applicable in the vicinity of the Fermi surface and the lifetime at low temperatures (T
\
1+  ^ /cs
/
,
(4.22)
where the phonon wave number is assumed to satisfy q < 2/cp. The ratio /cs//cp is given in terms of the ratio of the Bohr radius ao = I/me2 and the mean electron separation ro as K2
/ 4 \ ! / 3 _Anrn
r0
4/CF
The ratio ro/ao is of the order of unity for ordinary metals. According to band theory, the electron specific heat at low temperatures is proportional to the density of states 2iV(0) = mbfep/Ti2, where m^ is the band
4.2 Electronphonon interaction in the normal state
79
Table 4.1. Observed values of m^ and the mass enhancement parameters X. Element
mth/m
mh/m
mth/mh
Li Na K Rb Cs Al
2.22 1.24 1.21 1.37 1.80 1.49
1.54 1.01 1.07 1.19 1.53 1.05
1.44 1.22 1.13 1.15 1.18 1.42
1.41 1.16 1.13 1.16 1.15 1.44
Remark: m\> and X are obtained from the pseudo potential theory, see [D2].
Fig. 4.6. Vertex corrections.
mass. Let mth be the electron mass determined from the observed specific heat. Then we expect these two masses to satisfy ^th/^b = 1 + 1
(4.23)
Table 4.1 shows that for simple metals the theoretical estimates obtained by the pseudo potential theory agree very well with the observed values. 4.2.2 MigdaVs theorem When we evaluated the selfenergy S, we neglected the higher order diagrams in Fig. 4.3(b). These higher order processes are the socalled vertex corrections and Migdal's theorem states that these corrections are proportional to the powers of y/m/M and hence small. Origin of the lowest order correction is illustrated in Fig. 4.6 and is given by
where k denotes k and co collectively. We have replaced the matrix element Mk+q,k by its average since it is not a rapidly varying quantity. The dominant contribution to the selfenergy S comes from the region where both k and
80
Superconductivity due to electronphonon interaction
Fig. 4.7. Vertex corrections and pair formation.
k + q are near the Fermi surface. Since most phonons have wave number q of the order offcp,either k — qf or k + q — q' is far from the Fermi surface and accordingly £ ~ £p Then one of the G's becomes gp1 and the above integral is of the order of CODAF ~ y/m/M. There is an exceptional case in which all of k, k + q and k — qr are close to the Fermi surface (in the sense that l£/cl < &>D) and the fourth vector k + q — q1 is also close to the Fermi surface. However the contribution from this process is a small quantity proportional to N(0)coj)/n ~ fs/^F ~ y/m/M. Migdal's theorem is not applicable to a system that can be unstable against the formation of a charge density wave or a spin density wave due to nesting. This is the case for a system with a quasionedimensional Fermi surface. We also note that the channel leading to superconductivity is made of particleparticle ladder diagrams and hence the vertex correction is as illustrated by the diagrams in Fig. 4.7. Although each diagram is proportional to a power of y/m/M according to Migdal's theorem, the infinite sum of the series diverges. Accordingly one cannot apply perturbation theory to these processes.
4.3 Eliashberg equation
The strong coupling theory of superconductivity due to electronphonon interaction starts with the Eliashberg equation, which is an extension of the Gor'kov equations. This extension amounts to replacing the electronelectron interaction V\w by g(k9k',x). It should be noted, however, that a phonon propagates with a finite velocity. Consequently there is a retardation in the interaction and the mean field itself depends on the excitation energy as will be shown below. It should also be noted that although the HartreeFock term in the Gor'kov equations may be absorbed by simply renormalising ^ , one has to deal directly with the ordinary selfenergy due to the manybody effect in the present theory. In the 2 x 2 matrix form introduced in Section 3.6, the selfenergy parts appearing in the Green's function G are given by the FeynmanDyson
4.3 Eliashberg equation
81
equation, which is an extension of Eq. (4.9) in the previous section, as ±{k,co) = GoHbco)  G\k9co).
(4.24)
Here G(k,co) is the Fourier transform of G defined by Eq. (3.103) while Go(k,co) is obtained similarly from Eq. (3.105). The electronphonon interaction, that is, the third term in Eq. (4.4) is obtained by replacing a[+ ak by a matrix al+ T$ak in this formalism, see Eq. (3.106). Therefore evaluating Z with the Feynman diagrams in the previous section amounts to applying the same approximation to the superconducting state. Then one obtains, corresponding to Eq. (4.12), the selfenergy
X
co — cof — x + id
co — co' + x — i J (4.25)
Let us consider the general relation between G and E before we start explicit calculations. We again note that there is no magnetism in the system under consideration and hence G is independent of the spin and the system is invariant under spatial reflection, that is, G(—k, co) = G(k, co). Let us write, therefore, G^(co) = Gn(co) = G(a>) (we will omit the variable k in the following unless necessary). From the definition of G, Gn(co) = G(co),
G22(co) = G(co).
(4.26)
Let us rewrite Eq. (4.24) as (GQ1 — E)G = 1. This equation is equivalent to the set of four equations for the Green's functions defined by Eq. (3.103). One notes from Eq. (4.26), however, that there are only three independent Green's functions. If we write Eq. (4.24) for each component we find that the components Sajg of 2 satisfy the relations (4.27)
The components of G are G((O) = [Go = S,21(
) F(CO) =
(4.28)
82
Superconductivity due to electronphonon interaction
2
2,
Fig. 4.8. Two selfenergies in a superconducting state. where d(co) = [Go1 (co) + Sn(G))] [Go'1 (co)  Sn(o))]  £i 2 (a))£ 2 iM = d(ra).
(4.29)
If one substitutes Eq. (4.28) into Eq. (4.25), one finds that the oflfdiagonal components £12 and £21 of £, which correspond to the energy gap function Afc, satisfy the same equation. Therefore the remark made for A^ at the end of the previous chapter equally applies to the oflfdiagonal components (the components £12 and £21 correspond to A^ + A^ and AJ^ — A[ , respectively). Namely e~lz£2i(ca) = elz£i2(co). The phase x is associated with 'spontaneous symmetry breaking'. It can be shown that this equality is true in general and independent of the approximation employed in deriving Eq. (4.25). Accordingly one needs to consider £12(00) only, which is now an codependent function unlike A in the BCS theory. Considering these facts, let us define co — (£(&, co) — £(£, co)) = coZ(k, co) 2
(4.30)
where we have put £n(co) = — £22(—co) = £ and £12 = £1. The selfenergies £ and £1 correspond to the diagrams shown in Fig. 4.8. If one assumes that £(&,0) is renormalised into &, one may neglect £(A:,co) + £(&, — CD) for such values of CD that are used in the following. In terms of these quantities the solutions for a uniform system can be written as
( a^lk
).
(4.31)
It now remains to solve the nonlinear simultaneous equations obtained by substituting Eq. (4.31) into Eq. (4.25). An approximate calculation is possible since the dominant contribution in Eq. (4.25) comes from the region \k\ ~ fep, in the same way as the normal state. Let us rewrite the integrand of the cointegral in terms of ImG and
4.3 Eliashberg equation
83
e
0
co plane Fig. 4.9. The integration contour to evaluate Z and Zi. (that is, the difference of the Green's function in the upper and the lower halfplanes along the cut) instead of G and F\ just as we did when we derived Eq. (4.14). In doing so, special note must be taken of the facts that (i) G and F^ satisfy the analytic property of ordinary Green's functions, namely they are analytic in the upper (lower) halfplane for co > 0 (co < 0) and (ii) cuts along the real line, that is the lines on which the denominators of G and F^ vanish, are given by co > Ao as shown in Fig. 4.9. The meaning of Ao and Eq. (4.31) lead to the definition Ao = A(Ao).
(4.32)
Thus the integration over ^ is carried out first. Then g is replaced by g(x) after being averaged over k as was done in Section 4.2. If the system is isotropic, Z and A become functions of co only and Eq. (4.25) becomes ~
poo
[1 Z(co)]co = /
dz Re
JAo
V
Z
A*+W),
(433)
 A (z)
Z(co)A(co) = f°dz Re JA0
2
A{z)
2
\/z  A 2 (z)
/~\^z\
(4.34)
where
±V, z) = f°dxg(x) (—4 Jo
\co + z + x — io
rj ±
1
~rrj)
•
(4.35)
co — z — x + ioj
To understand Eqs. (4.33)(4.35), let us find a solution of these equations when all the phonons have a common frequency COE (Einstein phonons). Since we are interested in the gap equation A(a>), we put A = 0 in Eq. (4.33) and employ the normal state solution Z(a>) ^ 1 + X, which is obtained with an assumption co
(4.36)
If this expression is substituted into Eq. (4.16), one finds that the mass
84
Superconductivity due to electronphonon interaction i
(a)
3
V A\ \\ / A", / \ A 1
2.0 1.0
I
1.0
(b)
i
y,
2.0
i
2
•
—
V
/] t \
1
\
\
V
(o—Ao
^2
—
COE
(c) o
(o—Ao
COE
Fig. 4.10. (a) The phonon spectrum with a single phonon peak. This spectrum has been used to evaluate the solution A(co) whose real (imaginary) part is shown by the solid line (the broken line) in (b). (c) is the solution with the Coulomb interaction taken into account. (DJ. Scalapino: [C2] vol. I.)
enhancement parameter is just given by this L If Eq. (4.36) is substituted into Eqs. (4.34) and (4.35), one obtains the integral equation dz Re
COE
i
W
. (4.37)
Figure 4.10 shows numerically the phonon spectrum close to the Einstein phonon and the gap function obtained from the spectrum. Some important qualitative features are found from Eq. (4.37): 1. If one takes co = Ao, one obtains an equation which determines the gap edge Ao. This equation has a nonvanishing solution Ao. 2. The real part of A(co) is positive (negative) for co < COE (CO > &>E)3. The imaginary part ImA(co) appears for co > COE + Ao. At finite temperatures, however, ImA(co) is finite even for co < COE + AQ.
4.3 Eliashberg equation
Particle
Hole
Hole
85
Particle
t= t
Condensate
Condensate
Z12U) Fig. 4.11. The processes represented by Z12 and S^i
4.3.1 Weak coupling The dominant contribution to the integral in Eq. (4.37) comes from the domain z < COE if A < 1 namely Ao
dz
A
°
from which we obtain the BCS gap equation. We thus obtain A(co) = const. = Ao, co < coc. This is the weak coupling limit where we have justified the BCS theory. Before we close this section, let us comment on the codependence of the gap function. Z12 and S21 are the probability amplitudes for the processes shown in Fig. 4.11. Since it takes a finite time for a phonon to propagate, the amplitudes S12 and L21 are functions of t and hence complex functions of its Fourier transform co. It is physically expected that these amplitudes are identical since the amplitude for a hole at t = 0 remaining a hole at later time t = t is the same as that for a particle at t = 0 remaining a particle at t = t. The selfenergy Si and hence the imaginary part of A(co) leads to the finite lifetime of a pair state due to phonon emissions (and scattering of thermally excited phonons at finite temperatures). The phase associated with symmetry breaking, namely the phase of the condensate can be understood as the phase of A at the gap edge, which has been taken as a real value of Ao above. Even if A at the gap edge is chosen real, the function A(co) for co 7^ Ao is in general complex. Let us consider the present problem as that of a twobody bound state as mentioned in the beginning of Chapter 2. Since the interaction due to the exchange of phonons (pions for the nuclear force) involves retardation in
86
Superconductivity due to electronphonon interaction
A(*)/Ao
A(*)/Ao
> tQ)E
Fig. 4.12. The Fourier transforms of A(co). The solid (broken) line depicts the real (imaginary) part. Only the electronphonon interaction is considered in (a) while the Coulomb interaction is also included in (b).
time, the twobody wave function must be thought of as a function of x\,X2 and t\9t29 or equivalently, (l/2)(ti + £2) a n d h — ti. If the wave function is Fourier transformed, it becomes C(k,co,q,Q) instead of C(k,q) as in Section 2.1. Since the momentum and the energy are conserved if there are only two particles, those states with different q and Q decouple in the equation of motion. The codependence appears, however, in the equation corresponding to Eq. (2.8). We can regard this codependence as the temporal extension of the wave function (see Fig. 4.12). It will play an important role in the effect of Coulomb repulsion studied in the next section.
4.4 Coulomb interaction
Needless to say, the repulsive Coulomb interaction Vc between electrons must be considered at the same time as the electronphonon interaction. Unlike the phononmediated interaction, the codependence of Vc appears when co reaches the plasma frequency a>p. Here Vc is assumed to have no retardation and hence be independent of co, since cop > co? in many cases. We say that the repulsive force Vc is diluted over the range 0 < \co\ < cop, in contrast with the phononmediated attractive force which is localised at \co\ ~ COD We will take advantage of this fact to treat the problem approximately. First of all, contributions to 2 and £1 are restricted to the lowest order diagrams in Vc (Fig. 4.13), which are formally the same as those for electronphonon interaction. This amounts to keeping the Fock terms only. In this approximation, and dropping the summation and integration symbols, one simply adds ifi = VcoG and Z ^ = Vc o F^ to those terms due to electron
4.4 Coulomb interaction
87
• \
I
Fig. 4.13. The selfenergies due to Coulomb interaction (dotted lines).
phonon interaction to obtain S = Z (ph) + E (c) ,
Si = S(Ph) + 2
(4.38)
Let us first consider lSc\ The contribution Vc o Gn to the selfenergy in the normal state is expected to have a weak to dependence due to the reason mentioned above. Accordingly one can assume that this contribution is taken into account by renormalising &• Thus one only needs to consider S(c)' = yc o (G  Gn). It should be noted, however, that G and Gn differ only in the vicinity of the Fermi surface while the contribution to Vc comes from a much broader area in momentum space. Therefore one may drop E ^ ' and, as a result, one needs to consider only ^ c ( * , * ' ) i r f ( * > ' ) = VQoI*.
(4.39)
In the above equation, the a/integration extends over a broad domain \co'\ ~ cop > COD Let us introduce a frequency coc, which is several times as large as COD, and divide the a/integration domain into I (c/ < coc) and II (o)' > coc). Since  2 ^  < c»' in region II, F^ is approximately given by
2
K(k',co') =
2 1
(4.40)
Note that 2 ^ is also negligible in the numerator. By making use of this fact, one may introduce an effective interaction U in which the contribution from region II is incorporated and rewrite Eq. (4.39) into an integral equation over region I. For this purpose, let us consider U which satisfies an equation expressed by the diagram Fig. 4.14, which is of the same form as the Tmatrix. Here the intermediate states are restricted within region II, where a/ > co c. The diagram is written, in a symbolic form, as U = Vc + VcoK1oU.
(4.41)
If this equation is compared with the following equations, obtained from
Superconductivity due to electronphonon interaction II
U
Vc
Vc
U
Fig. 4.14. The equation which determines the effective Coulomb interaction. Eqs. (4.39) and (4.40),
z
+ VCO FJ = VCO FJ
+ vc ox E o sf)
it is found that UFj and Z^ satisfy the same equation. Therefore one may put Zf) = U o Fi f . (4.42) One may anticipate this relation by comparing Fig. 4.13 with Fig. 4.14 for the interaction U. Thus once a U that satisfies Eq. (4.41) is obtained, we can determine Z ^ by solving the (nonlinear) integral equation (4.42), which contains an integration over region I only. If a screened Coulomb interaction is assumed, the potential Vc is approximately constant over the region under consideration and hence U determined by Eq. (4.42) is also a constant. Then, taking the analyticity of K into account, only the following integration need be carried out, N(0)
^r
J\co'\>coc ^nl
d?K=N(0) J£b
dco'±. Jo)c
CO
Here the upper bound s^ ^> coc of the \^\integration is considered to be of the order of the band width. The commonly used symbols \i = N(0)Vc and /i* = N(0)U are related by "*=
If this relation is substituted into Eq. (4.42), one finally finds that the effect of the Coulomb interaction reduces to the replacement of Eq. (4.34) by Z(co)A(co) = r
dz Re (
A{z)
) {^"W)
" /}•
(4.44)
The upper bound of the integral in the phonon part is replaced by coc, which is justified if coc is taken several times as large as CODLet us note that since Vc is nonvanishing for a wide range of frequencies, H is weakened as in Eq. (4.43) and secondly, that \i is finite when X in
4.5 Strongcoupling effects and critical temperature
89
Eq. (4.44) is peaked at \z\ ~ COD. The effectiveness of the phononmediated attraction can be understood from these reasons. The solution A(co) when /i* is considered is also given in Fig. 4.10. One also finds that, when A(co) is Fourier transformed, the amplitude of A(t) is suppressed near t = 0 as is shown in Fig. 4.12. Note, however, that Migdal's theorem is not applicable to the present problem since there is no retardation in the Coulomb interaction and hence it operates over a wide range of frequencies. Accordingly, it should be kept in mind that the approximate 2 obtained above has no quantitative meaning. We will discuss the size of the Coulomb interaction parameter fi* in the next section. 4.5 Strongcoupling effects and critical temperature 4.5.1 Tunnelling effects The codependence of the energy gap A is directly observed by the tunnelling effect. As was mentioned in Section 3.4, the density of states SJ(CD) can be obtained from the tunnelling characteristics between a superconductor and a normal metal at low enough temperatures, see Eq. (3.79). Using the Green's function (4.31), the density of states 3)((D) is obtained, in the present case, as 2{co) =  ^ V{G(k 9 co + iS) G(k9 CD  id)}
(4.45)
and by simply putting A = A(co). The result is ®{co) = J V ( 0 ) R e ^ = ^ = = . Vco2 — A2(co)
(4.46)
Note that A2 in the square root is not A2. The density of states in BCS theory is obtained by the substitutions A = Ao (Ao = A(Ao)) for \co\ < COD and A = 0 for  co  > COD in the above expression. The strong coupling effect is measured as a deviation from this BCS result. Figure 4.15 is an example of such a measurement for lead. The deviation is 10% at most even for such a strongcoupling metal. The density of states (4.46) may be obtained, in principle, from the Eliashberg equation once g(k9k'9co)9 defined by Eq. (4.11), or its average g(co) and the Coulomb interaction parameter JA* are known. However it is difficult, in practice, to evaluate these quantities theoretically. McMillan and Rowell [C2], conversely, made an attempt to determine g(co) and n* numerically so that the measured tunnelling characteristics and Ao might be obtained from the Eliashberg equation. They obtained fi* = 0.12 and g(co) shown in
90
Superconductivity due to electronphonon interaction
1.16
0.92
8 12 16 20 co — Ao(mV)
24
Fig. 4.15. The energy dependence of the density of states of lead in a superconducting state. The broken line represents the data obtained from the tunnelling effect while the BCS weakcoupling theory yields the dotandbroken line. The strongcoupling result is shown by a solid line. (J.R. Schrieffer, et al.\ [C3].)
Fig. 4.16(a) for Pb. It is interesting to compare g(co) of Fig. 4.16(a) and the phonon density of states Fig. 4.16(b) obtained by neutron diffraction experiments. The renormalisation function Z(co) and the amplitude A(co) of Pb in the same calculation are shown in Fig. 4.17(a) and (b). The peak of the phonon density of states (van Hove singularity) manifests itself in the structure of A(co). Since phonon emission is dominant in the vicinity of the peak, the imaginary part of A increases there.
4.5.2 Transition
temperature
To study finite temperature properties such as the transition temperature T c, the temperature Green's function is employed. In actual numerical computations, moreover, it is easy to solve equations with the discrete frequency (Matsubara frequency) con = (2n + 1)TTT, n being an integer. Here we only quote the equation which determines Tc,
X(n  n>)  ?  5n
 n")^
•
4.5 Strongcoupling effects and critical temperature

1.4
1.2 _ 1.0
0.4 0.2 0
1
A
2
1
1
1
• AJV L 'k
0.80.6
91
1
1
5 0) (meV)
0
10
10
20 30 co (meV) (b)
(a)
Fig. 4.16. (a) g(co) for Pb. The dotted line shows the phonon density of states obtained by neutron diffraction experimentz. (W.L. McMillan and J.M. Rowell: [C2] vol. I.) (b) g(co) of M ^ A l obtained by the tunnelling effect. • is for a sample with Tc = 16.4 K while o is for Tc = 14.0 K. The dotted line denotes the phonon spectral density obtained by neutron scattering experiments. (From [G12].) 1
1
1
1
1
1
1
"A
3.0

1 _ I
<
I 0
* ^ .
1
10
1
1
i
i
i
i
i 
1
1
1
t
i
i
30 40 co — Ao(meV)
\
0J 1.0 
\
2.0 I
i
20

1 1.0

J i
1

2.0 :
2 
N
i
1
3 /
50
1
10
(a)
w 1
^^
f i
i
i
i
i
20
30 40 coAo (meV)
(b)
Fig. 4.17. (a) The real (solid line) and the imaginary (broken line) parts of the renormahsation function Z(a>) of Pb in the superconducting state, and (b) the real (solid line) and the imaginary (broken line) parts of the amplitude A(co) of Pb. (W.L. McMillan and J.M. Rowell: [C2] vol. I.) The function X(n — nr) above corresponds to A(co,z) in Eq. (4.35). The above equation is obtained by taking A = 0 in the denominator of the finite temperature version of Eqs. (4.33) and (4.34) and then eliminating Z(co). To find a convenient expression for Tc, we put
(n ri)=
 \con\)9(coD

92
Superconductivity due to electronphonon interaction
in the first term and X(n) = X6(cov — \con\) in the second term of Eq. (4.47) so that this equation becomes 'separable'. Here X is the mass enhancement parameter. Then if A(n) = A • #(COD — con>) is substituted into Eq. (4.47), one obtains T where xp is the diGamma function. From the above equation we finally find Tc = 1.13COD exp{—(1 + X)/(X — /**)}. We quote, en passant, McMillan's formula k^Tc = 0.83coinexp <
'——
>,
(4.48)
which has been employed most frequently in the discussion of T c. Here coin = exp(lnco),
(In co) =  / dcog(co) . X Jo co There are other improved expressions for Tc, see [E3]. 4.5.3 Isotope effects The first experimental evidence that electronphonon interaction is responsible for superconductivity in ordinary metals was derived from the isotope effect, first observed in Sn and Hg. It may be assumed that the phonon frequency co^, and hence the Debye frequency COD or the averaged frequency coin is proportional to M~ 1//2 . It is seen from Eqs. (4.14) and (4.16) that X is independent of M. Therefore only coin and /** containing coc depend on M in the expression for Tc. The isotope effect is measured by the index a defined by AH*
T
\
(4.49)
d(lnM) One finds from Eqs. (4.48) and (4.43) that
a=
\ V  1M\1';
: :::z
' ' *•
(4 5o)

One obtains the BCS value a = 1/2 if /i* is independent of M. One also notices that a is never greater than 1/2. 4.5.4 Strongcoupling effects at finite temperatures Thermal excitations tend to weaken the mean field as already mentioned. They also manifest themselves in a different form in the strongcoupling
4.5 Strongcoupling effects and critical temperature
93
theory. To see this new effect, let us generalise Eq. (4.37), which determines A(co) in the Einstein model, to finite temperature cases. The result is
\f (z) + n(coE)]
( ^ \co — z + COE —1<5 co+ z — coE where n(x) = [exp(x) — I]""1 is the Bose distribution function. The above equation reduces to the BCS expression in the weakcoupling limit. This equation also shows that A(co) is comparatively more suppressed by the finite temperature effect in the strongcoupling theory. Accordingly the ratio 2Ao/T c becomes relatively large. Furthermore Imco remains finite at T =f= 0, even when co < COE, due to the last term in Eq. (4.51). This should be compared with the fact that Imco is finite only for co > COE at T = 0. As was shown in Chapter 3, the ratio 2AO//CBTC = 3.53 and the specific heat jump AC/C n = 1.43 are 'universal' numbers and the ratio Hc(T)/Hc(0) is a 'universal' function (see Eq. (3.28)) in the BCS theory. The strongcoupling corrections to these equations are 2Ap
2
(4.52)
= 3.53
and \r
f
/K,T_\2
/
ro,..
\"
(4.53) according to approximate calculations. These ratios and the comparison of the theoretical Hc(T)/Hc(0) curves with experiments are given in Table 3.1 and Fig. 4.18. The strongcoupling effect also appears in transport phenomena. The stronger the coupling is, the shorter the quasiparticle lifetime becomes. Consequently the density of states ^(co) is modified. We note in particular that because of the appearance of ImA due to thermal excitations, as was remarked below Eq. (4.51), the divergence of 3)(co) at the gap edge is weakened and ^(co) is broadened as a result. This effect causes suppression of the peak of the nuclear spin relaxation time T^1 at Tc. The degree to which the peak is suppressed depends, of course, on the parameters of the individual system. Although we have dealt with the cases X < 1 in the present section, there
94
Superconductivity due to electronphonon interaction
0.03
0
0.2
0.4 0.6 (T/Tc)2
0.8
1.0
Fig. 4.18. The temperature dependence of the critical field. The broken line is the BCS result while o is the strong coupling result in Pb. ([E2] vol. I.)
are theories of strongcoupling limit with larger L We note in particular that the largest possible Tc in the phononmediated model has been discussed in connection with highT c superconductivity. Similar analysis has been carried out for mechanisms in which bosonic excitations, other than phonons are exchanged. These aspects will be discussed in Chapter 7.
4.6 Impurity effects
The formalism developed here is useful in treating quantitatively the impurity problems considered in Section 3.5, although it is somewhat beyond the scope of the present chapter. It is assumed that the interaction between randomly distributed impurity atoms with positions Rj and the conduction electrons is given by (4.54) Here FN denotes the interaction strength of the spinindependent scattering and Fp the strength of the exchange interaction between the impurity atoms with spin S and the conduction electrons. They are both assumed to be of the 8 function (contact) type. The latter interaction represents the paramagnetic
4.6 Impurity effects
/ /
(b)
^
\ \
/
Ue + «J
/"IN I \
1
95
/ /
W
+ «J
\ \
/ /
LJ
\ \
U. f
...
Fig. 4.19. The selfenergy diagrams due to impurity scattering. effect of the impurity atoms. It is assumed that the scattering is elastic and the impurity spin S is classical, that is, it changes only when it interacts with the conduction electrons. The conduction electron selfenergy due to the interaction Jf im is given by the sum of the series shown in Fig. 4.19. After being averaged over the impurity positions, however, only those diagrams given by Fig. 4.19(b) contribute since they are independent of the random phase proportional
to Rj. Scattering by a single atom is represented by broken lines starting from a single x. The first diagram of Fig. 4.19(b) is the lowest such process and keeping only this term amounts to the socalled Born approximation. In this approximation, one just replaces the phonon Green's function in our previous analysis by • • • x • • •. The dotted line represents FN or V?. Since the scattering is elastic, the energy co remains unchanged while the momentum and the spin change. Accordingly g(x) in Eq. (4.15) is replaced by ^
(4.55)
where —l T+
=
—l T]Sf
i T~
—l Tp
(4.56) 1
= 2nmpN(0)S(S + 1)F P  2 .
The average above is taken over the scattering angle near the Fermi surface while HjN and n,p denote the concentration of the impurity atoms. From Eqs. (4.55) and (4.14) one obtains in the normal state 2 i m = i©/(2T+M),
(4.57)
96
Superconductivity due to electronphonon interaction
\
/
\ z,
Fig. 4.20. The selfenergy diagrams due to impurity scattering in the superconducting state. from which one finds that T+ is the lifetime of quasiparticles due to impurity scattering. The AbrikosovGor'kov theory (the AG theory) analyses the impurity effects in the superconducting state, using diagrams such as Fig. 4.20 to obtain Z and Si. Note that the contribution from Fp changes sign in Si since the spins at each end have opposite sign. Then A^ in Eqs. (4.33) and (4.34) are replaced, when co > 0, by
(4.58)
where T I 1 = T^ 1 — tp 1 . In the following, electronphonon interaction will be treated within the weakcoupling approximation in order to focus on the impurity effects. Accordingly the phonon contribution to S is ignored. If Eq. (4.58) is substituted into Eqs. (4.33) and (4.34), one obtains
[1Z(co)]co = 
2T+ yjco2  A2(co)
(4.59) Z( M )A(a,)
A+
^/CO1 — A Z(CD)
IT
Here the weakcoupling approximation was employed to write dz Re , ^
2
A(z) y } A
2
=.
( )
(4.60)
From the two equations of Eq. (4.59), we obtain for u(co) = co/A(co) (4.61)
4.6 Impurity effects
97
where we have defined C = (TpA)"1.
(4.62)
Suppose these impurities were not paramagnetic and tp = oo, that is, C = 0. Then from Eq. (4.61) one obtains A = A = const, and Eq. (4.60) becomes the same expression as that without impurities. Thus the statement made in Section 3.5 has been justified. As paramagnetic impurities are increased, not only does the critical temperature Tc decrease by depairing but the gapless state appears, where the excitation has no gap in the spectrum even in the superconducting state. One simply needs to inspect Eq. (4.45) to discover this state. Since it follows from Eq. (4.61) that ^
(4.63)
one simply needs to find how Imu appears as a function of co in Eq. (4.61). Then one finds that u becomes real for co less than cog = A ( l  C 2 / 3 ) 3 / 2 provided that £ < 1. When C > 1, Imw appears from co = 0 and hence it is gapless. It is convenient to use temperature Green's functions to calculate such quantities as A and Tc as one may expect from the fact that for an imaginary frequency Eq. (4.61) becomes a relation between real numbers. Here we simply quote the results (see K. Maki in [C2] vol. II for details). The change of Tc due to rp is given by +
(464) > where Tco is the critical temperature for tp = oo, xp is the diGamma function and
TPC"1 = nTc0/2y = Aoo/2 is the value of Tpx at which Tc vanishes. At this value of tp 19 the mean free path TpfctfF for spinflipping scattering becomes of the order of the coherence length £o Figure 4.21, depicting Eq. (4.64), shows an excellent agreement between experiment and theory. The supercurrent is stable even in the gapless state and the Meissner effect is also observed there. These facts show that what is essential for superconductivity is not the energy gap but the existence of coherence. We also note firstly, that even nonmagnetic scattering causes depairing in the presence of a supercurrent such as in a magnetic field, and secondly,
Superconductivity
due to electronphonon
interaction
1.0 < 0.8
0
0.2 0.4 0.6 0.8 1.0 1.2
1.4
Fig. 4.21. The critical temperature Tc of (LaGd)Al2 as the concentration of the magnetic atom Gd is increased. The temperature Tco defined in the text is 3.24 K while the critical concentration is ncr = 0.59 at.%. The solid line shows the result obtained from AG theory. 1.0.
1
1
1
1
1
1

0.5
0
\
AG theory "
I\ 1
1
1
0.5
1.0
Fig. 4.22. The critical temperature Tc of (LaCe)Al2 as a function of the Ce concentration n. The broken line is obtained from AG theory. (M.B. Maple in [D5].)
that pairs are broken even by nonmagnetic scattering except in an swave superconductor. Although the spin of the impurity atom has been treated classically in the analyses so far, the Kondo effect appears for Fp > 0 (antiferromagnetic coupling) if the process given by the second diagram in Fig. 4.19(b) is considered. The effect of an impurity atom which shows the Kondo effect manifests itself clearly when the Kondo temperature TK is close to Tc. In this case, there is a conflict between a bound state between conduction electrons
4.6 Impurity effects
99
(i.e., the Cooper pair) and a singlet bound state between a conduction electron and an impurity spin. Therefore Tc becomes zero at a relatively low impurity density. Moreover, since tp * changes with temperature when Tc > TK, there appears a reentrant phenomenon, shown in Fig. 4.22, in which the sample becomes a superconductor at low temperature but it becomes a normal conductor again as temperature is lowered further.
5 GinzburgLandau theory
The GinzburgLandau (GL) theory has been employed for general analysis of the physical properties of an ordered phase. This theory is especially useful when the system under consideration has a spatial variation, due to an applied external field for example. It should also be noted that this theory serves as a basis for studying the effects of fluctuations, that are neglected in the meanfield approximation. The GL theory was proposed before the microscopic theory of superconductivity by BCS and has played an important role in the analysis of superconducting phenomena even after the emergence of BCS theory. In the present chapter, the timeindependent GL theory and its applications are first discussed; its extensions and the effect of fluctuations are then considered. 5.1 GL theory of superconductivity
The free energy Fs of the system is not only a function of the temperature T and other ordinary thermodynamic variables but a function (in fact, a functional in general since we are dealing with a system with spatial variations) of the order parameter. The order parameter of a spinsinglet swave superconductor is the pair wave function ^(x) = {ip/\(x)xpi(x))9 which is equivalent to the gap parameter A(JC) = g^ix) in the BCS model. Here the order parameter is written ¥(*) including a multiplicative constant. Let us write the free energy as Fs = Fs({x¥(x)}) 9 where such variables as T and V are and will be dropped to simplify the notation. It is assumed, in the GL theory, that the spatial variation is gradual and, accordingly, the free energy density / s is taken to be a function of *F(JC) and Y¥(x) only. Moreover, since the free energy is left invariant under gauge transformations, which change the phase of *F, and spatial rotations, / s must be a function of the combinations ^E/*(x)xP(x) and Y¥*(x) • V*F(jt) only. Actual calculations are 100
5.2 GL theory of superconductivity
101
possible only when l1^!2 and IV^FI2 are small and hence / s can be expanded in powers of these quantities. As a result, a commonly used form of the free energy in the GL theory is
Fs = Jdx{a\V\2 + ^\V\4 + c\Vy\2}+Fn,
(5.1)
which is applicable when T is close to Tc. Fn is identified with the free energy of the normal state since the order parameter *¥ vanishes for this state. First note that the order parameter *¥ = *¥ Q is realised in a uniform equilibrium state (V*F = 0). Thus one has l ^ l 2 = a/b, for which (FsFn)Q = see Section 3.2. If one rewrites ¥ / p F e  as ¥ , the free a2/2b = H2(T)/8n, energy relative to the normal state is written as
/ •
dx j¥ 2 + i¥ 4 + £2V¥ 2} ,
(5.2)
where the coherence length has been defined by £(T) = ^J~c]~a. The coefficients of the above equation in the BCS model have been obtained in Section 3.2. Since the gradient energy with the order parameter \p ^ Qiqx m u s t b e the same as Eq. (3.41), one finds = iWV6A e (T) = 0.74^(1  T/TcTl'\
(5.3)
where £0 is defined by Eq. (3.16) at T = 0. (It should be noted that here differs from the definition used in Eq. (3.16) by a factor of 7i2/6.) When the mean free path / is finite due to the presence of nonmagnetic scattering, £2 above should be multiplied by a factor _1
[(2n + l)2Vn + ! + &//)]" n=0
Let us next consider a system coupled with a static magnetic field. Since *F is the wave function of a charged pair and the free energy should be invariant under gauge transformations of the second kind (local gauge transformations), the third term of Eq. (5.2) should take the form
Although e* is arbitrary in a phenomenology, we will take the pair charge e* = 2e as in the BCS model. Supplementing the magnetic field energy
102
f dxB2/8n,
GinzburgLandau theory
one finally obtains the free energy
A)(VxA)9
(5.4)
where 0o = hc/2e is the flux quantum introduced in Section 1.1. The field configurations ^(x) and A(x) in an equilibrium state are determined by the conditions dF/S^l** = 0 and SF/dA = 0. Explicit expressions of these conditions are ^ A )
Vx(VxA)
Y
¥ + ¥F
0
(5.5)
4n
= — js
^ T T
r
(5.6)
'
w
" yvr " ^ " ^ s ( T )  l F  2 ^'
(5 7)
'
where n s (T) is the density of the superconducting component defined by Eq. (3.40), which reduces to ns{T) = 2n(l  T/Tc) in the vicinity of Tc. If the number density of the pairs ns/2 is employed, one finds that the current density (5.7) is a quantum mechanical expression for a particle of mass 2m and charge 2e. Equation (5.5) is called the GinzburgLandau equation. The analogy between this equation and Eq. (1.7) should be obvious. In addition to the coherence length £ in Eq. (5.5), there appears another characteristic length scale X in Eq. (5.6), defined by I'1 = 4ne2ns( T)/mc2, which is just the London penetration depth given by Eq. (1.12). Equation (5.6) is then rewritten as X2V x (V x A) = (0o/4rci)OF* • V ¥  VT* • ¥ )  \^\2A.
(5.8)
The ratio of the two characteristic lengths /
2
^
(5.9)
is called the GL parameter. We note en passant that 2? has a factor r\~l when / is finite, and hence K ozrf1.
5.1 GL theory of superconductivity
200
103
100
AT=Tc0T (mK) Fig. 5.1. The temperature dependence of the critical current Ic measured on a thin wire of Sn. 5.1.1 Transition in the presence of a supercurrent Let us consider, as the simplest application of the GL theory, the transition in a thin wire carrying a supercurrent. If the radius of the wire is less than both £(T) and X(T) introduced above, then *F is considered to be constant across the crosssection and the effect of a magnetic field is negligible. Therefore the problem reduces to a onedimensional problem, whose coordinate is written as x. If one writes *F = \p&kx, xp being a real constant, one obtains \p2 = 1 — £2k2 from Eq. (5.5) and accordingly, from Eq. (5.7), jx = (ns/2m)fc(l  £2k2). This supercurrent takes the maximum value k =
en*
(c2/4ne)
(5.10)
when £k = 1/^/3. If F oc (1 — £2k2)2 is looked upon as a function of j , it is found that dF/dj diverges at j c . Thus it follows that jc is the critical current in the sense that it is the maximum possible current without destroying siiperconductivity. The system makes a first order transition to a normal state if a current j > jc flows. It follows from Eq. (5.10) that jc oc (1  T/Tcf'2. Figure 5.1 is the /  V characteristic of a whisker of Sn showing the current at which the voltage across the sample appears, as a function of temperature. A close study of the data reveals that there is a deviation from the theory near T c, which is considered to be due to a thermal fluctuation effect. On the other hand, the system cannot be regarded as onedimensional at low temperatures and there is a deviation from the / 3//2 rule. In fact, the / — V characteristic of
104
GinzburgLandau theory
a thin wire is a complicated subject and is an interesting problem which cannot be explained by the simple transition above, see Section 5.6.
5.1.2 Transition in a cylinder of a thin film in a magnetic field Let us consider the transition in a cylinder of a thin film placed in a uniform magnetic field parallel to the axis of the cylinder. It is assumed that the radius R of the cylinder is much larger than k and the film thickness is smaller than X. Accordingly the magnetic field is constant over the whole sample and, since B = H, the vector potential A has only the ^component in cylindrical coordinates, which is taken as A^ = RH/2 in the film. If xy == ^eim/> i s substituted into Eq. (5.5), one finds
(Note that one is lead to the magnetic flux quantisation for a thick film since the first term must then vanish.) In the present case the integer n, which minimises the free energy, is realised of course. The deviation of the critical temperature ATC = Tc — Tco, where Tco is the critical temperature at H = 0, is therefore given by ATC/TC = 0.54m/R)2(n
 (D/^) 2,
(5.11)
which is a periodic function of the flux 0 through the cylinder. In contrast to 7c of the previous problem, there is a second order transition at Tc since the external field is related only to the phase of *F. Figure 5.2 shows the relation between Tc and H determined by the temperature dependence of the resistance, and clearly indicates the periodic dependence of Tc on the flux. The thickness of the film must be considered to explain why the maxima in Tc become smaller as H increases.
5.2 Boundary energy Let us consider the system shown in Fig. 5.3, where the plane x = 0 is the boundary between a superconducting state (x > +oo) and a normal state with an applied critical magnetic field (x —• —oo). One may choose the gauge A = (0,^4(x),0) provided that B  z. While we can find *F and B by solving Eqs. (5.5) and (5.6), we are interested in the free energy as a function of an external magnetic field, given by G = F — J dxH • B/An. Suppose ¥ = 1,5 = 0 for x > 0 and Y = 0,J3 = H c for x < 0. Then the
5.2 Boundary energy
3.60
105
3.70
Fig. 5.2. The critical temperature as a function of the flux through a cylinder of a thin film of Sn. (From [G13].)
>X
Normal Boundary Superconducting state state
Fig. 5.3. Variations of the magnetic field and the order parameter at the boundary of a superconducting state and a normal state. density of the free energy G is —H 2/8n everywhere. Therefore the difference between the free energy G of the configuration shown in Fig. 5.3 and this free energy is B
A
_oo
dx
47C V 87T
e
(5.12) Furthermore, if one subtracts / ^ dx^F* {GL equation} = 0 from the above
106
GinzburgLandau theory S
N
N
N
S
S
Fig. 5.4. The boundary energy 2£b is the free energy difference between the two states.
equation, one obtains a simple expression Eh
1
B
(5.13)
since *¥ is a solution to Eq. (5.5). It is reasonable to consider the boundary energy thus defined because the free energy difference between the two states shown in Fig. 5.4 is written in terms of E^ as 3£b — £b = 2£bOne has to solve Eqs. (5.5) and (5.6) to find E\>, which is easy if *¥ = ^(x) is chosen to be real. Let us scale lengths by X and vector potentials by 4>o/2nl, that is: x^x/1,
A+A/(
(5.14)
Then the equations to be solved are 2
(5.15) d2 A X 2 = A ¥ dx 2 The boundary conditions are *F = I, A = 0 as x —> oo and *P = 0,dy4/dx = K/S/2 as x —> —oo, where use has been made of Eq. (5.9). Let us first consider the limit K < 1 . Since A is of the order of K, the first equation of (5.15) is approximated by (l/K 2 )d 2 x P/dx 2  (1  ^ 2 ) T = 0 at x > 1 and, as a consequence, the solution is given by *F = tanh(Kx/^/2). The magnetic field penetrates into the sample to a distance X. Therefore one obtains 4V2 Eb dx(l  ¥ 4 ) = (5.16) H}/%n Let us next consider the opposite limit K >• 1, namely the London limit. The magnetic field penetrates toward the interior of the sample in the form e~x and *F is restored as 1 — e~KX. Therefore Eq. (5.13) is estimated to
5.3 CriticalfieldsHcl and Hc2
107
be ~ —3A/2. In this way, boundary energy changes sign according to the value of K. In fact, it can be proved from Eq. (5.15) that £b vanishes when K = 1/V2, see [A2]. In summary, superconductors are classified according to whether K < l/>/2 (type 1 superconductors) or K > l/>/2 (type 2 superconductors). The boundary energy E\> is negative when K > \/ yj2, in which case it is expected that the free energy is lowered if there are as many SN boundaries as possible, as shown in Fig. 5.4. Accordingly the superconducting states in a magnetic field differ significantly depending on whether they are of type 1 or type 2. There are two critical magnetic fields Hc\ < HC2 in a type 2 superconductor, as is shown in the next section, and a vortex lattice state is realised when a magnetic field intermediate between the two critical fields is applied. 5.3 Critical fields Hc\ and HC2
The magnetisation curve of a type 2 superconductor, for which the GL parameter K is greater than 1/^/2, has been shown in Fig. 1.4(b). A magnetic flux starts to penetrate into a sample as an external magnetic field H exceeds the lower critical field HC\{T\ which is less than the thermodynamic critical magnetic field HC(T). The sample makes a transition to a normal state as the field H is further increased beyond the upper critical field HC2(T), which is greater than HC(T). 5.3.1 Lower critical field Hc\ When a magnetic field is applied parallel to the axis of a long superconducting cylinder, the first flux penetrating the sample should be located along the axis of the cylinder. Therefore, the vector potential in cylindrical coordinates takes the form A = ( 0 , ^ ( r ) , 0 ) and consequently the magnetic field is given by Bz(r) = [dirA^/drl/r. (The subscript indicating the component will be omitted in the following.) Since the supercurrent is an axially symmetric vortex current, the order parameter may be put in the form *F = tp(r)em^5 where xp is real. Substituting these expressions into Eqs. (5.5) and (5.6) one obtains K2 1 r dr
\ dr )
did,
,,
\r
fn '
where A has been scaled by 2nHcl2 /fa to be made dimensionless.
(518)
GinzburgLandau theory
108
0 A:1 Fig. 5.5. The spatial variations of the order parameter \p and the vector potential A associated with a quantised flux. The above equations can be treated approximately when K > 1, in which case the scale of variation of A(r) is of the order of unity while that of \p(r) is ~ \/K (that is, of the order of k and £ respectively in physical units) as is shown in Fig. 5.5. Therefore one may put xp(r) ~ 1 in the region r > K~1. Then Eq. (5.18) reduces to
[dr2
rdr
rl) J \r
\
)
Since A should not blow up at 1 > r ( > l//c), the solution must be proportional to 1/r. Such a solution assumes the form
A
(5.19)
= nKl{r\
where K\(z) = —(n/2)[Ji(iz) + iNi(iz)] is the modified Bessel function. (Note that Ki(z) » 1/z as \z\ > 0.) When r > 1, on the other hand, Ki(r) behaves like z~r / yjr and accordingly the magnetic flux is confined within the region r <> 1. Therefore the total flux through a circle of radius R > 1 is quantised as
/
B(r)  dS = [
r
A'dl =
(=
(5.20)
Jr=R
Let us next consider the difference between the free energy G of the above configuration and Go of the configuration xp = 1,5 = 0 to find the lower critical field Hc\. If the method used to obtain Eq. (5.13) is employed again, the free energy difference per unit length is expressed as
=
(GG0)/(H2c(T)/4n)
= l I dx(l\xp\4)
1J
(H  Bf
~\
(5.21)
5.3 CriticalfieldsHcl and Hc2
109
In the region r > 1/K, where A(r) is given by Eq. (5.19), the derivative term in Eq. (5.17) is negligible and, combining it with the Maxwell equation (5.18), one may put (1 — xp 2) ~ K~2(V X B)2. If this relation is substituted into Eq. (5.21), one obtains, along with the estimate \xp\2 = 1 + 0(1/K2), Ag =  1 I cbc{(V x B)2 + B2 2HB}.
(5.22)
K J
Since one obtains from Eq. (5.18) V x (V x B) ~ —B in the same region, the sum of the first and the second terms in the curly brackets above may be written in the divergence form as V(2? x (V x B)). Then the integral is estimated as  \
/
rd
where use has been made of the relation B(r) = nKo(r) and the asymptotic form Ko(r) ~ — lnr + In 2 — y. The third term is found to be equal to —AnnH/K 2 from Eq. (5.20). Therefore one finds Ag ~ 2nK2(lnK + 0.116)  4nnK2H.
(5.23)
The smallest H which makes the above expression negative corresponds to the lower critical field. If Eq. (5.9) is used to restore the dimensions, one obtains Hcl{T)/Hc(T) = (1/J2K)\\HK
+
0.116].
(5.24)
That is, a vortex with a flux quantum 0o penetrates into the sample at H = Hc\. Note that Eq. (5.24) is applicable only when K > 1 is satisfied. Note also that xp(r) cc r in the vicinity of r = 0 when n = 1. The central part of the vortex with 0 < r <J ^, where the order parameter changes from 0 (r = 0) to ~ 1 (r ^ £), is called the vortex core. The contribution to the energy from the core is of the order of K~2. The free energy of two vortices placed at a finite distance r ^> K~1X is larger than that with r —• oo by (4>l/'16n2X2)Ko(r/7), which means that a repulsive force acts between two vortices. Due to a screening effect, however, the repulsion weakens exponentially at r > L As a result a magnetic flux suddenly starts to penetrate into a sample as H is increased above Hc\. 5.3.2 Upper criticalfieldHC2 A type 2 superconductor under a sufficiently strong uniform magnetic field is in a normal state. As H is decreased, superconductivity appears, that is, the order parameter *F becomes finite at a certain value of H, which we call the
110
GinzburgLandau theory
upper critical field HC2. At this field, therefore, *F is small throughout the sample and the effect of supercurrent is negligible. In other words, the theory may be linearised with respect to *F and one may put B = H everywhere. Let us suppose H  z and choose the gauge Ax = Az = 0, Ay = Hx. We need to consider Eq. (5.5) only, which may be written as 1 ^2
d2 dx2
21
f d \dy
= {l + co)\p,
(5.25)
where r 0 " 2 = inHX2/^.
(5.26)
Equation (5.25) is written in the form of an eigenvalue equation for convenience. A solution i p ^ O appears when co < 0. This equation is just the Schrodinger equation in the presence of a uniform magnetic field, whose solutions are the Landau orbitals. If one puts xp = &pyf(x), Eq. (5.25) becomes > ( _)ro 2 )/ = (l + a/)/
(5.27)
where _ x' This is the Schrodinger equation of a harmonic oscillator with the centre pr\ and the solution is given by U x exp(x / 2 /2r 0 2 ), /„ x D("+)/o con = {2n +
o l)(Kr0)~2l.
(5.28)
Thus coo is found to cross zero when KTO = 1 and as a result, superconductivity emerges at
H = Hc2 = fo/ln? = V2 KHC(T).
(5.29)
5.4 Vortex lattice states The phase diagram of a conventional type 2 superconductor is shown in Fig. 5.6. It had been thought that the line HC2 dividing the shaded area and the normal state in this figure corresponded to a lattice of vortex lines carrying a flux quantum. Recently, however, during research on highT c superconductors with extremely small coherence length, it was found that the line HC2(T) is not a clear phase boundary and that the vortex lattice just below the Hc2(T) line is, rather, a liquid state continuously connected
5.4 Vortex lattice states
111
H
Fig. 5.6. Phase diagram of a type 2 superconductor.
to the normal state. This is in accord with theoretical analysis which takes into account fluctuation of the order parameters (see Chapter 7 and Section 2 in Appendix A2). In spite of this recent progress, it is still necessary to know the results of the meanfield theory (the GL theory), to understand the properties of type 2 superconductors. A.A. Abrikosov was the first to study the lattice state near Hc2(T\ see [G14]. Since H ~ HC2(T), one may consider that I1?! < 1 and accordingly the nonlinear term in the GL equation is small and also that the deviation of the flux density B from a uniform Bo in the superconductor is small. Therefore *F may be approximated by a superposition of the lowest energy solutions xp oc Qlpyfo(xf) = exp
X
of the linearised GL equation in the presence of a magnetic field Boshould recall here that r^2 = 2nBo2?/(j)o. Keeping in mind that p is the centre of the Gaussian function xp, let us consider the superposition (5.30) l=oo
This form of
,y) • exp[i(27r/a)(y/ro + b/2a)].
(5.31)
(In fact, 4> c a n be written in terms of Jacobi's $ function and the above periodicity is a direct consequence of this fact.) Therefore xp is periodic, if we disregard its phase, with the unit cell shown in Fig. 5.7. The area of the unit cell (2n/a)ro x aro = 2nrl is pierced through by exactly a unit flux quantum
112
GinzburgLandau theory
(0,a)
0
x/r0
Fig. 5.7. The unit cell of a flux lattice.
Fig. 5.8. The contour lines of \
and
5.4 Vortex lattice states
113
above and as a result one obtains the minimum value (
"2)
where the physical dimensions are recovered. One finds from the above expression that the lattice giving the smallest PA is most stable. This is found to be the triangular lattice, for which /?A = 1.16. Since —AnM = Bo — H, the magnetisation is given by M = (Hc2  H)/[4TZ(2K2
 l)j8 A ],
see [A2] for details.
5.4.1 Quasipavticle excitations associated with a vortex Figure 1.6 is an STM (scanning tunnelling microscope) image of a vortex lattice obtained by scanning a surface perpendicular to the applied magnetic field. The sample is a layered crystal NbSe2 (T c = 7.2 K, K ~ 9) and a magnetic field of 1 T was applied perpendicular to the layers. Since a tunnelling current between the needle and the sample surface is observed in the STM, this system can be treated in the same way as the tunnelling current between a superconductor and a normal metal studied in Section 3.4. Since a vortex lattice state is not spatially uniform, however, the quasiparticle spectrum changes with the nonuniformity and thus an image such as Fig. 1.6 is obtained. Theoretically a spacedependent quasiparticle density of states \un(x)\2  \vn(x)\2]8(co  con\
(5.33)
necessary to find the tunnelling current, may be obtained from the solutions un(x) and v^(x) to the Bogoliubovde Gennes (BG) equation (see Section 3.5). Let us consider a superconductor with K > 1, as before, whose impurity effects are negligible. An external field H is taken to be sufficiently smaller than HC2 and accordingly it may be assumed that the lattice constant of the vortex lattice a is larger than £ and that each vortex line is independent of the others. Consider, therefore, a single vortex along the zaxis and introduce the cylindrical coordinates (r,
114
GinzburgLandau theory
also takes the form A = A(r)e"^ with A(r) real. Therefore one puts un(x) =
M/fc (r)e
fc+i
^
where / is an integer and the radial quantum number is omitted. Substituting the above expressions into the BG equations, one obtains [D + l2/r2 — fep 2 sin 2 a — 2ms]uik(r) + 2rnA(r)vik* (r) = 0 [D + (/  l ) 2 / r 2  kF2 sin 2 a + 2me]vik*(r)  2mA(r)uik(r) = 0,
where D = r  1 d/dr(rd/dr) and 2m8p — k2 = fcpsin2a. To be more precise, one has to solve the above equations simultaneously with the gap equation (3.95). We will be content ourselves, however, with solutions u9v*9 given in Fig. 5.5, which are obtained under the assumption that A(r) is proportional to xp(r).
Let us first note that Eq. (5.34) is left invariant under the substitutions 8 —> —8, / —> — / + 1 and u —> —v*. (All the negativeenergy eigenstates are occupied at T = 0.) Therefore one may assume s positive and study only the states with / = 1 since they give the lowest energy. One may assume fcpsin2a > 2mA since 8p > A. Then one finds from Eq. (5.34) that the approximate forms of the solution are u(r) = fu(r)Ji(kFr sin a) and v*(r) = fv(r)Jo(kFr sin a), where the envelope functions fu and fv vary with the characteristic scale £. Here the indices of u and v* are omitted. One expects that there are scattering states with s > Ao and bound states with s < Ao. In fact, there is a bound state with the wave numberfcpsin a localised near the centre of the vortex with extension £, whose energy eigenvalue is 8 ~ (7c/4)(Ao/£F)g(a)/sina, see [Cl]. Here g(a) is a slowly varying function of order unity. Thus there are almost gapless excitations localised near the vortex core and accordingly the density of states (5.33) varies spatially. A single vortex has been considered so far. The density of states due to low energy excitations in a vortex lattice is larger along lines connecting the vortex with the nearest neighbour vortices. This has been confirmed by the STM images. It is interesting to note that a sixfold symmetry of a NbSe2 crystal around the oaxis is also seen in the STM images of a vortex. 5.5 Timedependent GL equation
Let us generalise the GL equation introduced in Section 5.1 so that we may study phenomena in which the order parameter *F depends on both space and time. That is, assuming that temporal variations are slow enough, one
5.5 Timedependent GL equation
115
introduces a time derivative term in Eqs. (5.5) and (5.6). Unlike static cases, this extension is possible only under limited conditions. As is shown below, however, there are interesting applications of the timedependent equation, the socalled TDGL equation. The order parameter A(l) at a spacetir point 1 = (xi,£i) is related to A at nearby points. (Here the BCS model is employed and hence A is taken to be the order parameter.) When A does not change, namely when A = A(l) at any nearby point, the rule by which A's are related is just the gap equation A(l) = g/(A(l))A(l), where the gap in / = JV(O) / d ^ tanh ^ is A(1). If there is a variation SA(2) = A(2) — A(l) between the gaps at 2 and 1, we can express this relation by taking the effect of the variations into account, as = 7A(1)  g J d2{Kn(l
2)SA(2) + K12(l,2)<SA*(2)},
(5.35)
where we have only kept terms linear in dA, assuming the variation (5A(2) is small. Causality restricts the ^integration within the range ti < t\. The second term of Eq. (5.35) represents the response to variations dA and dA* of the mean fields. This term yields the linear response equation (3.48) with Q and C replaced by the meanfield variations (5 A and <5A*. It is sufficient to consider the case A(l) oc e1^1, that is, SA(2) = [e1^2"1) — 1] A(l), for the present purpose, where q = {q,co). If this is the case, Eq. (5.35) becomes = g[Ku(q)
~ Xn(O)]A(l)  g[Kl2(q)  Kl2(0)]A*(l). (5.36) In a superconductor without impurity scattering, one obtains
Kn(q) (1  n+  n_)
CO + 8+ + £ _
CO + £ + — S
CO — 8+ — 8_ /
CO — £ + +
£
(5.37)
where the subscripts + correspond to 6 C + ^ F # * ^ A a n d co is assumed to have a small imaginary part +i(5. Provided that K may be expanded in powers of q2 and co and after the replacements q2 —> —V 2 and co —> id/dt, Eq. (5.36) turns out to be the partial differential equation we are seeking. Although the denominator of the first term of Eq. (5.37) may be expanded in powers of co when co
116
GinzburgLandau theory
possible. If these conditions are satisfied, one obtains K22 °c A2, which is thus negligible, and one simply considers the expression 2 7_i x [(2£ + qvFi* + co + id)'1 + (2<^ + qvF/i co
i5)~l]
(5.38)
in which A is set equal to 0. Since v?q > co, the imaginary part is dominant in the term proportional to co in Eq. (5.38). Finally one obtains
*„,„,»> Kll(0,0,, N,0, { (A) ^ _ ( f ) ™ ± t }
(3J9)
The second term of the above equation is the gradient term obtained previously while the first term corresponds to the time derivative — x(dx¥/dt) in the GL equation. Comparing the first term with the gradient term, we determine the relaxation time x
V
(5.40)
This result is in agreement with the expectation that the order parameter relaxes towards a free energy minimum according to the equation
where FHl/An is identical with F in Eq. (5.4). The relaxation mechanism is considered to be the scattering of thermally excited quasiparticles by the timedependent mean field. It should be noted that x remains unchanged while the coherence length £ changes by nonmagnetic impurity scattering. As was noted in Section 3.6, the order parameter *¥ has a phase factor 2ifit Q e v e n j n a n equilibrium state, where \i is the chemical potential of an electron. Therefore, by noting that the chemical potential changes as \x —> ji + ecj) in the presence of a scalar potential 0, one arrives at a correct expression by making the following replacement d/dt + d/dt + 2i(/j + e
V V
+  ¥  ¥ = 0.
(5.42)
The TDGL equation of this simple diffusion type is valid only in a very narrow temperature region near Tc because of the group velocity anomaly
5.5 Timedependent GL equation
111
of quasiparticles and the divergence of the density of states at the gap edge. In a gapless state due to magnetic impurity scattering studied in Section 4.6, the relaxation time T is replaced by T P, in which case the theory has a wider applicability. This suggests that the dissipation term becomes larger if there are pairbreaking interactions. In reality, however, the contribution of inelastic scattering, due to an electronphonon interaction, to the relaxation term is large and it is shown that the first term of Eq. (5.42) should be replaced by 211
(2T E A) 2 ]
(5.43)
Here TE is the relaxation time due to inelastic scattering and it is known that takes a large value, where Ae is the mean field at an equilibrium state. For example the maximum value is 17 for Pb and 47 for Sn, see References [D7] and [D8] for details. Another case where a differential equation for *F may be obtained is a system at T ~ 0 with little thermal excitation, in which case such physical quantities as K in Eq. (5.37) are expanded in powers of co/Ao and qv?/Ao. As a result, one obtains a wave equation, containing an operator [d2/dt2 — (fp/3)V 2], whose solutions include a NambuGoldstone mode with a spectrum co = qvY/s/3. However, time variation of the order parameter *F is in general accompanied by a density change dp oc i(*F*d*F/d£ — ^Vd^/dt) as can be seen by studying the density response to change of pair mean field. Accordingly this mode is identified with plasma oscillation. In the TDGL theory we assume, in addition to the restrictions already mentioned, that quasiparticle excitations are always in a local equilibrium state corresponding to ^(x, t). Therefore there are some cases that defy description in terms of the TDGL equation. As was pointed out in Section 3.2, the charge density Q* associated with quasiparticle excitations does not vanish if the system is in a nonequilibrium state so that the particlehole symmetry is violated. Then the pair contribution Qs deviates from the equilibrium value ens and, as a result, there appears a state called the charge imbalance. An important example is a collective mode called the CarlsonGoldman mode. If there is a wave associated with the pair charge density Qs, the charge Q* oscillates out of phase to maintain charge neutrality. Although quasiparticle excitations decay by scattering, the above collective motion is near a welldefined mode with a phase velocity [(ns/n)(4T/nA)]1/^?/y/3 T ~ Tc since Qs is small there. Although this mode is similar to the second sound in superfluid 4 He, where the superfluid and the normal fluid oscillate out of phase, the present mode is not an entropy mode; the restoring force
2TEA C
118
GinzburgLandau theory
of the wave motion comes from the change of the pair chemical potential, see [D7, D8] for details. 5.6 Applications of the TDGL equation 5.6.1 Sliding of vortex lattice A vortex state appears in a type 2 superconductor when an external magnetic field H satisfies Hc\ < H < HC2, as was noted in Section 5.4. It is expected that the Lorentz force will act on the vortex if a current flows perpendicular to the flux. In fact, in an ideal system without vortex pinning centres, vortex lattice sliding appears, leading to energy dissipation caused by an applied electric field. Let us demonstrate this with the TDGL equation. Suppose a scalar potential 4> — —Ex giving a uniform electric field E is applied parallel to the xaxis, along with a vector potential A = (0,ifx,0). Then Eq. (5.42) becomes T (j
 2ieEx\ ¥  £2d2x¥/dx 2
?{d/dy  ilnHx/^o)2^ *? + l^l 2 ^ = 0,
(5.44)
where physical quantities are equipped with proper dimensions for later convenience and the chemical potential /n has been included in the phase. Assuming that *F depends on time as ^(x,y — vt), the first term of Eq. (5.44) becomes —w(d/dy + lieEx/v)^. Accordingly if the choice v = —cE/H is made so that the Hall voltage cancels the electric field £, this term and the third term may be combined. Therefore one obtains a vortex lattice solution sliding along the yaxis with velocity v = cE/H, if one superposes functions xpp = exp
i
rzcE r u y p[y + n,* o\ jpHJ 2 \r2 2H?
as in Eq. (5.30) within the linear approximation introduced in Section 5.4. Let us find the spatial average of the current density j ^ along the xaxis with the present solution. Since all xpp contain a phase factor exp(icr£x/2^ 2 if) proportional to x, one easily finds eCT
W4r,
(545)
where \
when H ~ HC2.
5.6 Applications of the TDGL equation
20
40 60 KfiA)
80
119
100
Fig. 5.9. The I — V characteristic of a whisker of Sn (length 8 x 10 2 cm and cross section 1.93 urn2). An arrow pointing up (down) denotes the data when a current is increased (decreased). AT = Tc — T. (From [G15].)
Even when the TDGL equation is not applicable, there is vortex lattice sliding, and hence energy dissipation, in an ideal system supporting a current perpendicular to a magnetic field H. In this respect, it is not adequate to call the state 'superconducting'. In reality, however, the vortex lines are pinned by various defects (pinning) and the supercurrent is stable in so far as the pinning force balances the Lorentz force. Superconducting magnets are possible because of this mechanism. Due to a low electron density or other reasons in the vicinity of a defect, the condensation energy of superconductivity is locally suppressed. The vortex energy is then lowered if the vortex core stays where the condensation energy is small. If the defect size d is larger than the coherence length, the energy is of the order of H^2d/Sn. A distribution of these pinning centres will fix the whole vortex lattice since a vortex lattice has stiffness due to interactions between vortices. See [C2, vol. II] and [E6] for creep of lattices in the presence of pinning. 5.6.2 Phase slip oscillation (PSO) The critical supercurrent density jc of a thin wire has been obtained in Section 5.1. Related experiments have been carried out with a whisker crystal or a microbridge of such metals as Sn and In. Figure 5.9 shows an example of an / — V characteristic thus obtained, from which one finds that the transition from a superconducting state (V = 0) to a normal state does not take place suddenly at j = jc. Instead the voltage V increases stepwise
120
GinzburgLandau theory «
T
»
(a)
0
V
(b)
Fig. 5.10. Winding of the phase % of *F in the presence of a potential difference V.
over a considerable range of applied current /. The first step is considered to be important and we will concentrate first on this phenomenon. Suppose a thin wire of length L connects two large superconductors as shown in Fig. 5.10(a). If the electric field is uniform along the wire and the potential difference is finite, the phase of ¥ = *F e1* is given by X(x, t) = —2eVxt/L and therefore the supercurrent increases in proportion to vs(x, t) = —eVt/mL. Accordingly the system cannot be in a steady state. As v s increases, *F decreases and there appears a region where *F is smaller than the average. The velocity vs in this region then further increases, which leads to a further decrease of *F and eventually *F vanishes, see Fig. 5.10(b). The phase jumps by 2n at the same time, which implies that the phase difference created by the potential difference decreases by 2n. Then vs becomes smaller and *F is restored. Since the jump in the phase is 2TT, *P at the two sides of the zero point are smoothly connected. This unwinding mechanism repeats itself. If the phase jump takes place at intervals of i ps , the equality of the winding by 2eV per unit time and the unwinding described above leads to the Josephson relation 2eV = 2TZ/TPS, from which one obtains the average potential difference. This periodic phase jump is called phase slip oscillation (PSO). Early theories, which explained the / — V characteristic near jc using PSO, assumed the phase slip but later it was shown that PSO naturally arises as a solution to the TDGL equation. Since there appears a point where *F vanishes and a normal state sets in, to observe the charge neutrality, that is, the contribution j n of the normal component to the current, one has to consider thermally excited quasiparticles. Note that a timedependent electric field may exist in a
5.6 Applications of the TDGL equation
121
\Wt)\
0.8 0.6 0.4
0.40
0.2
0
*x (a)
(b)
Fig. 5.11. (a) The spatial profiles of *F and 0 when *F(0,£) takes a minimum and a maximum value in a PSO cycle. The coordinate x = x/6d is measured from the phase slip centre, (b) The temporal variations of *F and j n . (From [G16].)
superconductor although a static field does not. One can expect that j n at T <> Tc obeys the same Ohm's law j n = anE as in the normal state. Since a quasionedimensional system is under consideration, one may put A = 0 in js given by Eq. (5.7). Accordingly the total current is 2m
dx
n
dx9
(5.46)
where x(x, t) is the phase of *F and (f)(x, t) denotes the scalar potential. The problem is to find solutions of the TDGL equation T I
IT
CXL
(5.47)
under the condition that the current j given by Eq. (5.46) is constant. (It is sufficient to use Eq. (5.42) for qualitative discussions although Eq. (5.43) must be employed to compare the theory with experiments.) One first notes that there are two uniform solutions: the normal state solution *F = 0, (j> oc x; and the superconducting solution *F = const., x °c x, 0 = 0. Although the first of these is stable for j > j c , there exists a third solution corresponding to PSO, which is more stable than the second solution in a certain region j \ < j < jc This solution appears as a limit cycle when a relevant initial condition is chosen and, in practice, is analysed numerically. In an actual calculation, a periodic boundary condition over an interval —d/2 < x < d/2 is imposed and the point x = 0 is taken to be the phase slip centre (PSC) where the order parameter *F vanishes periodically. Figure 5.1 l(a) shows the spatial profiles of I1?! and at moments when 1^(0, t)\ = 0 and 1^(0,01 = max. Figure 5.1 l(b) shows, on the other hand, the time dependences of *F and j n at the phase slip centre x = 0. In practice the
122
GinzburgLandau theory
PSC appears at the most 'vulnerable' point on a thin wire. The jump in the I — V characteristic is understood as a transition from the second solution with (j) = 0 to the PSO solution with (j) ^ 0. The successive appearance of steps as j is increased is attributed to the creation of many PSCs on the wire, see [D8] for details. Phase slip is also possible when the temperature is close to T c, if points in a normal state appear due to thermal fluctuations. According to this mechanism, the resistance is proportional to the Boltzmann factor where AF ~ ^S(H^/Sn), S being the cross section of the wire.
5.7 Fluctuations in a superconductor
We have studied the meanfield theory so far, in which only the statistical average of the order parameter *F is considered. This is, of course, an approximation and there are phenomena which cannot be understood within this framework. Among these, the most important is the critical phenomena near Tc in which order parameter fluctuations play a crucial role. Let us restrict our discussion to superconducting fluctuations in a normal phase at T > Tc. Therefore ^(x) appears only through thermal fluctuations and, as a result, a state with the order parameter profile ^(x) is realised with the Boltzmann weight exp(—/JF), where the free energy F( x¥(x)) is given by Eq. (5.4). The contribution of thermal fluctuations to thermodynamic quantities is derived from the partition function Z = $>xpH8F0F(x))].
(5.48)
Although F has been written in the above as if it were a functional of only, to be more precise, it also depends on the fluctuation bA of the gauge field A. The fluctuation bA is of the second order in *F, however, as can be seen from Eqs. (5.6) and (5.7), and accordingly the magnetic energy in F, induced by the fluctuation of VP, is of the fourth order in *F. Note also that the magnetic energy is proportional to K~2 in a system with a large GL parameter (K > 1). Therefore one may neglect bA in the Gaussian approximation, in which terms are kept up to the second order in *F, or in a system with K >> 1. Let us consider, as the simplest example, fluctuations in a uniform system without an external magnetic field. Since the dependence of physical quantities on E = T/Tc — 1 is most important in a critical phenomenon, one
5.7 Fluctuations in a superconductor
123
writes
pF = p I dx (
(5.49)
where P = PH2(T)/4ne, ^ = si;2 and the Fourier transform of ^(x) is denoted by xpk = ipik + iV2/c> where xpik and xp2k are independent fluctuation variables for each k. The fluctuation amplitude is small, unless s is very small, and thus the Gaussian approximation which neglects *F4terms is applicable. Then the statistical average of the fluctuation is obtained from
=
p pQ
II // ^
p(£02k2 + 8) x (\plk2 + \p2k2)}
J J— 0
(550) k
Among contributions to the specific heat, for example, the term which diverges as s —• 0 is C F = kB ]T(£o2fc2 + s)2 x (kB/Zod)s(d4)/2,
(5.51)
k
where d is the dimension of the system. Therefore CF diverges as e" 1 / 2 as T —• Tc in a threedimensional sample. Let us recall that in the meanfield approximation there appears merely a jump in the specific heat at T = Tc. The coefficient in front of s" 1 is, however, very small compared to the electron specific heat N(0)k^Tc in the normal state and hence Cp may be negligible. However the contribution of this term to the electrical conductivity is sizeable as will be shown below. We note that {VkWkn=hk~p\tfk2 + zTl
(5.52)
in the same approximation, from which the correlation function for *¥ is obtained as
V ) ) = [47c^ 0 2 xJc']" 1 expHxa//a
(5.53)
This shows that the correlation length of the order parameter diverges as that is, as s~1/2 as T > Tc. 5.7.1 Electrical conductivity due to fluctuations Since a local superconducting state is created and annihilated continually even at T > Tc, these fluctuations are expected to manifest themselves in
124
GinzburgLandau theory
the electrical conductivity. It is convenient to employ the Kubo formula in the classical approximation to calculate this quantity. This corresponds to the imaginary part proportional to co in the approximate form of Eq. (3.48) with (ico < 1. One thus obtains rco
oXx{q, co) = P /
(jx(q, t)jx(q, 0)) cos cot dt,
(5.54)
where
Mq, t) = ~ YK2kx + qX)v*k+q(t)yk(t),
(5.55)
since the external field is set equal to zero. The symbol (• • •) denotes the statistical average with respect to the fluctuations. One has to know the time dependence of xpk, namely how the fluctuation ¥(*) relaxes to 0, to evaluate Eq. (5.54). A frequently employed assumption is that ¥(*, t) obeys the simple TDGL equation (5.42), which we also assume here. Accordingly \pk in the Gaussian approximation becomes
e)f Ao],
(5.56)
where TO = TC/8/CBTC in the absence of impurity scattering (/ > £o). The conductivity a(q,co) is found if Eqs. (5.55) and (5.56) are substituted into Eq. (5.54) and then (Iv^l4) = 2/T2(<^fc2 + s)~2 is used. The direct current conductivity a(q = 0, co = 0) is found to be
where d stands for the dimensionality of the system and the relation ns/2m = H^2/n has been used. The result of the integration yields
s
i
(5 58b)
«mm
<5 58c)


In the above equation, / is the thickness of a thin film while S is the cross section of a thin wire and it is assumed that /, y/S < £o It is interesting to note that the conductance in Eqs. (5.58b, c) is expressed in terms of the elementary unit e2/h only.
5.7 Fluctuations in a superconductor
125
15 T
o Ga
f
D []
10 " ^
dL cL 5 • < L
T rc
Q
Ga
* Ga
• Bi • Bi * Bi
1720 1020 180 2240 470 160 210
0.01 r/jTci
0.02
Fig. 5.12. The conductance due to fluctuations in a thin film of 1 cm x 1 cm with thickness d. The solid line is the prediction by the AslamasovLarkin theory. (From [E4].)
'<•> (a)
(b)
Fig. 5.13. Contribution of fluctuations (wavy lines) to conductance a. (a) The AL term, and (b) the MT term.
Thus far, we have employed the Gaussian approximation where the ^ 4 term in F has been neglected. As the temperature T approaches Tc and s becomes small, however, fluctuations grow so large that this approximation is no longer applicable. Then the system is in the critical region where
126
GinzburgLandau theory
thermodynamic quantities blow up with anomalous powers of s. The order of magnitude of s under which the system is in the critical region is called the Ginzburg criterion. Let us consider the averaged order parameter *F = y Jv x¥(x)dx over a volume V ~ £3 since typical fluctuations have a linear size ~ £. The statistical average of the modulus of *F is obtained from
1
1
where Eq. (5.53) has been used. When the above average becomes of the order of s, one finds that the fourth order term (l^l 4 ) ~ (l^l 2 ) 2 is of the order of e(*F2), which indicates that this term is not negligible. Thus it follows that the condition for the system to be in the critical region is (P€Q)~~2 ^ e, which may be rewritten as
o3r2£s.
(559)
For an ordinary superconductor, the left hand side is less than 10~~12 and the critical region is negligibly small, e is of the order of 10~2 even for a highTc superconductor for which £o is small. A different situation appears in a high magnetic field as will be discussed in Chapter 7. It should be remarked that fluctuations are quite important in superfluid 4 He in contrast with superconductors. This is for two reasons: the length £ defined by Eq. (1.9), which corresponds to the coherence length £o, is of the order of the interparticle distance; and since the condensation energy for one particle is ~ /CBTC, the left hand side of Eq. (5.59) is (nft 3 ) 2  1.
(5.60)
Accordingly properties near the critical point deviate significantly from the meanfield predictions. A good example of this is the temperature dependence of the specific heat C shown in Fig. 1.1 (b), where C is observed to diverge remarkably at the critical point due to critical fluctuations.
6 Superfluid 3He
Superfluidity in liquid 3 He, discovered in 1972, is due to pairing, as is the case for superconductivity in ordinary metals. However, the pair is in the 3 P state so that a new aspect of superfluidity appears with internal degrees of freedom. It offers quite an interesting real example of 'spontaneous symmetry breaking'. This aspect will be emphasised in the following discussion.
6.1 Fermi liquid 3 He
A 3 He atom is a fermion with nuclear spin 1/2. Although 3 He gas liquefies at low temperatures due to the weak van der Waals force, it does not solidify even at T = 0 unless the pressure exceeds 33.5 atm (3.4 x 106 Pa) as shown in the phase diagram (Fig. 6.1 (a)). While Bose liquid 4 He becomes superfluid at about 2K, 3 He is Fermidegenerate at less than Tp ^ O.IK and shows the properties of a normal Fermi gas. For example, the specific heat and the susceptibility are proportional to T at T < Tp. It is only at an ultralow temperature in the mKregion that the system undergoes a transition to the superfluid state. Figure 6.1(b) is the phase diagram showing the superfluid phases with variables T,P and external magnetic field H in the mKregion. It should be noted that there are two thermodynamically distinct phases called the A phase and the B phase even at H = 0, and that for H ^ 0 the Ai phase appears. Moreover, the transition between the A phase and the B phase is of the first order, which suggests that these are ordered phases with different symmetries. The appearance of superfluidity has been suggested by the specific heat jump, observation of the fourth sound propagating in the 'super leak' of packed fine powder, the anomaly in heat conductance and, above all, the shift in nuclear magnetic resonance frequency (see Section 6.4). 127
Superfluid 3He
128
= 28.92 atm 0.32 K
(a)
critical point P c =1.15atm 'liquid/ \7 C = 3.32K 'gas
33.5 atm
phase
melting plane (b)
zerofieldplane 1 2 3 Temperature (mK)
Fig. 6.1. (a) The phase diagram of 3 He at low temperatures, (b) The phase diagram of liquid 3 He in the mKregion. There appear three distinct superfluid phases denoted by A, Ai and B.
<8
Xi
o
CX O CO —
i rv X U *
Fig. 6.2. Temperature dependence of the specific heat with a magnetic field 0.88 T under melting pressure. Jumps are seen in the transition from the normal phase to the Ai phase (Ai) and that from the Ai phase to the A phase (A2). (From [G17].)
The existence of the Ai phase in a magnetic field is deduced from the specific heat measurement (Fig. 6.2) for example. The starting point of the theory of the superfluid state in liquid 3 He is, as in the case of superconductivity, the model for the normal state. In addition to the van der Waals force, there is a hard corelike repulsive
6.1 Fermi liquid 3He
129
potential between 3 He atoms and, as a consequence, the interaction can not be considered weak. This should be evident if one compares the interatomic distance 2.88 x 10~8 cm, at which the repulsion starts to operate, and the mean interparticle distance (under saturated vapour pressure) f = 3.49 x 10~8 cm in the liquid state. In fact, liquid 3 He undergoes a phase transition to a bcc crystal due to this repulsive force if the particle density is increased by 5% under applied pressure. It should also be noted that the specific heat and the magnetisation calculated within the free particle model greatly deviate from the observed values. In spite of these facts, the lifetime of a quasiparticle excitation dressed by interactions is rather long owing to the surrounding degenerate Fermi sea. Accordingly the physical properties at T < Tp may be well described by a theory based on quasiparticle excitations, the socalled Landau Fermi liquid theory, see also [A6]. Since the critical temperature Tc of this superfluid is of the order of Tp x 10~3, similar to that for superconductivity in a metal, one can naturally study the system on the basis of this theory. In the Fermi liquid theory, the quasiparticle is also specified by the momentum p and the spin a, hence being in onetoone correspondence with the original particle. The normal ground state of the system is represented by the Fermi sphere with radius fcp = (3n2ri)1^ and an excited state is specified by the deviation Snp(X of the quasiparticle distribution from the Fermi sphere. It is assumed, furthermore, that not only direct interaction but interaction via surrounding particles (i.e., polarisation of the surrounding particles) acts between excited quasiparticles. The effective interaction is customarily separated into spinindependent and spindependent parts as Hint = 2
(6.1) To be more precise, V® and V^ are the irreducible vertex parts of the channel indicated by an arrow in Fig. 6.3(a) and given by the scattering amplitudes of quasiparticles on the Fermi surface. Equilibrium properties including the linear response are obtained from the generalised meanfield approximation for the effective interaction above. Thus, one uses the Hamiltonian
PA
^
{ V }
p,p> 1=0
tr (a^paap)d(tr a^oa^)} + (interaction with external fields), (6.2)
Superfluid 3He
130 P
+
P
<1
p+q
p'+q (a)
(b)
Fig. 6.3. Interparticle interaction.
where £p(X = p2/2m* — JJL. The symbol 5( • •) represents the deviation of a physical quantity from the mean value due to external fields, for example, in an equilibrium state and is a function of momentum and spin. One usually considers the quasiparticle density, the spin density or the momentum density as the physical quantity of interest. The ordinary HartreeFock term independent of external fields is considered to be renormalised into the chemical potential /a. The quantities Fj and p\^ made dimensionless by 2iV(0) are called the Landau parameters. Suppose the chemical potential is changed by dfi. The particle density then changes by Sn = ^Zp^8(nPA), which leads to a quasiparticle energy lPa = Zp« &H + F^5n/2N(0).
(6.3)
Accordingly it follows that
where /£ is the Fermi distribution function and dfp/d^pa may be approxi mated by a S function localised at the Fermi surface. Thus it follows imme diately from
df° that the compressibility is given by 1 +r0 where KQ = 2N(0)n~2 is the compressibility of a free Fermi gas. As is seen from Table 6.1, FQS^ takes a large value due to the pressure from the hard core, suppressing density fluctuation.
6.1 Fermi liquid 3He
131
Table 6.1. The molar volume, the Landau parameters at T < Tc and the critical temperature of liquid H \e p n x 1021 k¥ x 107 V 3 (cm 1 ) m /m (bar) (cm ) (cm"3) 0 15 34.4
36.84 28.89 25.50
16.3 20.8 23.6
7.84 8.49 8.87
2.80 4.28 5.85
f (s)
r(s)
F 3
o
5.39 9.30 0.6951 9.85 41.73 0.753 14.56 88.47 0.753
TAB
(mK)
(mK)
0.929 2.067 2.491
1.933
Similarly, if a uniform magnetic field B ( z) is applied, one obtains (6.6) corresponding to Eq. (6.4), where d(sz) = ^2PAo^S(npa) and y/2 is the magnetic moment of a 3 He atom. Therefore the susceptibility is
1 = Y^y
(67)
which shows that the correction to Xn = y2N(0)/2 is given by F^. The parameter F^ is negative and its magnitude is rather large. Thus it is found that liquid 3 He is easily spinpolarised which is also due to the hard core repulsion. Suppose finally that one references to a frame moving with a constant velocity —v. The quasiparticle energy becomes £ pa + p • v under the Galilei transformation. One only needs to replace dju above by p • v to recover the original Fermi sphere from the Fermi sphere in the moving frame. That is,
One obtains, by making use of the above equation, an expression / = mnv for the current / = ^2PApSnpa. On the other hand, one should have / = nmv since all the particles move with velocity v if seen from the moving frame. Therefore the effective mass is related to F, as (6.8)
132
Superfluid 3He
The parameter F[S^ also appears in the expression for the specific heat. The values of these Landau parameters are listed in Table 6.1, from which one concludes that the interaction is by no means negligible. 6.1.1 Pairing interaction It can be seen from Eq. (6.2) that Landau parameters give the magnitude of the effective interaction when q ~ 0 in Eq. (6.1). This corresponds to the forward scattering amplitude with a small exchange momentum q from the viewpoint of a twoquasiparticle scattering, see Fig. 6.3(b). In contrast with this, it is that part of an interaction with rather large q, such that q <> 2/cp, that leads to superfluid pairing. Therefore it is not easy to estimate the pairing interaction qualitatively from the magnitude of the parameters F^ and F\*\ (See [B7] for numerous attempts to do this.) In qualitative discussions below we keep the above points in mind. It was shown in Section 2.1 that an interaction can be separated into V^ acting in spinsinglet pairs and V^ acting in spintriplet pairs in the absence of spinorbit coupling. This decomposition and that into symmetric and antisymmetric parts V^ and V^ in Eq. (6.1) are related as follows. Since the projection operators onto a singletpair and a tripletpair are px = (1  G . a1)/A and P 3 = (3 + a • a1)/A respectively, one has Px+P3 = l and a • a' = P3 — 3P\. If these relations are used in Eq. (6.1), one obtains (6.9) 7(0) = ^(s) +
v^\
It is expected that the dominant contribution to pairing is provided by the component / = 0. (The angle with which the Landau parameters are decomposed into partial waves is of course different from that used in the decomposition of the pairing interaction into the swave, pwave and so on.) We now note that F[^ takes a large negative value. It follows from Eq. (6.9) that if V^ is negative, it works as a repulsive force for a spinsinglet pair and an attractive force for a spintriplet pair. One may then presume that this is related to the fact that the triplet pwave pairing is responsible for the superfluidity in 3 He. Conversely singlet swave pairing cannot be expected since FQ takes a large positive value. In fact, right after the BCS theory was expounded there were theoretical predictions on the nature of the pairing in 3 He and leading opinion favoured either dwave or pwave pairing. It is established nowadays that the spintriplet pwave pairing is responsible for superfluidity in 3 He as is shown below. The problem of the interaction is considered again in Section 6.4 in the context of the strong coupling effect.
6.2 Superfluid state of3He pairs
133
6.2 Superfluid state of 3 He pairs The weak coupling theory for the superconducting state with XS pairs has been studied in Chapter 3. Let us repeat the same analysis here for 3 P pairs. It has already been shown that the order parameter for a spintriplet pairing is expressed as *F^ = A^fyio^oi, where A^(k) transforms as a vector under a spinspace rotation. Let us assume here that the / = 1 component (i.e. pwave) is the most attractive force when the interaction is decomposed as in Eq. (2.12). Therefore one has
V(k,k') = 4ngl J2 Y m=l
= 3gl(k X fe; + kyk'y + kZk'z\
(6.10)
where k = k/\k\, Y^1 = ^/W^$x ± iky\ Y? = ^J/A^ikz and gl stands for \V\\. The order parameter A^(k) may be considered to be a function of the direction of k only and expanded in terms of the pwave orbits Y™(k) or kj (j = x, y, z) as Ap(k) = Y, AimYim(k) = ^A.jkj m=—1
(6.11)
j
for the interaction (6.1). Representation in terms of kj will be mainly used in the following. Clearly the triplet A^ (j = x,y,x) with a fixed index ji transforms as a vector under a rotation in momentum space. Accordingly the order parameter of a superfluid state with 3 P pairing is given by 3 x 3 A^/s with the spin component ji and the porbital component j . Moreover each A^j is a complex number since it is a pair wave function. In contrast with a ! S pairing, for which the order parameter is a single complex number A, it is expected from the above arguments that the superfluidity with a 3 P pair can have far more diverse phases. Given an ordered state represented by {A^}, it transforms to a different ordered state under the above mentioned operations, namely a spinspace A
rotation, a rotation in A>space and multiplication by a common phase e1* (0 < x < 2TT) called a gauge transformation. The normal state is invariant under these transformations since the Hamiltonian does not contain the spinorbit interaction. That the system is in an ordered state implies, therefore, the breaking of the symmetries these operations represent. Since the broken symmetries are rotations in two threedimensional spaces and change in phase, the symmetry under consideration in the superfluid phase in 3 He is G = SO3 x SO3 x [/(I) x T (6.12)
134
Superfluid 3He
in terms of the group theoretical symbols. Here the timereversal operation T is also included. The action of T on the order parameter of a triplet pairing is
It should be noted that the symmetry operations in Eq. (6.12) are not mutually independent. All the states of liquid 3 He represented by Eq. (6.11) share the common critical temperature Tc as was mentioned in Chapter 2. There is only a single class at Tc in this sense. Strictly speaking, there is a magnetic dipole interaction Hj), to be introduced in Section 6.4, which is a form of spinorbit interaction, and the Hamiltonian is not invariant under separate rotations in momentum space and spin space. Accordingly different states have different Tc if Hj) is taken into account. This splitting of Tc is, however, so small (~ 10~7 K) that it has not yet been observed and this effect is neglected in the present and the next sections. In neutron matter, due to a strong tensor force, the J = 2 pairing state, 3P2 superfluid in particular, is thought to have the highest Tc. Liquid 3 He is classified into many different states at T < Tc. The symmetry G is not completely broken in an ordered state in general and some symmetry corresponding to a subgroup H of G may be left intact. In other words, it is the symmetry of the coset group G/H that is broken in many cases. The set of states constructed by operating G/H on one of these states form a class. Naturally all the states belonging to a certain class have the same free energy, although the free energies of states in different classes are not degenerate in general. While there is only one class in the XS pairing, each member of which is specified by the phase, there are many classes with different symmetries in the 3 P pairing as will be shown below. Since the free energies of these classes change with temperature, pressure and other parameters, there are possibilities that phase transitions between superfluid states take place and indeed these transitions are observed. Classes of typical ordered states, including those actually appearing in the superfluid phase of liquid 3 He, are given below. We note that related subjects will appear at the end of Chapter 7.
6.2.1 BW state First consider the simplest form: Ali]=A6fij.
(6.13)
6.2 Superfluid state of3He pairs
135
Written in the 2 x 2 matrix form this state is
(
A
A
A
kx + ikv A
kz
y
A lx
kz
\
\ A
(C.A.
.
(6.14)
kx + iky J
The factor A contains a phase %, A = \A\e . This order parameter corresponds to a state with J = \L + S\ = 0, that is, a state with condensation of 3Po pairs. If this state is rotated round a direction h by an angle 6 in spin space (0.15) (or orbital space), there appears a new state Rji(n, 9) = cos 63 ji + (1 — cos 6)hjhi + sin Osjih This class of states with phase x a n d rotation specified by h and 6 is called the BW state (Balian and Werthamer 1963, see [B7]). One of the characteristics of the BW state is that it is invariant under simultaneous rotations in spin and orbit spaces, which are in the subgroup H of G. The symmetry SO 3 x (7(1) in Eq. (6.12) is broken in the BW state while the other symmetry SO3 is left unbroken. In this sense, the BW state is the most symmetric state among possible 3P states. Note however that the symmetry with respect to the relative angle between spin space and orbital space of the pair is broken. This manifests itself most clearly in the nuclear magnetic resonance mentioned later. It can be readily shown from Eq. (6.15) that A* x A = 0, since \(k) in Eq. (2.40) is proportional to A(k), and hence the BW state is unitary. Moreover the energy gap is isotropic since A"!"A = A* • A = \A\2kjkj = 1. 6.2.2 ABM state Consider three mutually orthogonal unit vectors /, m, h in momentum space A
such that m • h = 0 and I = m x h. Then the orbital state represented by A
m + in is a state whose orbital angular momentum along / is unity as shown in Fig. 6.4. Suppose both spin  j pair and spin j  pair take this orbital state as shown in Fig. 6.5. The components A^ when m = x and h = y are (A,j)=A\
1 i 0 .
(6.16)
Although the vector A^ in this form is directed along the yaxis in spin space, it may in general take any direction. Let us call this direction d. Thus one obtains a class of order parameters A^j = Ad^rhj + ihj)
(6.17)
Superfluid 3He
136
A
m Fig. 6.4. The triad of three mutually orthogonal unit vectors.
tt
L^ ABM
11
a tt
BW Fig. 6.5. The orbital state and the spin state in the Ai, ABM and BW states.
which is specified by a vector d and a triad of unit vectors (l,m,h). This class is called the ABM state (AndersonBrinkmanMorel 1973, see [B7]). The orbital state transforms as (in + in) —> e 1%(m + in) under rotation of the triad along / by an angle x Thus the state (6.17) is left invariant if this rotation is combined with a multiplicative gauge transformation e"1*. In other words, gauge transformation is absorbed into a rotation of the triad. The state is also left invariant under rotations around the rfvector in spin space. Furthermore, Eq. (6.17) is left invariant under the simultaneous A
A
transformations d —• — d and phase rotation by n/2. Therefore, the residual A
symmetries in the ABM state are products of the rotations around d, those around / and the inversion of d, namely (7(1) x (7(1) x Z2. The ABM state is unitary too and it follows from Eq. (6.17) that the A
A
A
A
A
A ,•»
energy gap is proportional to (m • k — in • k)(m • k + in • k) = 1 — (/ • k) . A
Accordingly the gap vanishes at the poles along / as shown in Fig. 6.6(a). This fact may be deduced directly from the symmetry of the ABM state as A
A
follows. If the operation R(l, n) of the rotation along / by n acts on *F, one has
6.2 Superfluid state of3He pairs
(a)
137
(b)
Fig. 6.6. The energy gap in (a) the ABM state and (b) the planar state. This transformation is equivalent to multiplication of the phase e17t of (7(1) A
A
A
A
as mentioned above. If k is equal to k$  /, one finds ^(ko) = 0 si n c e A
A
A
A
A
R(l, n)ko = ko implies *F(#o) = —^(^o) The nodes in the energy gap may be obtained from group theoretical consideration as can be guessed from this example. This kind of reasoning is employed when the gap in a heavy fermion system is considered in Chapter 7. 6.2.3 A\ state A state with spin f f pairs only, called the Ai state, is obtained if Eq. (6.16) is replaced by /i (Allj) = A\
1 \ 0
1 0\ i 0 . 0 0 )
(6.18)
If rotations in spin space and A>space are applied separately on the above state, one obtains an order parameter (Atf) = A(d, + ie,)(mj + in,) A
(6.19)
^^
with d _L e. This time, so far as rotations in spin space are concerned, the A
state is invariant only under rotations round the vector d x e. The Ai state is of course nonunitary. This state, in which spins in a particular direction form pairs while oppositely directed spins remain in a normal state without the energy gap, describes the Ai phase which is realised in a magnetic field. 6.2.4 Polar state and planar state Let d and h be unit vectors in spin space and A>space respectively. Then the state whose order parameter is Atf = Ad^hj
(6.20)
138
Superfluid 3He
is called the polar state since the orbit extends along the vector h. Because the energy gap is proportional to {hk)2, it vanishes on the equator perpendicular to h on the Fermi sphere as shown in Fig. 6.6(b). If the order parameter is given by A^j = A(R,j  Rjjjj)
(6.21)
in terms of Rij(h90) in Eq. (6.15), the state is called the planar state since the orbit extends perpendicular to /.
6.2.5 Other superfluid states Other superfluid states with different symmetry are possible. Their group theoretical classification is given in detail in [B7]. In connection with the superfluidity of 3 He we will mainly consider physical properties of the states described in Sections 6.2.16.2.3. It should be remarked that the 3P2 pairing is considered to be responsible for the superfluidity of neutron liquid in a neutron star since the nuclear force contains a strong tensor force as previously mentioned. In other words it is a superfluid whose spin and orbits are fixed in the J = 2 state. It might be thought in this case that each pair carries an angular momentum of 2% and hence the system carries an intrinsic angular momentum of 2h • ns/2 per unit volume. It must be understood, however, that particles form a pair outside the Fermi sphere while holes form a pair inside the Fermi sphere and there is therefore net contribution to the intrinsic angular momentum due to deviation from particlehole symmetry. Therefore the magnitude of the intrinsic angular momentum is reduced by a factor A/ep This argument applies equally to the pair orbital angular momentum of the ABM state. For the angular momentum of the whole system, however, one must include the contribution from superfluid flow near the container wall, and no simple conclusion can then be drawn from the present argument; see Section 6.6.
6.3 Physical properties of the 3 P superfluid states The expressions for the free energy, the gap equation and so on within the weak coupling theory are of the same structure in a superfluid state regardless of the pairing, as shown in Chapter 2. Therefore the results for liquid 3 He with a 3 P pairing will be obtained if the theory of 1S superconductivity in Chapter 3 is generalised mutatis mutandis.
6.3 Physical properties of the 3P superfluid states
139
6.3.1 Energy gap Let us consider the energy gap touched upon in the previous section in more detail. If the interaction (6.10) is assumed, Eq. (2.58) becomes
A, = 3gl £ tr { ^M'M^f*™}
•
(622)
In a unitary state this simplifies to &iii = 3gi 2 ^ A/m 2 ^ ki
kn
22^^
'
'
'
We must keep in mind that the gap in the quasiparticle excitation energy 8k is in general a function of k. In a unitary state, this gap is given by Afc2 = J[t;r(AjAfc). The critical temperature Tc is given, in any 3 P state, by kBTc = 1.13 coce~1/N^
(6.24)
just as in the BCS theory, as was mentioned at the end of Chapter 2. 1. BW state The gap in the BW state is given by A^ = Ai?^(w, 0), see Eq. (6.15), and the energy gap is isotropic, lA^2 = A2. Therefore Eq. (6.23) is identical to that for the {S pairing and the temperature dependence of A agrees with the BCS result. It should be noted that the only case in which an isotropic gap is produced in 7 ^ 0 pairings is the BW state in the 3 P pairing. 2. ABM state In Eq. (6.17) one may take m = x and h = j , without loss of generality. Then the gap equation (6.23) becomes
where 8 = Jt;2 + A^(l — fi2) and ji = k • z. The above integral is evaluated as ln(2coc/A) + 5/6 — In 2 at T = 0 and AA is given by AA = A 0 e a14
(6.26)
where Ao is the gap of the BW state at T = 0. The condensation energy is proportional to the angular average of AA 2 (1 — in2) over the Fermi surface, which becomes (2/3)eO28Ao = 0.88AQ. Accordingly the BW state has lower energy in the weak coupling theory. In fact, the B phase with an isotropic gap, identified with the BW state, appears at low temperatures. Weak coupling theory, however, cannot explain why the A phase, identified with the ABM state, appears just below Tc, since it predicts that the BW state is stable even near T c as
140
Superfluid 3He
will be shown in Section 6.5. It should be noted that the pair f f is independent of the pair j j in the ABM state in the weak coupling limit and there is no reason why they should take the same orbital state. The reason for this must be sought in the strong coupling effect. Finally the gap in the planar state is the same as that in the ABM state and the gap in the polar state is given by \Ak\2 = \Ap\\2(kl)2. The amplitude at T = 0 is Api = e 1/3 A 0 . Therefore \Ak\2 = (e2/3/3)Ag in the polar state and its condensation energy is the lowest.
6.3.2 Specific heat The energy gap profile is reflected in the temperature dependence of the specific heat C. Once the quasiparticle energy ^ is known, the specific heat C is obtained from the entropy (2.57). Let us make a qualitative consideration of the temperature dependence of C at T
(6.27)
Calculation shows that the coefficient of the above equation is In2/5. Similar calculations for the polar state, for which A = 0 on the equator, yield the density of states N(0)e(e/Api) and specific heat proportional to T2. The existence of a specific heat proportional to a power of the temperature in a certain class of states gives an important clue to understanding superconductivity in heavy electron systems as discussed in Chapter 7.
6.3.3 Superfluid component The expression (3.39) for the number density contributing to superfluidity is general, in so far as the quasiparticles can be regarded as elementary excitations, and may be applicable to any 3 P superfluid state. It should be noted, however, that the magnitude of the superfluid component depends
6.3 Physical properties of the 3P superfluid states
141
12
0.05
0.10
0.20
0.15
1T/Te Fig. 6.7. The temperature dependence of the superfluid components with the flow parallel and perpendicular to an applied magnetic field. (From [G18].)
on the direction q relative to the centre of mass motion in general since the energy gap Ak2 is anisotropic. In other words, ns is a tensor with components Sf(sk)
A
A
kjkj.
(6.28)
Since the BW state has an isotropic gap, ns in this case is identical to that in the BCS theory. In the ABM state, on the other hand, the gap depends on the relation between / = m x h and q. One carries out the calculation near Tc in a similar way to that for Eq. (3.41) to obtain 7C(3) lOn2Tc2
i(T)
(6.29)
= 2n g ». In other words, the normal fluid component when the flow is parallel to / is larger than that when the flow is normal to /. This result is not unexpected since the gap vanishes along +/ on the Fermi surface and hence there are large numbers of thermally excited quasiparticles around these points. The direction of the vector / is controllable as it is perpendicular to the wall and also perpendicular to an applied magnetic field. Figure 6.7 shows experimental results on superfluid density in the A phase, which is one of the proofs identifying the A phase with the ABM state.
142
Superfluid 3He 6.3.4 Magnetisation
The susceptibility associated with the nuclear spin of 3 He well demonstrates the characteristics of the spintriplet pairing. Suppose the direction of an external magnetic field is taken as the quantisation axis. Among the triplet of spin states,   , H and   + j  , the third one is made of oppositely directed spins and hence we expect the same result for this component as the *S case. On the other hand, it seems that one only needs to make the simple replacements & —• & + yB/2 for the components ff and j j . In fact, this can be easily verified by examining Eqs. (2.50) and (2.51) with %k = &1 + o?>yB/2. (If one puts A oc 10^02, yB/2 does not appear in Eq. (2.50) as in the spinsinglet case.) Since there are only   a n d   pairs in the ABM state with d _L B, pairing with these components is possible although the number of up spins differs from that of down spins by N(0)yB/2 just as in the normal state. Accordingly one finds x = Xn = y2N(0)/2 in this case. On the other hand, one has the same result as the XS case if d is parallel to the magnetic field B. The dvector satisfies d _L B in a magnetic field if there is no other mechanism that fixes d and hence one should obtain x = Xn In fact it is observed that x does not change at the transition to the A phase. Next we consider the BW state. It follows from the above consideration that the part kl + kj yields Xn while the part k\ yields the same Xs as that for the XS pairing given by Eq. (3.43). Therefore the susceptibility in the BW state is given by Xs). ^^Xn + Xs).
(6.30)
We expect the above susceptibility to approach 2# n /3 as the temperature is lowered since Xs vanishes at T = 0. Figure 6.8 shows that x i n the B phase decreases with decreasing temperature, approaching a finite limit. This limiting value deviates from 2/3, however, and for quantitative agreement, the Fermi liquid effects should be considered, as is the case also for ns. Liquid 3 He undergoes a transition from the normal state to the A phase through the Ai phase in a magnetic field as shown in Fig. 6.1 (a). The number density of particles with spin parallel to the magnetic field is larger than that with the opposite spin by N(0)yB in the normal state. Therefore the densities of states at the respective Fermi surfaces differ as A/fQ)(0) = N(0) + (—)m 2yB/2n2kY and, as a consequence, the Ai phase with ff pair has a higher Tc. A rough estimate of the difference in Tc is obtained from Eq. (6.24) as ?V ~Tci Tc
1 yB JV(O)gl e F '
where the change in the interaction has been ignored.
(6.31)
6.3 Physical properties of the 3 P superfluid states
143
1.0
0.6 0.8 T/Tc Fig. 6.8. The temperature dependence of the susceptibility at 20 bar in the B phase. (From [G19].) 6.3.5 Fermi Hquid effects The pairing itself does not change the particle and spin densities if there is particlehole symmetry above and below the Fermi surface. Accordingly the Fermi liquid effects do not appear in the gap equation for example. However the expressions for, say, the normal component and the susceptibility must be modified due to the Fermi liquid effects since the way the medium polarises changes substantially under the superfluid transition. This is most easily understood in the susceptibility. In the superfluid state one needs to put x® in Eq. (6.6) in place of Xn which corresponds to df®a/dt;vaL. Here x° is the susceptibility without the Fermi liquid effects. Then one obtains 7 (a)
Xs_ Xn
7°
As
(6.32)
Therefore one finds Xs = Xn in the ABM state while 2
1
i
r(a)
as T —> 0 in the BW state. Figure 6.8 clearly shows this effect. The correction to the normal component can be obtained in a similar way, resulting in the expression (6.33)
Superfluid 3He
144
6.4 Spin dynamics and nuclear magnetic resonance One of the remarkable phenomena in superfluid 3 He is nuclear spin dynamics. As already noted, the dominant interatomic force in 3 He is invariant under separate rotations in spin space and real (momentum) space. However superfluid ordering breaks the relative symmetry. This spinorbit symmetry breaking manifests itself most clearly in the nuclear spin dynamics since there is a very weak spinorbit coupling interaction between the nuclear spins, called the magnetic dipole interaction HD, or the dd interaction. The interaction H^ between nuclear magnetic moments ^ya is written as ( ^ 3 T k,k',q
V
"
j ) J
4
q
l
j
q
(6.34)
where tr stands for the trace over spin indices. The statistical average in a specific superfluid state £ D = ( # D ) may be obtained in the mean field approximation. Thus, if the order parameter is written as *F(A;), one obtains
where the approximation \k\ ~ fep is employed as usual. If the representation *F = A^IG^GI is used, one obtains tr( • •) = —2(AiA*j +AtA* — dijAxA]). Then substitute Eq. (6.11) into the above equation and integrate the resulting A
A/
expression with respect to k,k and £, £'. These integrations are easily carried A
out if one takes three contractions with respect to the four components of k and k since only scalar quantities remain after integrations with respect to angles. Finally one finds (635) where the notation Ay = JV(O)gi /d^Ay(^) has been introduced. The magnitude of the above equation is estimated as £ D ~ ^(AO/£F) 2 (^7 2 ) since l/JV(O)gi is of the order of unity. The energy £ D of course depends on the state. For the ABM state, if Eq. (6.17) is substituted into Eq. (6.35), one obtains
6.4 Spin dynamics and nuclear magnetic resonance
145
While for the BW state, if Eq. (6.15) is substituted into Eq. (6.35) one obtains 5
(6.37)
This expression is independent of h since h is the only vector in Eq. (6.15). In contrast with the condensation free energy which is independent of dl or 9, the energy £ D depends on these parameters representing the 'breaking of the symmetry' although the magnitude of the latter is far smaller than that of the former. This dependence is observed directly by nuclear magnetic resonance (NMR). The energy £ D is known to vanish by symmetry in a liquid or in a crystal with a cubic symmetry even with a ferromagnetic order. It remains finite in a superfluid state of 3 He, though it is a fluid, since the relative orientation of the position vector and the triplet spin vector is fixed, that is to say, the spinorbit symmetry is broken.
6.4.1 Spin dynamics and NMR The spin motion in a superfluid state is a form of collective mode. A small amplitude oscillation with a finite wave number is just a spin wave. Here, uniform motion with wave number 0, that is, the motion of the total spin angular momentum S is considered, since nuclear magnetic resonance is under consideration. One should recall that S is a classical quantity and the generator of infinitesimal rotations in the spin space of the system. Accordingly the canonical conjugate quantity to S is a vector 6(= hO) representing a rotation in spin space and the equations of motion in an external field H are (6.38)
The second equation is just Larmor's theorem, which states that the effective magnetic field in a rotating system with angular velocity o = dO/dt is H+y~l
y
d6
d? dt
xH+yx
2
_xdEv
y
dH
~w =  ^
(639)
Superfluid 3He
146
Fig. 6.9. Spin motion in the ABM state. ABM state Explicit calculation is easily carried out for the ABM state identified with A
the A phase. The d vector is perpendicular to a uniform static magnetic field Ho as remarked in the analysis of the susceptibility. Furthermore, the most stable state is realised when d _L Ho and d \\ I since £ D in Eq. (6.36) is A
A
A
A
A
minimised when / is parallel to d. Let us consider small oscillations about this state. It may be assumed that the orbital part of the pair, namely the A
vector /, is kept fixed. The coordinate axes are taken as Ho  z and /  j , see Fig. 6.9. Equation (6.39) separates into transverse oscillations, in which 9X and 9y change, and a longitudinal oscillation, in which 9Z changes, since for a small oscillation 6 is given by a summation of respective rotation angles around each axis and hence (/ • d) = 1 — \(9]. + 92). The resonance frequencies are co2 = coo2 + ^ A 2 , 7 co2 = Q A 2 ,
(6.40)
where a>o = yHo and A
5^ ZAgi 2
is the shift in the transverse, i.e., ordinary NMR resonance frequency, see Fig. 6.10. Longitudinal oscillation is oscillation in the magnitude of S, characteristic of the superfluid state. This mode is called ringing when the amplitude is finite and can be regarded as a form of a.c. Josephson effect in which the weak dd interaction couples the   and j j superfluids. BW state The variables which represent the breaking of the spinorbit symmetry in the BW state corresponding to the B phase are h and 9 in Eq. (6.15). The
147
6.4 Spin dynamics and nuclear magnetic resonance
10 0.002
0.005 0.01
0.02
0.05
0.1
0.2
0.3
Fig. 6.10. The temperature dependence of the shift QA in the NMR resonance frequency in the A phase under melting pressure. The data obtained from transverse resonance are denoted by A while those from longitudinal resonance are • and • . (D.M. Lee and R.C. Richardson, from [Bl].) susceptibility % is isotropic, however, and the direction h cannot be fixed from magnetic energy considerations. Moreover the energy £ D of Eq. (6.37) does not fix h either. It can be shown, however, that a term proportional to H2 in £ D is minimised when n \\ H. Although this £ D contribution is even smaller than that in Eq. (6.37), it makes h parallel or antiparallel to H in the uniform equilibrium state. The angle 6 in Eq. (6.37) is, then, the rotation angle 6Z around the axis z ( Ho). Therefore there is no torque due to £ D acting on the transverse oscillations and hence the resonance frequency does not shift from CDQ = yHo. Equation (6.37) is minimised at 00 = cos" 1 (—1/4) = 104° and 2n — #o The frequency of a small oscillation of 9Z around the equilibrium angle, namely the frequency of the longitudinal oscillation is "' 2"
(6.42)
The ratio of the above frequency to that of the A phase is 2
= (5/2)(AB/AA)WZB),
(6.43)
which has been verified experimentally near the AB transition point. The frequencies QA and QB are of the order of a few kHz. Although £ D is fairly small, the shift in the resonance frequency is easily observable since X, corresponding to the inertial mass in the above equation of motion, is small. (A shift due to the same mechanism has been observed in the u2d2 phase in solid 3 He with nuclear spin ordering.) At finite temperatures only
Superfluid 3He
148
the resonance at co = JCOQ + Q^ is observed even in the presence of thermal excitations. This is because unpaired particles also receive torque from £D6.5 GinzburgLandau theory It has been shown in Chapter 5 that the GinzburgLandau theory is effective for practical analysis of many phenomena in ordinary superconductivity. This approach is indispensable in the more complicated 3 P superfluid. In the GinzburgLandau theory, free energy Fs — Fn is expanded in terms of the energy gap or the order parameter assuming T ~ Tc. Terms up to the fourth order in the order parameter and terms up to the second order in the spatial derivative of the order parameter are kept in the above expansion, assuming that the scale of the spatial variation is larger than the coherence length £o One may readily write down the form of the free energy since it must be invariant (a scalar) under transformations associated with symmetry breaking, namely spin space rotation, orbital space rotation and gauge transformation. First of all, the second order term in the order parameter must be a scalar in spin and orbital spaces separately and invariant under a global phase change and hence it is singled out to be A^A^. The same reasoning yields the free energy density in the form
U  / n = ^N(0)A e 2 (T)a4^ + i
^
+ HA^A^2
f p^A.^A.^jA.viA.vj^
ljlj
;
j
j
^djA^
(6.44)
where A 2 (T) = [8TC 2 /7C(3)](1  T/TC)T2. The sum of terms quadratic in diA^j is called the gradient energy. The coefficients a,/?* (1 < i < 5) and Kt(l
3glN(O)(i?c3)AwAlmA^tr Q ss /
6.5 GinzburgLandau theory
149
where s^ = i c r ^ . The above equation is easily evaluated to yield /?. Similarly the coefficients K are obtained if the gap equation with centre of mass momentum q of a pair is expanded in terms of v?k • q. In summary, the coefficients in Eq. (6.44) are obtained within the weak coupling theory as
ft =  1 / 2 ,
p2 = fo = p4 = l,
ps = l,
(6.45)
K\ = K2 = KT, = £ /5, 2
where £ = z;p/6A2(T) is the coherence length defined by Eq. (5.3). If we use the order parameters of the BW (Eq. (6.15)) or the ABM state (Eq. (6.16)), we get the free energy of the respective state measured from the normal value as 5 A/BW/iV(0)A2 =   [3(/Ji + h) + ft + ft 4 (6.46) 1 2 A/ABM/N(0)A =   ( f t + ft + ft)" . If the weak coupling values are used, these numbers turn out to be —3/5 and —1/2, so that the BW state has lower free energy and should be stable. 6.5.1 Momentum density associated with superfluidity One assigns a virtual 'charge' 2m to the 3 He pair and obtains the current density by taking the derivative of the free energy in the presence of a vector potential A with respect to A to find the momentum (mass flow) density associated with a superfluid flow. That is, one makes the replacement V —• V — i2m^ in Eq. (6.44) and then takes the derivative with respect to the ith component of A to find
jsi = 2m^N(0)A2e(T) I m { X i ^ 5 ^ + X ^ M ^ + ^A^djA^}.
(6.47)
6.5.2 Magnetic free energy Next an additional term in the presence of an external magnetic field H is obtained. The quadratic invariant with respect to H and A is fH = a B i ^ V # v ^ w ,
(6.48)
where OCB is a constant. This energy must be a term proportional to A^A in the spin paramagnetic energy
ij.
(6.49)
150
Superfluid
k
k'
(a)
k
(b)
ft ft'
oo
Fig. 6.11. (a) The gap equation, (b) Approximation to the effective interaction (the
wavy line).
The magnetic susceptibility in the superfluid state is in general a tensor. One compares Eq. (6.48) with Eq. (6.49) in the BW state to find the constant OCB, noting that if j ^ in Eq. (6.32) is expanded in A"!" A at T < Tc, the ratio of the coefficients is given by Xs/x®' = (1 + P^)~2 Then one obtains an additional contribution to Eq. (6.44) of the form
fH = \N(0)A£(T)± ( — O
H^HyAyi.
(6.50)
Note that, for the magnetic dipole interaction, Eq. (6.35) can be used.
6.5.3 Strong coupling effects and spin fluctuations It is assumed in the weak coupling theory that the pairing interaction itself is independent of the order parameter. The interaction has been represented by a constant gi in the analyses so far. In reality, however, the interaction should change in the presence of pairing since it is an effective interaction in a manybody system including polarisation effects. The wavy line, which represents interparticle interaction in the gap equation (Fig. 6.11 (a)) corresponds to an interaction including polarisation effects, namely density and spin density fluctuations as shown in Fig. 6.11(b). Static polarisation due to an external field has been considered in Section 6.1. Now, one of the interacting quasiparticles plays the role of an external field, and hence fluctuations are dependent on space and time. These fluctuations are clearly modified under the superfluid transition. Therefore the gap equation has to be analysed taking the Adependence of the wavy line into account. Let us consider the gap equation up to the third order in A, which
6.5 GinzburgLandau theory
151
Fig. 6.12. Correction to the coefficients /? under the strong coupling theory.
amounts to keeping the fourth order terms in the free energy, since we are interested in the corrections to the coefficients ft of the fourth order terms. Terms obtained by expanding the factor s^1 tanh(/J 8/^/2), from the Green's function of the pair (k',—k r) in Fig. 6.1 l(a), in A^A correspond to the terms with coefficients ft already found above. The correction is a term obtained by drawing out At A, denoted by a slash, from one of the particlehole pairs in Fig. 6.11 (a) and is depicted in Fig. 6.12. The wavy line in Fig. 6.12 is the effective interaction in the normal state. In this discussion only the spin fluctuation, also known as the paramagnon, is considered and the density fluctuation will be neglected since the former is large in liquid 3 He as already noted in Section 6.1. Then the wavy line represents F^xn including the coupling constant with quasiparticles. Here one has to use F^xn(q,co) since fluctuation depends on both the momentum q = k — k r and the frequency. Provided that the co dependence is negligible and assuming an appropriate qdependence, one may estimate the correction Sfc to the coefficient fr as
8Pi = Sp3 = 0,
dp2 =
P4
S=c(Tc/TF)[N(0)gl]2
ps
(6.51)
Here the coefficient c9 which is of the order of unity, increases with pressure, and is a correction stabilising the ABM state at relatively high pressures. Although this model has a resemblance to the attractive force due to phonon exchange studied in Chapter 4, MigdaFs theorem is not applicable to spin fluctuations and vertex corrections must be considered to be more precise. The interaction from spin fluctuations is proportional to the factor [F^x(q)]2, which becomes large as q > 0, as mentioned above. In other words, one may consider physically that ferromagnetic fluctuations are dominant since the Fermi liquid effects enhance the susceptibility. This type of qdependence favours pwave pairing.
152
Superfluid 3He 6.6 Textures and superfluidity
'Symmetry breaking' in superfluid 4 He or an ordinary superconductor has to do with gauge transformations, and the phase x of the order parameter W was the variable associated with the broken symmetry. It has been shown, moreover, that if the phase JJ changes in space a flow of the superfluid with the velocity us(x) = Vx(x)/2m appears. On the other hand, symmetries associated with spin and orbital rotations are broken in the superfluid state of 3 He, in addition to that broken under gauge transformation. Because of these facts, there appears in 3 He a superfluid with texture, just like a liquid crystal, and its superfluid properties are far more complicated than a conventional superfluid (or a superconductor). These aspects are considered here with emphasis on the relatively simple ABM state.
6.6.1 The London limit Those states belonging to a particular class, such as the BW state or the ABM state, are mutually connected by 'residual symmetry' transformations. Therefore all the states in a class are energetically degenerate, just as XS superconductors with different phase of the order parameter *F share common free energy. These considerations show that the most easily realisable among spatial variations should be those involving symmetry transformations within the given class. Therefore one can suppose that the order parameter at an arbitrary point in the system in the B (A) phase belongs to the class of the BW (ABM) state. In the following we will be mainly concerned with spatial variations within this framework. This framework corresponds to the London limit in an ordinary superfluid, which is applicable when the scale of the spatial variation is larger than the coherence length £. One may also say that only those variations connected to the NambuGoldstone mode are considered in this limit.
6.6.2 Superfluidity in the ABM state The order parameter in the A phase takes the form of Eq. (6.17), namely A^j = Ad^rhj + my), anywhere in the London limit. In other words, one considers a vector d and a triad /(= m x h),m,h. Since they are fields of directed quantities, the superfluid may be considered as if it shows a 'texture'. Of course there appear new characteristics such as anisotropy of physical quantities associated with texture.
6.6 Textures and superfluidity
153
The current density (6.47) of a superfluid in the ABM state is written as hi = ns  Ida  hlj] mkVjhk + ldij  lilj] (V x /), j ,
(6.52) A
where ns\\ in Eq. (6.29) has been simply written as ns. When / = m x h has no spatial dependence, the current js depends only on m^V^. If this is the case, m^Vn/c is just the spacederivative V% of the phase % of the order parameter, as was noted in Section 6.2, and the current has an identical form to that of an ordinary superfluid, except for the anisotropy. Note, however, that the second term does not vanish when / varies in space. The /vector indicates the direction of the angular momentum of the pwave pair. Therefore V x / resembles the effective current in a magnet V x M induced by spatial variation of the magnetisation M. The term containing V x /, however, contributes to the actual mass current in the present case. This implies that variation in texture leads to superflow since the vector / denotes, so to speak, the direction of the texture. Let us consider, as an actual example, a linear vortex structure which is uniform along the zaxis. Suppose the axis of the vortex is taken to be the zaxis. The uniqueness of the order parameter implies that, although it may change as one moves around the zaxis, it must revert to the same configuration upon return to the starting point. Then the problem is to classify the types of configurations of the field d(m + in) which satisfy the A
A
condition mentioned above. Let us suppose, first of all, that the rfvector is uniform, which may be taken to be y for example. One has an ordinary A
superfluid if / = m x h is uniform taken to be z for example; and the possible structure is a vortex line with a circulation quantum number AT(integer). This structure produces the velocity field 2m r around the zaxis, see Fig. 6.13. The triad rotates around the /vector N times as one goes around the zaxis once. This structure has a core of radius ~ £, within which the superfluid density is suppressed, since vs diverges as one approaches the zaxis, see Section 5.3. The vorticity V x vs is finite only in the vicinity of the core. This type of configuration is called a vortex structure with a core. A
A
Let us next consider the case with varying /. Suppose /  —z on the zaxis and the vector / gradually rises as the distance r from the zaxis increases, eventually satisfying /  z for sufficiently large r. If m and h are considered along with /, one finds that the triad far from the zaxis rotates around /(= z) A
A
154
Superfluid 3He z
Fig. 6.13. The flow around a vortex line.
m
Fig. 6.14. A vortex structure without a core.
exactly twice as one goes around the zaxis once as is shown in Fig. 6.14. Accordingly the structure looks like a vortex with N = 2 if seen from far outside, while there is no core associated with the structure since the vortex current vanishes as r —> 0. Of course, the circulation is not quantised and the A
vorticity is finite in a region where / varies in space. Provided N is even, a vortex with a core may in general be deformed into such a structure, called the continuous vortex structure. The vector d has been kept fixed so far. Now let us consider cases where d also varies in space. The order parameter Ad(m + in) is left invariant under the simultaneous transformations m,h —> — m, —n and d —> —d. Accordingly a vortex structure with a core, as considered previously, with N = ±\ is possible, where m and h rotate around /(= z) by an angle n while d reverses in direction as one goes round the zaxis. In other words, the spin t t component of the superfluid is in a vortex state while the spin j j component
6.6 Textures and superfluidity
155
is in the N = 0 state, or vice versa. It should be added that spatial variation of the dvector leads in general to a spin current.
6.6.3 Textures The texture realised under a given condition is determined by minimising the free energy, in particular the gradient energy in the London limit. One must also specify an appropriate boundary condition. Let us first consider the boundary condition imposed on the order parameter at a wall of the vessel. The wall is idealised and considered to be specular and the zaxis is taken to be normal to the wall. Then it is expected that, among three orbital states of the 3 P pair, the component kz is destroyed while kx and ky are unaffected, since the zcomponent of the particle momentum kz becomes —k z upon reflection off the wall. Therefore there are no effects of the wall in the ABM A
A
state provided that the /vector is perpendicular to the wall. If the /vector is not perpendicular to the wall, there is a loss of condensation energy of the order of (Fs — Fn) • £(T) per unit area. Accordingly the boundary condition A
at a wall within the London limit is I \\ h, n being the unit normal to the wall. It follows from the same consideration that the London limit is not applicable to the BW state and the planar state is considered to appear in the vicinity of a wall. A
A
The boundary condition /  h 'pins' the vector / perpendicular to the wall in the A phase between parallel plates. In a cylinder, the texture inside the inner circle of Fig. 6.14 is realised in the A phase. The A phase superfluid in a cylinder then automatically supports vortex flow, namely an angular momentum. The magnitude of the vorticity is of the same order as that of an JV = 1 vortex line at the centre. To determine the texture one must often include the magnetic dipole energy £ D given by Eq. (6.35) in the free energy to be minimised. Similarly one can consider the free energy (6.50) in the presence of an external magnetic field. Where the spatial variation is mild enough, a texture is realised, which minimises these energies everywhere in the sample. In other words, one may apply the London limit not only to the condensation energy but also to other smaller energies as well. The energy scale beyond which the London limit is not applicable is determined from the condition that the gradient energy becomes of the order of the energy under question. If the constant K in Eq. (6.45) is employed in the GL regime, one finds
156
Superfluid 3He
for the dipole energy and hence the relevant length scale is estimated as KO,
(6.54)
where £o is the coherence length at T = 0. The length scale £D is of the order of 10~3 cm according to the above estimate. Similarly the length scale £H defined by the magnetic energy / H is given by & ~ (HA/H)Zo,
(6.55)
where HA ~ 2 x 104 G (= 2 T). The two scales £D and £H are of the same order when H ~ 28 G. It follows from Eq. (6.36) that £ D tends to align d parallel to /. It is also found from Eq. (6.50) that an external magnetic field H introduces the condition d _L H. The vector I satisfies / _L H if these are the only two relevant energies.
6.6.4 Rotating system One of the most interesting experiments on superfluid 3 He is observation of the state realised in liquid 3 He rotated together with the vessel. So far system angular velocities of Q < 3 rad/s have been achieved. One expects that a vortex lattice parallel to the rotation axis will appear in this case since coordinate transformation to a rotating system with a constant angular velocity is equivalent to applying a uniform static magnetic field in a charged system. If N = 1 vortices appear as in superfluid 4 He, the number of vortices per unit area is Ny = {2m?> /nh)£l. Note that the intervortex distance ry is 0.02 cm and ry > £D for Q = 1 rad/s. For the above reason, if a magnetic field (> 28 G) is applied parallel to the rotation axis, the vector / satisfies / _l_ H  Q outside a region of radius £D from the centre of each vortex, A
A
A
as shown in Fig. 6.15. The vector / varies in the region r < £D and the vorticity is expected to be finite there. Figure 6.16 shows one candidate vortex structure that minimises the free energy. One technique to study the texture experimentally is nuclear magnetic resonance. A satellite appears in the resonance absorption spectrum with area proportional to the angular velocity, that is, the number of vortices in the structure when the system is under rotation, see Fig. 6.17. The vector / is unlocked from d for r < £D, which leads to a potential energy due to £ D  Then a localised spin wave mode appears which is considered to be responsible for the satellite. These facts support the proposed continuous vortex structure.
6.6 Textures and superfluidity
157
^* t \ \\\W
\ t
S/ ? t t t t t t /
Fig. 6.16. The /texture associated with vortices.
6.6.5 Vortex in B phase
So far vortices in the ABM state have been considered. In fact vortex structures in the B phase are also quite interesting. Figure 6.18 shows the NMR data obtained from rotating superfluid in the B phase. There are many peaks due to the spin waves produced by the /itexture when the B phase fluid is under rotation. The vortices produced by rotation lead to an increase in the interval between two neighbouring peaks as shown in Fig. 6.18. These resonance frequencies depend on the temperature and the pressure, and jump
Superfluid 3He
158
(a) O = 0
(a) Q = 0
0
2 4 vv o (kHz)
6
Fig. 6.17. Appearance of a satellite in the NMR absorption curve when liquid 3 He in the A phase is rotated. (From [G20].)
Frequency Fig. 6.18. The change in the NMR absorption curve when liquid 3 He in the B phase is under rotation. (From [G20].)
suddenly at some temperature as shown in Fig. 6.19. This demonstrates that in the B phase there are two phases of a vortex structure, FA and FNA as shown in Fig. 6.20. Moreover it is found that the resonance frequency of the low temperature phase depends on whether il  H or il \\ —H, hence spontaneous magnetisation is associated with the vortex structure.
6.6 Textures and superfluidity
0.5
0.6 T/Tc
159
0.7
Fig. 6.19. The temperature dependence of the NMR frequency due to spin waves. (From [G20].)
Fig. 6.20. The phase diagram of a vortex structure in the B phase. The region FA denotes the phase with an axially symmetric vortex while FNA denotes the phase with a vortex without axial symmetry. (From [G21].)
160
Superfluid 3He
The BW state has an isotropic gap and behaves in a similar way to an ordinary superfluid in the London limit. Accordingly the vortex structure is no different from that of a quantised vortex line with a core if seen from a distance r > £ from the centre. The London limit is not applicable, however, in the vicinity of the core r <; £ and there appears a structure which deviates from the BW state. To analyse this structure theoretically, one minimises the GL free energy up to the fourth order terms with such boundary conditions that the structure approaches the vortex in the BW state at r > £. According to theoretical calculations, the core part is filled with a superfluid similar to the ABM state. There is an axially symmetric vortex FA and asymmetric vortex FNA and the latter is the candidate for the structure that appears in the low temperature (or low pressure) phase. The core of an asymmetric vortex can be regarded as made up of halfquantised vortex pairs in the A phase.
7 New superconducting materials
Ever since the discovery of the phenomenon by Onnes, the quest for new superconducting materials has enlivened the history of research in superconductivity. The strongest motivation for this research has been the search for a superconductor with higher Tc. Since the discovery of superfluid 3 He, nonswave superconductors have also been sought. The fruit of the former is represented by discovery of the high temperature superconductors (abbreviated hereafter as HTSC) in 1986 while the heavy electron system (also called the heavy fermion system) is highlighted as an example of the latter. The characteristics of these two systems are discussed in the present chapter. 7.1 Superconducting materials Let us first outline typical materials undergoing superconducting transition. Table 7.1 shows characteristic materials from several categories. It was shown in Chapter 4 that, where the electronphonon interaction is responsible for (or Eq. (4.48) to be more the superconductivity, Tc ~ coj^exp (—JM,J precise). Accordingly the system should become a superconductor if the parameter X for the attractive interaction exceeds the effective Coulomb interaction parameter \i \ which is about 0.1 in an ordinary metal. Since large X implies a large electrical resistivity, a bad conductor as a normal metal tends to be a superconductor. In fact, all the metallic elements, except magnetic metals such as Co, Ni, Fe, alkaline metals and noble metals, become superconducting at low enough temperatures including such elements as Si, S and I that undergo metallic transition under high pressure. The parameter I is large if the density of states JV(O) on the Fermi surface and the electronphonon coupling constant are large. Metals with a rather small Debye frequency are strongly coupled. Figure 7.1 shows that there is a correlation between JV(O) [= \y/{nk\)} and T c. There have been 161
New superconducting materials
162
Table 7.1. Various superconductors
Elements
Material
^Tc(K)
Au
< 0.001
Al Pb Nb Under pressure
Metallic compounds and alloys
Heavy electron systems
Ga Si I (Metallic H
k ~ 0.1. Weak electronphonon interaction. 1.2 k ~ 0.4. Typical BCS type. 7.2 k ~ 1.55. Strong coupling system. 9.2 k ~ 1. A dband metal. The element with the highest Tc. 8.6 Tc = 1.1 K for an amorphous crystal. 7 A metal at P > 1.2 x 1010 Pa. 1.2 A metal at P > 2.1 x 1010 Pa. 135 ~ 200? Large coD. A metal at P > 1.5 x 1011 Pa.)
Nb 3 Sn Nb 3 Ge
18 23
Gdo.2PbMo6S8
14.3
ErRh 4 B 4
8.5
ErMo 6 S 8
2.2
CeCu2Si2 UPt 3
0.5  0.6 0.5
A15 type,;. ~ 1.651.95. Thin film, the largest Tc among A15 type. Chevrel type, the highest Hc2 except for HTSC. Becomes ferromagnetic at 0.9 K, superconductivity disappears. Superconductivity coexists with antiferromagnetism at T < 0.2 K. Three distinct superconducting phases, 3Ppairing(?).
UBe13 Oxides
Copper oxides
Organic compounds
SrTiO3_x
0.05  0.5
LiTi 2O4 Ba(Pb!_xBix)O3 Bai_ x K x BiO 3
13 13 >30
La 2 _ x Ba x Cu0 4
> 30
YBa 2 Cu 3 0 7  <5 Bi 2 Sr 2 CaCu 2 O 8
93 125
(TMTSF)2C1O4 [BEDTTTF]2Cu(NCS)2 K3C6o Rb 3 C 60
1.2  1.4 11.4 18 28
A superconductor with a small carrier density n < 1020 cm" 3 . Perovskite structure. x ~ 0.25. An insulator at x > 0.35. x ~ 0.4, an electronphonon type (?), threedimensional. The first copper oxide, twodimensional.
Onedimensional. The largest Tc among organic materials, twodimensional. Doped fullerene, k  0.5 (?).
Remarks: A table based on data around 1980 (P.B. Allen and B. Mitrovic [E3]) was used in compiling the above table. The data for I are taken from recent research. (From [G22].)
7.1 Superconducting materials 1 V7V
YBa( "
,
bO
~o
Ba(PbBi)C 10 /
TJ
ga,
CO
cri I:ic
O
3
1 ~ •Ga
SrTiO 3
NbaGa N b 3 \* •
Nb» > # tfLa a
NaWU3
NbO * *Zr
n
 ^ x  ' " # •PbMo 6 S 8 y^s'm SnMc>6S8
7CuMo6S8
/
I
Chevrel compounds
(BEDTTTF) 2 Cu(NCS) 2
heavy electron systems
• Re
s#
"Cd*
r
LiTi2O4
/3 H g T ; In Tl*
K Cu0 A L S compounds h^
MoC *•
Pb»
1
L
(BaK)BiO3
1— —i
s
163
*'*
h
":
UB
i
\upt 3 o
i
o;
Ru..T.
•C 8 K
0.1
10 100 Sommerfeld constant (mJ/(molK 2))
1000
Fig. 7.1. The relation between the Sommerfeld constant y and Tc.
numerous theoretical works, based on the strongcoupling theory, on how far Tc may be raised when ordinary electronphonon interaction is responsible for superconductivity. Although no definite conclusion has been reached, it has been considered that the upper bound of Tc is about 30 ~ 40 K since very large X may lead to lattice deformation. Another approach towards high Tc is to look for an interelectron force in mechanisms other than phonon exchange. The exchange of bosons, not necessarily phonons, with an appropriate spectrum leads to an attractive force between electrons. One example of this mechanism is the case of liquid 3 He mentioned in Chapter 6, where a part of the attractive force is due to spin density fluctuation called the paramagnon. The first proposal along this line was the excitonic mechanism. An example of this mechanism is depicted in Fig. 7.2, in which an electron moving along the primary chain polarises the side branches which in turn attract another electron to result in an attractive force between these electrons, see [G23]. It is expected that this system might have large Tc since, instead of the Debye frequency &>D> a far larger exciton energy appears as a prefactor of the exponential function in the equation for Tc. Although such a proposal suffers from theoretical
164
New superconducting materials
Fig. 7.2. A model of an exciton mechanism. difficulties and has had no specific successes, it has stimulated research in organic conductors and many organic conductors showing superconductivity have now been fabricated. The quest for new superconducting materials has in reality proceeded empirically. The first big success was the discovery of the A15 superconductors which followed the discovery of the Chevrel metallic compounds with large HC2. One of the characteristics of the A15 superconductors is that transition metals with delectrons line up along x9 y and zdirections like chains as shown in Fig. 7.3. Present understanding from the tunnelling spectrum and other means is that superconductivity in the A15 system is due to electronphonon interaction. It should be remembered that there is a structural phase transition competing with superconductivity in the A15 system. The next remarkable progress is the discovery of BaPbi_ x Bi x O3 by A.W. Sleight, J.L. Gillson and P.E. Bierstedt ([G24]) which is the first system showing superconductivity among oxides basically of the perovskite type, see Table 7.1. BaPbC>3 is a semimetal while BaBiC>3 is an insulator of the Peierls type. A metallic phase showing superconductivity appears between these two systems. A member of the same group, Bai_ x K x Bi03 with Tc as large as ^ 30 K was found later. From recent research it appears that their properties might be explained within the framework of electronphonon interaction. The research on copper oxide highT c superconductors which pushed up Tc from 23 K (Nb3Ge) to 120 K at a stroke was triggered by the discovery of La2xBaJCCuO4 in 1986 ([Gl]). The cuprates have not only large Tc but other unique properties described in the next section.
7.2 Copper oxide superconductors
Fig. 7.3. The crystal structure of
165
(A15 type).
Let us add a few lines on organic superconductors before we close this section. Typical systems in this group include the TMTSF system (T c = 0.4  1.4K) and (BEDTTTF) 2 X (Tc = 10 ~ 12.8K) in Table 7.1. Figure 7.4 shows the crystal structure of (BBDTTTF) 2 [Cu(NCS) 2 ]. Their common property is conductivity of the chargetransfer type with small carrier density (n ~ 1021 cm" 3 ) and low dimensionality. For the compound shown in Fig. 7.4, the coherence length in the bcplane is ^ ~ 30 A while that along the aaxis is £± ~ 3 A. The nesting of the Fermi surface becomes important in these systems due to low dimensionality so that a state with a charge density wave or a spin density wave can appear under pressure for example. It is not yet established whether the superconductivity is due to swave pairs or not. An interesting system related to this is C6o, one of the fullerenes, doped with an alkaline metal K or Rb, see Fig. 7.5. According to popular theory the conduction electrons in this system are mainly 7celectrons and their coupling with the intramolecular vibration of C6o, whose energy is 1000 ~ 2000 K, is responsible for rather large Tc.
7.2 Copper oxide superconductors
7.2.1 Structure There are more than ten copper oxide superconductors (abbreviated as HTSC hereafter) known to date. Structures common to these are the CuO 2 sheets in an alternating layer structure with blocks of a metallic element other than Cu (alkaline earth, rare earth, Bi, Tl and so on) and oxygen.
166
New superconducting materials
Cu
Fig. 7.4. The crystal structure of (BEDTTTF) 2 [Cu(NCS) 2 ].
K
Fig. 7.5. The crystal structure of K3C60
Four typical HTSC structures are shown in Fig. 7.6, where the CuC>2 sheet is seen to be sandwiched by the shaded block layers. There are two kinds of CuC>2 sheet, one with a Cu atom surrounded by O atoms at the corners of an octahedron or a pyramid and the other with all the atoms in a sheet as
7.2 Copper oxide superconductors
O
167
Cu
(a) La 2_jrSr;rCu04
O Y O Ba O •
O Cu
11.69A
3.
.V3.82A
(c) YBa 2 Cu/) 7
(d) TIBa2CaCu2O7
Fig. 7.6. Typical crystal structures of HTSC. The arrows indicate the CuO2 sheets. (See Yoshinori Tokura in [D16] for the structure.) in Fig. 7.6(b). Properties such as doping differ between these sheets but we will not be concerned with that difference here.
7.2.2 Electronic structure In order to understand the basic electronic states of HTSC such as La2 x Ba x Cu04 or La2 x Sr x Cu04 (Fig. 7.6(a)), discovered first, it is preferable to study their parent material La2CuO4. Two electrons are transferred from the La2C>2 layer to the CuCh sheet; thus on average the system is charged as (La2O2) 2+ (CO2)2~. Accordingly in this crystal the coupling between the two layers is ionic in nature. Then the 3d shell of Cu has a
168
New superconducting materials
0 Fig. 7.7. The orbitals used in the threeband model of the C11O2 sheet.
single hole while the 2p shell of O is closed as far as the formal valency is concerned. Let us examine in greater detail the electronic structure of the CuCh sheet, which plays the central role in what follows. The 4s orbitals of Cu may be neglected since they form a broad band. The 3d orbitals are relevant to the present problem. It is important to realise that, compared to other 3d transition metals, the energy of the 3d orbitals of Cu is the closest to that of the 2p orbitals of O. Accordingly these two orbitals tend to hybridise. Suppose the CuC>2 sheet is taken to be the xyplane. Among the 3d orbitals dx2_y2 has the largest amplitude in the plane and, together with p x and py of O, makes up three hybridised orbitals (Fig. 7.7) having highest energy and accomodating five electrons. Of the three bands, the one with the largest energy is halffilled from the band theoretical viewpoint. Hence we expect this system to be metallic. Actually La2CuC>4 is an insulator and, moreover, is antiferromagnetic below ~ 300 K. The reason for this behaviour is found in the strong Coulomb interaction between electrons. In particular, the 3d orbitals of Cu have a small extension in the crystal and the Coulomb energy U, when two electrons (spin  and  ) occupy the dxi_y2 orbital of the same site, is larger than the band width. Thus the system is a Mott insulator when each site is occupied by exactly one electron. It is well known from discussion on the Hubbard model that in such a case the spins align in an antiferromagnetic way at low temperatures due to exchange interaction, see [A6]. Suppose a part x of La is replaced (i.e., doped) by Ba or Sr. Then the number of electrons transferred to CuC>2 decreases by x, thus there appear holes with concentration x in the Mott insulator. (It is known from the light absorption data that holes mainly exist near the O atoms.) These holes move around the crystal without being blocked by the Coulomb repulsion
7.2 Copper oxide superconductors 500
169
500 antiferromagnetic phase
0.1 (a) La 2  x Sr r CuO 4
0.2 Ce(x)
0.3
(b) Nd 2 xCe x Cu0 4 ,
Fig. 7.8. Phase diagrams of (a) the La system and (b) the Nd system. TN is the Neel temperature at which the system undergoes a phase transition to the antiferromagnetic phase. (From Yasuo Endoh in [D16].)
U and hence the system becomes metallic as x is increased. A similar change appears in Nd2 x Ce x CuO4 in Fig. 7.6(b) for which even more electrons are supplied by doping. Note that the superconducting phase is adjacent to the antiferromagnetic phase as found from the low temperature phase diagram (Fig. 7.8). An extended threeband Hubbard model with the Hamiltonian H =
+ Ud
(7.1)
is used in the analysis of the manybody problem in an HTSC system. Here d\d and p\p are the sets of creation and annihilation operators of electrons in the d orbital of the Cu atom and the p orbital of the O atom respectively, where the site index has been omitted. Rough estimates of the important 0.5 eV, 10 eV and parameters are sp — sd ~ 2.5 eV, tpp Up  4 eV. Suppose the system enters a metallic state leading to superconductivity as carrier density is increased by doping. Then questions to ask are whether the Fermi liquid theory is applicable or if new kinds of elementary excitations have to be introduced due to strong correlations; and what is the mechanism for superconductivity? Since there seem to be no definite answers to the above questions at present, let us next summarise the observed characteristic properties of HTSC in the superconducting state.
170
New superconducting materials
100
150 200 250 Temperature (K)
Fig. 7.9. The resistivity of YBCO at zero magnetic field. p\\ denotes the resistivity along the caxis while p± denotes that in the abplane. (From [G25].)
7.2.3 Superconducting state 1. Electrical resistivity Figure 7.9 shows the temperature dependence of the electrical resistance of YBa2Cu3C>7 (YBCO) with no magnetic field. The resistivity in the afoplane (CuO2plane) is quite different from that along the caxis perpendicular to the plane as expected from the layered structure described above. In other words, the system is twodimensional so far as electrical conduction is concerned. The twodimensionality is even stronger in Bi systems. It must be noted next that the resistivity p in the normal state is proportional to T as p = aT over a broad temperature range. Deviation from this behaviour should be found if the resistivity is due to scattering by phonons, though there are no quantitative calculations on this yet. Finally it should be added that the Hall coefficient Rn in the normal state shows a notable temperature dependence, which cannot be explained from the ordinary Fermi liquid result Ru = I/he where n is the carrier number density. 2. Cooper pair It is certain from measurement of the magnetic flux quantum (hc/2e) and the observation of the Shapiro steps (see Section 3.4) that pairing of electrons is responsible for the superconductivity in HTSC. Whether the pair is of swave or nonswave type has not yet been determined. 3. Coherence length The coherence length £ at T = 0 (the subscript
7.2 Copper oxide superconductors
111
,1300. 1500 £ 0)
2000 o
2500 H 3000 g 20 40 60 80 100 120 140 160 Temperature (K) Fig. 7.10. The penetration depth of two HTSCs obtained from muon spin relaxation. The solid lines are the prediction of BCS theory. (From [G26].)
0 is omitted) is extremely small and has a strong anisotropy. If £a ~ £b ~ 15 A is employed in the CuO2plane, there are only 4 x 4 C11O2 unit cells in the area £%. Put another way, provided that each unit cell delivers a single carrier, the ratio of £a to the average intercarrier distance is 4, which is quite different from the ratio 103 ~ 104 for an ordinary superconductor. The coherence length £c along the caxis is about 2 A even for YBCO with relatively small anisotropy. Thus the interlayer coupling is rather close to a Josephson junction and, when discussing the microscopic mechanisms of superconductivity, we can regard the pair wave function to be confined in the CuC>2plane. Note that the finiteness of the mean free path / may be negligible (the clean limit) since £ is so small that 4. London penetration depth X^ The length X^ is extremely large in contrast with £. The most reliable measurement seems to be the muon spin relaxation (/iSR) result, which makes use of dephasing in the muon spin precession induced by an inhomogeneous magnetic field. Figure 7.10 shows the temperature dependence of X^ measured in the flux lattice state of YBCO with H  c, which roughly reproduces the temperature dependence of the superconducting component predicted by the BCS theory if X^2 oz ns(T) is assumed. Since the GL parameter r = XI^ is ~ 100, HTSC is a typical 'type 2 like' superconductor.
172
New superconducting materials
0 0.05
0.00
0.05
Voltage (V) Fig. 7.11. The gap structure of a thin film of YBCO observed by STM at 4.2 K. (From [G27].)
5. Energy gap A The energy gap may vanish at points or along lines on the Fermi surface, as found in Chapter 6, if the pairing is of nonswave type. Then at low temperatures the thermodynamic quantities and relaxation time approach zero as a power of T, rather than exp(—j8A). Even for swave pairing one must keep in mind that the temperature dependence of A may deviate from the BCS result in the strong coupling regime. Although the energy gap A may be directly observed in the electromagnetic absorption spectrum, tunnelling measurements and so on, no definite data are yet available partly due to the smallness of £. According to the recent tunnelling conductance measurement using scanning tunnelling microscopy (STM) (Fig. 7.11), there are no excitations within the gap, which favours swave pairing. The ratio AO//CBTC for all HTSC materials seems to be much larger than the BCS value given in Eq. (3.14). 6. Nuclear spin relaxation time T\ The inverse of the nuclear spin relaxation time, Tf 1 , of an swave superconductor of the BCS type is peaked at just below Tc and is exponentially small at low temperatures due to the coherence factor and the energy dependence of the density of states as shown in Chapter 3. Figure 7.12 shows the T\ of 63 Cu in HTSC. Observe that T^1 has no peak at just below Tc and does not decay exponentially at low temperatures. Although this fact may be explained if dwave pairing is assumed, it is not clear if the swave pairing should definitely be rejected when such effects as depairing
7.2 Copper oxide superconductors
173
•
1
•f •


«w
1 •
;
gio
2
•
r
X
• 10"
3
•
». xBiPb*Sr*CaCu*O ." o (La1_xSrJC)2Cu04 • YBa 2 Cu 3 0 7 :
0.1
1
T/Tc
10
Fig. 7.12. The nuclear spin relaxation rate, normalised by the value at T c, measured from the nuclear quadrupole resonance of 63Cu. (From [G28].) 1.5
.Tl 2 Ba 2 Cu0 6 + /Tc = o YBa 2 Cu 3 0 7
0.5
Fig. 7.13. The temperature dependence of the ratio (Ks/Kn) of the Knight shifts. The residual shift at T = 0 is subtracted from the data. The dotted (solid) line depicts the result of BCS theory with 2A = 3.5(4.5)/cBTc. (From [G28].)
are considered. The Knight shift measurement is given en passant in Fig. 7.13. The approximate agreement between Fig. 7.13 and the BCS result obtained in Section 3.3 should not be taken seriously since the shift at T = 0 is assumed to be totally from the orbital part and has been subtracted from the data in Fig. 7.13. 7. Neutron diffraction Since La2CuO4 shows antiferromagnetism, it is considered that the antiferromagnetic spin fluctuation remains strong even when the system is doped to be a metal. In fact this fluctuation has been observed in inelastic neutron scattering experiments.
174
New superconducting materials
Interesting data such as the temperature dependence of the phonon spectrum density are currently being obtained.
7.2.4 Mechanism of superconductivity There has been intensive theoretical research on the mechanism of superconductivity in HTSC based on the threeband Hubbard niodel (7.1) or its more simplified variant called the tJ model. It is interesting to ask what kind of long range order appears in the ground state when the filling factor deviates from 1/2, independently of its relevance to the actual HTSC. Although there are many attractive attempts to determine this, such as the resonating valence band theory and the anyon theory, so far none seems to yield consistent physical results. (See [D12], [D13] and [D14] for reviews of recent research.) An attempt along a conventional line of arguments is a theory which makes use of bosonic antiferromagnetic fluctuations, rather than phonons. Since these fluctuations become attractive at large wave numbers, in contrast with paramagnons, they can lead to dwave pairing, see Fig. 2.2. It is reported that resistance proportional to T may be obtained in the normal state when electrons are scattered mainly by antiferromagnetic fluctuations. On the other hand, phonons may not be totally negligible since HTSC, as with A15 systems, is always accompanied by lattice instability. The central questions are what plays the main role in the pairing and what type of pair appears as a result?
7.2.5 HTSC in a magnetic field Some of the remarkable features of HTSC are small coherence length and quasitwodimensionality as was noted in Section 7.2.3 and they result in new phenomena that have not been observed in other superconductors. They are particularly noticable in HTSC in a strong magnetic field. 1. Fluctuations The smallness of the coherence length £ implies that the effect of fluctuations will be substantial. In fact, Fig. 7.9 shows that the resistivity starts to decrease well above T c. This is the result of the superconducting fluctuations treated in Section 5.7 (see Eq. (5.58a)) for T ^ Tc, which can be observed in bulk HTSC, not just in thin films. The most remarkable features of the system are observed in a magnetic field. Figure 7.14 shows the temperature dependence of the electrical resistivity of a YBCO single crystal in a magnetic field. As
7.2 Copper oxide superconductors 20
175
°0(T)
°2
/4&
6 10
80
r
90
r(K) (b)
Fig. 7.14. The temperature dependence of the resistivity along the caxis. (a) The current / is in the abplane. (b) /  c. The solid lines are due to a theory with nonGaussian fluctuations. (Observed values are taken from [G29]. Theoretical curves are from T. Tsuneto, R. Ikeda and T. Ohmi in [D16].)
B is increased, the curve p(T) of an ordinary type 2 superconductor should shift towards the low temperature side as Tco shifts to TCH = Tco(l  o/B£$) (a relation obtained by solving Eq. (5.29) for Tc). In contrast with this, Fig. 7.14 clearly shows different behaviour, which makes it impossible to define HC2(T). In other words, the transition from the normal state to the Abrikosov flux lattice state mentioned in Chapter 5 is not clearcut in the present case. We can use the Ginzburg criterion introduced at the end of Section 5.7 to see whether or not fluctuations are of essential importance in the present system. The critical region in the absence of a magnetic field is e = 1  T/Tc\ £ 10" 2 for YBCO according to Eq. (5.59), which is not very broad. In the presence of a strong magnetic field such that the pair cyclotron radius ro = ((f)o/2nB)1/2 is smaller than £ = ^o^"1^2, the coherence length perpendicular to the magnetic field, the length scale perpendicular to the field is determined by ro rather than £, and Eq. (5.59) is replaced by /
\ 2/3
e£ (^4) \ AC (posoil /
.
(7.2)
Here £o is the coherence length in the direction along B. If £o = £Oc = 2.4 A and B = 5 T are entered in Eq. (7.2), the width of the critical region is 2 K and cannot be neglected. Furthermore, when the field B is sufficiently strong, the lowest energy solutions (n = 0 solutions of Eq. (5.28)) remain important as fluctuations. Then, the
176
New superconducting materials
energy of fluctuations depends only on variation in the direction of B(\\ z). In this sense, it must be emphasised, the system becomes onedimensional. Since long range order is proven to be absent in a true onedimensional system, it is doubtful if vortex lines in this case also undergo a phase transition to a lattice state with long range order, as shown in Section 5.4. In fact, data such as the magnetisation and the Peltier effect in addition to the electrical resistance indicate a continuous crossover from the normal state. Calculations based on nonlinear fluctuation theory agree fairly well with the observed value on the high temperature side, relatively close to T c# as shown in Fig. 7.14. 2. Melting of the vortex lattice What will happen at lower temperature? The electrical resistance of an ordinary superconductor may remain finite due to sliding of the vortex lattice in an ideal system without pinning centres. In reality, however, the superconducting current appears just below HC2 since the vortex lattice is fixed by the pinning centres. Now in HTSC interesting new features appear. First of all, the region in which the magnetic field is almost uniform is wide since 1 is very large. Therefore it is appropriate to call the structure a vortex lattice as in superfluid 4 He, rather than a flux lattice in an ordinary type 2 superconductor. Moreover, H;$c is so small (~ a few A) for B  c that the coupling between vortices created in the adjoining CuO2planes is suppressed by a factor of (£oc/£a)2 a n d hence a vortex line is easily bent. There is even a possibility that vortices in different planes are independent in the Bi system. As a result, it is considered that the vortex lattice starts to melt and becomes a vortex liquid far to the low temperature side of HC2(T) as shown in the phase diagram of Fig. 7.15. (The lower critical field HC\(T) is almost degenerate with the line H = 0 since the GL parameter K is large.) The vortex liquid cannot be distinguished from a state with strong fluctuations mentioned above and undergoes a continuous transition to the normal state. It is not clear whether there exists a definite melting curve in an ideal system or not. The vortex lattice may be stabilised by pinning centres if they exist. There is a possibility that a vortex glass state appears if the pinning centres are randomly distributed. It should be added that the topic mentioned above is just one of the problems associated with HTSC in a magnetic field; there are other interesting issues such as the critical current.
7.3 Superconductivity in heavy electron systems
111
Table 7.2. The Sommerfeld constant and the magnetic susceptibility of heavy fermion systems. y(O)/x(O) is the ratio per cubic cm 7(0) (mJ • mol" 1 • [cm 3] • K~2) CeAl3 CeCu 2 Si 2 URu 2 Si 2 UCdn UPt 3 UBe 13
1620 [18.5] 1000 [20] 180 [3.66] 840 [5.21] 450 [10.6] 1100 [13.5] 1.5 [0.063]
{Na
x(0) (10~3 emu • cm" 3 ) 0.41 0.13 0.03/0.10 0.24 0.19 0.18 0.001
45 153 37 22 56 75
63}
melting curve of vortex lattice
80
86
Fig. 7.15. The phase diagram of YBCO in a magnetic field. The shading indicates the crossover area.
7.3 Superconductivity in heavy electron systems
There are socalled 'heavy fermion systems' among the compounds of Ce and U with felectrons, which show extremely interesting properties. Table 7.2 lists some of them. Figure 7.16 shows the crystal structure of UPt3 as an example. The physical properties of these materials at relatively high temperatures can be understood based on a system consisting of magnetic moments localised on Ce or U, of the same magnitude as in the atomic form, and of conduction electrons found in ordinary metals. However the physical properties change drastically below 200 ~ 50 K, the exact value of which depends on the system under consideration. The number y(T) = C(T)/T, which corresponds to the Sommerfeld constant in an ordinary metal, and the susceptibility %(T) are very large and the extrapolated values as T —> 0
178
New superconducting materials
stack after 60°rotation Unit cell
Base plane
Fig. 7.16. The crystal structure of UPt3.
are larger than those of an ordinary metal such as Na by a few orders of magnitude, as shown in Table 7.2. Note however that the ratio y/% is of the same order as that of Na. These observations lead to the conclusion that at low temperatures these systems have extremely large density of states N(0) on the Fermi surface. In other words, they are described as liquids of dressed fermions whose effective mass m* is 102 ~ 103 times larger than the electron mass m. This has been confirmed by transport phenomena data, in particular measurement of the de Haasvan Alphen effect. Moreover, many of these systems undergo a phase transition to an antiferromagnetic state or a superconducting state at low temperatures. There are systems such as UPt3, which become superconducting, that show strong antiferromagnetic (large q) as well as paramagnetic (small q) fluctuations, as observed by neutron scattering. It is characteristic of these materials that the amplitude of the magnetic moment in the antiferromagnetic state is reduced by 1/2 ~ 1/10 from the atomic value. The reason why they become heavy fermion systems at low temperatures and why antiferromagnetism with a small magnetic moment appears are discussed in [A6] and will not be discussed here. Instead, we will be concerned here with the superconducting properties of heavy fermion systems. It should be added, however, that in a heavy fermion system the mixing of the s and delectrons with large band widths and the felectrons is extremely small. Consequently the Coulomb repulsion between the felectrons on the same site is large and hence the system is strongly correlated. In the latter sense, therefore, the system corresponds to a threedimensional version of the model Hamiltonian (7.1) with the replacements d —• f and p —• s and with the condition t&
7.3 Superconductivity in heavy electron systems
0.5 T (K)
179
1.0
Fig. 7.17. The temperature dependence of the specific heat of UBe^. The solid line is the theoretical curve assuming the ABM state of the 3 P pairing. (From [G30].)
73.1 The superconducting state It is important, first of all, to note that it is the heavy electrons that become superconducting since the specific heat jump AC at the transition temperature Tc is of the order of C(TC), see Fig. 7.17. The question is the type of pairing. The clue to this is the temperature dependence of various physical quantities. Such quantities as the specific heat C, the magnetic susceptibility /, the ultrasound attenuation coefficient a, the NMR relaxation rate T^ 1 and so on decrease exponentially at low temperatures in an swave superconductor due to the energy gap as described in Chapter 3. In contrast with this, it is possible that the energy gap vanishes on points or along lines on the Fermi surface for a nonswave pairing as noted in Chapter 6 for the superfluid 3 He with a 3 P pairing. As shown in Table 7.3, the above quantities in such a state decrease in powers of T (T2 for the points and T 3 for the lines) instead of exponential dependence on T. Figure 7.18 depicts the temperature dependence of T^1, which does not show growth due to the swave coherence factor just below Tc, as does a copper oxide superconductor. In addition to these, the temperature dependences of HC2(T) and the London penetration depth X(T) are reported to deviate from those of the BCS theory. Thus it seems that a nonswave pairing is responsible for the superfluidity in many heavy fermion systems. Especially in the cases of UPt3 and Ui_ x Th x Bei3 (x ~ 0.02 — 0.04), which show more than two superconducting phases, this is beyond any doubt. The temperature dependence of the specific heat of UPt3 is shown in Fig. 7.19. One sees there are two peaks in the curve. The phase diagram (Fig. 7.20) in the H — T plane has been obtained from this measurement
New superconducting materials
180
Table 7.3. The antiferromagnetic transition temperature T (the Neel temperature) and the superconducting critical temperature Tc. The symbol x denotes that the corresponding phase transition has not been observed to date. The third column denotes the temperature dependence of the specific heat C(T < Tc)
T N (K)
CeCu2Si2 URu 2 Si 2 UPt 3 UBei 3 UNi 2 Al 3 UPd 2 Al 3 UCdn CeAl3
(0.7?) 17 5 ?
4.6 14 5
0.65 1.5 0.5 0.9 1.0 2.0
X
T2 T2
X X
1000 r
9 ioo 
1
Fig. 7.18. The spin relaxation rate of
195
Pt in UPt 3 . (From [G31].)
as well as the ultrasound attenuation and the thermal expansion coefficient. According to this diagram, there are three superconducting phases A, B and C and four boundary lines sharing a single critical point. It seems that the superconducting phase of UPt 3 has a multicomponent order parameter, i.e., has a nonswave pairing, since there are several superconducting phases. This is analogous to the A phase of superfluid 3 He, which splits into A
7.3 Superconductivity in heavy electron systems
181
0.8
:0.4
H=0 H=2.5T //=6.25T
>JO.2 0.0
0.0
0.2
0.4 T(K)
0.6
Fig. 7.19. The specific heat of UPt3. Observe that there are two jumps. The jumps shift towards lower temperatures in the presence of a magnetic field. (From [G32].)
0.2
T(K)
0.4
Fig. 7.20. The phase diagram of UPt3 obtained from the specific heat, the upper critical field H& and the ultrasound attenuation. It is considered that there are three distinct superconducting phases A, B and C. (From [G32].)
phase and Ai phase in the presence of a magnetic field. It is estimated from HC2 values at low temperatures that £o ~ 300 A and K > 1 since AL, being proportional to sfm*, is large. Accordingly in the phase diagram the system is thought of as in a vortex lattice state in the region with a finite magnetic field. What is the mechanism for superconductivity in these systems? At temperatures (energies) sufficiently lower than the Kondo temperature TK, the system is regarded as a Fermi liquid made of heavy electrons and /CB TK is considered to play the role of the Fermi energy s?. The energy /CBTK is smaller than the Debye phonon energy con in many heavy electron systems. There
182
New superconducting materials
fore the number of phonons contributing to the attraction between electrons is limited and, moreover, the retardation effect cannot be expected, which makes superconductivity by the phonon mechanism less probable. Rather it is expected that spin fluctuations play the central role since electrons in the system are strongly correlated. Note, however, that even the theory of a heavy electron system in the normal state is still incomplete and hence the quantitatively correct microscopic theory of the superconducting state has not yet been obtained. Therefore semiphenomenological considerations using the group theoretical classification are now exclusively employed; the elements of this will be briefly surveyed next. 7.3.2 Symmetry of pairing in crystal Pairing has been considered in Chapter 2 with assumptions that the system is invariant under an arbitrary space rotation and, in particular, that the interaction between particles is written in the form of Eq. (2.12), namely + l)ViPi(k9k\
(7.3)
where V\ is regarded as a constant for fc,fc' ~fepThe gap equation in the BCS weakcoupling theory in this case takes the form (2.58) for both a spinsinglet (S = 0) pairing and a spintriplet (S = 1) pairing. Moreover, the equation which determines Tc is obtained from Eq. (2.60) as
Kp(k) = ^c"1 J dnk,V(kX)Kp(k)
(7.4)
since one may put Ska = l&al Here vc is given by l
3 cocpc)
in the weakcoupling theory and the integration yields the angular average over the Fermi surface. This is therefore a linear eigenvalue equation to determine j8c = (fesTc)"1. Determining the kind of superconducting states obtained as a solution to this equation is the same problem as the classification of wave functions according to the symmetry of the Hamiltonian and can be dealt with by obtaining irreducible representations of the symmetry group. It is wellknown that there is a 2 x (2/ + l)dimensional irreducible representation for a spin singlet (S = 0) pair and a 2 x 3 x (2/ + l)dimensional one for a spin triplet (S = 1) pair for each / if the system is isotropic. For instance, the 3 Ppair can be represented by nine complex quantities A^j. All the states belonging to the same irreducible representation have the same Tc while those with different /
7.3 Superconductivity in heavy electron systems
183
have different Tc. In other words, / (and S) specifies a degenerate class. There are thus infinitely many possible classes since the only requirement is an attractive V\. Then what kind of superconducting state is realised in a given crystal and how many classes of degenerate states are possible? It must be assumed, when considering the pairing in a crystal, that the density of states of the pairing electrons, the interaction between electrons and so on have only the same symmetries as those of the crystal. Let us restrict ourselves to the case of a uniform superconducting state without an external field. Suppose for simplicity that the spinorbit interaction is so strong that the invariance under separate rotations of the orbit space and the spin space of the pairs is frozen. (It should be noted, however, that spinorbit interaction in UPt3 is weak according to recent research and hence the relative rotation between the spin and orbit spaces must be considered.) Then the symmetry under question in the 'symmetry breaking' due to pairing is the product of the rotational symmetry Gp of the crystal, the gauge transformation and the time reversal, Gp x 1/(1) x T.
(7.5)
An example of timereversal symmetry breaking is the case with nonunitary pairing (A* ^ A), see Section 2.3.1. Since the order of the point group Gp is finite, there are only a finite number of possible classes in contrast with an isotropic case (the degrees of freedom such as those represented by f(k) in Eqs. (7.6) and (7.7) below are not considered). Note also that such expressions as the swave pair and the pwave pair in a crystal do not have the same meaning as in an isotropic case. Leaving detailed discussions to [E7], [E8] and [E9], let us consider a crystal with a simple cubic symmetry by way of example. In the case where Gp is the point group of a simple cubic system, there are five irreducible representations both for S = 0 and S = 1 and therefore there are five classes of states with different T c. These are two 1dimensional representations, one 2dimensional one and two 3dimensional ones. Here we list the bases of the 1dimensional representations only: S=0
A(k) = f(k)
(7.6a)
S = 1 \(k) = (xkx + yky + z kz)f(k) S =0
(7.6b)
A(*) = (kx2  ky2)(ky2  kz2)(kz2  kx2)f(k) 2
2
S = 1 A(*) = {5tkx(ky  k ) + yky{k 2
(7.7a)
2
2
 kx ) 2
+zkz(kx ky )}f(k\
(7.7b)
where \(k) is the dvector defined by Eq. (2.40) and f(k) is a function with
184
New superconducting materials
a cubic symmetry. The base (7.6a) corresponds to swave superconductivity while Eq. (7.6b) is similar to the order parameter of the BW state (6.15) of the superfluid 3 He. The gaps of Eq. (7.6) are finite everywhere on the Fermi surface while those of Eq. (7.7a) and Eq. (7.7b) vanish along lines and on points on the Fermi surface respectively. This is due to the loss of independence of the rotations and the gauge transformations as was shown in the ABM state of the superfluid 3 He. It should be noted that the gap may vanish on points or along lines in a superconductor without internal degrees of freedom (where the only degree of freedom is the overall phase). Let us give another example. Suppose we require in a hexagonal lattice system such as UPt3 that the gap should vanish along a line so that the specific heat at T < Tc is proportional to T2 and, also, that there are more than two phases. Then the twodimensional representation with a twocomponent order parameter given by A(k) = mkzkx + nikzky
(7.8a)
is the simplest form if we assume spin singlet (S = 0) pairing. (The function corresponding to f(k) above is set equal to unity.) The coefficients r\\ and r\i represent the twocomponent degrees of freedom. If, on the other hand, a spintriplet pairing is assumed, it takes the form called E2U given by
A(*) = zkz {m(k2x  k2y) + r,22kxky} .
(7.8b)
Recently, in [G33], the Knight shift of 195Pt in UPt3 has been measured down to 28 K and it was found that it does not change even in a superconducting state. If this observation is confirmed, the pairing in UPt3 would be of spintriplet form with odd parity. Whether this pairing is unitary or not is also discussed. The gap equation becomes nonlinear at T < Tc and the states which are degenerate at Tc no longer have the same free energy. The BW state or the ABM state in 3 He is a class of states as discussed in Chapter 6 and all the states belonging to the same class have the same free energy. The class forms a representation of a subgroup of the original group of symmetries. Ordinarily, using the free energy of the GL theory which retains the A4 or A6 terms, we try to find, with the help of group theory, possible classes of the order parameter and the associated energy gap in various crystals. In a system with coexisting ferromagnetism or antiferromagnetism, one has to take into account its order parameter and the coupling with the superconducting order parameter. The coupling between the altered crystal structure and the anisotropic superconductivity is possibly an interesting question for the future.
Appendix 1 BoseEinstein condensation in polarised alkaline atoms
A l . l Condensate in confining potential
This subject is directly related to Chapter 1 of this book and will be briefly summarised here although it has already been treated in an appendix of [Ell]. Spin polarised hydrogen H [ is listed in the right hand column of Table 1.1 as a system predicted to show Bosetype superfluidity. BoseEinstein condensation was observed, somewhat unexpectedly, in spin polarised alkaline gases Lij, Naj, and RbJ, with quite an ingenious method using laser light, prior to observation in H j gas (see [Hl] [H3]). It is unquestionable that the macroscopic wave function appears although superfluidity has yet to be observed. See [H4] for works on Hj, and related systems preceding this breakthrough. In a typical experiment the magnetooptical trap, which we can approximate by an anisotropic 3dimensional harmonic oscillator potential, is used to provide the confining potential for atoms. Its spatial scale is given by R ~ (fr/mco)1/2 ~ 10~3 cm, where m is the mass of the atom while <x> is the frequency of the harmonic oscillator. There are N ~ 106 atoms trapped in a volume ~ i? 3, for which the BoseEinstein condensation temperature TBE given by Eq. (1.3) is of the order of 10~7 K for Rb atoms. It should be added that evaporation cooling, which has been used to cool H j gas, is required in addition to laser cooling to reach this temperature. The condensate is described by the ground state wave function xpo in the trapping well provided that interatomic interaction is neglected. It takes the form ipo oc exp{—mcor 2/2h} if the potential is of the harmonic oscillator type, where the anisotropy is absorbed in rescaling. The atomic density at the centre is nc ~ \xpo(O)\2, which is approximately 5 x 10 14 cm~ 3 in an actual experiment. 185
186
BoseEinstein condensation in polarised alkaline atoms
In reality, there is an interatomic interaction. A repulsive force acts between two polarised (i.e., spinaligned) 87 Rb atoms, for example, and the scattering length for a low energy spintriplet swave is known to be a ~ lOOao, where ao is the Bohr radius. If the healing distance £ is evaluated according to Eq. (1.9) with density nc at the centre, one obtains £ ~ 10~3 cm. Therefore R may or may not be larger than £ depending on individual cases. Let V(x) be the confining potential energy. The equation that determines the condensate wave function \ps(x)9 corresponding to Eq. (1.8), is = 0.
(Al.l)
The first term is negligible if £ is sufficiently smaller than R, for which case the density of the condensate ns(x) = \xps(x)\2 is given by
Therefore the density profile of atoms is given by the inverted potential at low temperatures (T
A1.2 Dynamics of dilute BE condensate Once the BE condensation of a gas of polarised alkaline metal is observed, it is quite natural that the dynamic properties of the gas should be studied, see [H5] and [H6]. It is the collective motion of the condensate at low temperatures T
_
1,2_,
which is called the GrossPitaevskii equation in superfluid helium research. Suppose there is a condensate represented by the solution xps(x) of Eq. (Al.l). To study the motion of a small deviation from the condensate solution, that is, a low energy excitation, let us put the wave function of the deviation as xp  xps = (j)Qicot
(A1.4)
A1.2 Dynamics of dilute BE condensate
187
where the condition \(f>\
and a similar equation for 0*. Here tps = y/no(x) is assumed to be real for simplicity. Let us next consider what excitations are obtained for a uniform dilute Bose gas (i.e., V(x) = 0 and no = ns). Since the system is uniform, the wave function (/> is a plane wave (/> oc Q1P'x/n. The corresponding excitation spectrum, found from Eq. (A 1.5) is
where e^ = p2/2m. It turns out from Eq. (A 1.4) that this excitation is a density fluctuation, namely a phonon, and from Eq. (A1.6) that the energy approaches cp in the long wavelength limit (p —> 0). Here the sound velocity c is given by c = h/m^ = ^/nsg/m. This fact is essential in superfluidity, see Section 1.4 where it has been shown that the elementary excitation energy in the rest frame is given by sp + p • Vs when the whole system moves with velocity F s . Here p and sp are quantities in the frame moving with velocity F s . If the spectrum is of the phonon type sp = cp, as in the present case, the system energy cannot be lowered by creating an elementary excitation when  Vs\ < c. In other words, the flow does not decay. We should note that interaction must be present for the phonon velocity to be finite. It should also be added that the Bogoliubov transformation defined in Section 2.4 was first introduced to obtain the spectrum (A1.6) from Eq. (A1.5) in a dilute Bose gas model. The situation becomes far more complicated in the case of a condensate in a magnetooptical trap. Lower frequency collective excitations can also appear as deformations of the condensate. Let us estimate the order of the frequency cos when R > £ is satisfied. Note first that cos is given by the inverse of the time with which a phonon propagates through a system of size R. Therefore it follows that co"1 ~ R/c. Suppose the trapping potential is of the harmonic oscillator type with V ~ ^<£§r2 and the radius R is defined by the radius for which n(r) = 0 in Eq. (A1.2). Then one finds R ~ c/a>o and, as a result, cos ~ coo. Note that this is independent of the density of the condensate. In fact, it has been shown that, when the potential is of the harmonic oscillator type, there is a mode with frequency 2coo? which corresponds to oscillation of the condensate without change of shape.
188
BoseEinstein condensation in polarised alkaline atoms
Experimentally, a collective motion may be excited by applying a magnetic field with an appropriate frequency. The results obtained so far seem to roughly agree with theoretical results based on the nonlinear Schrodinger equation, see [H7]. Even when hydrodynamic collective motion is observed with no BE condensate, it has been confirmed that the frequency shifts as the system undergoes condensation. It is also observed that the lifetime of a collective motion becomes much longer in the presence of a condensate. Superfluidity in the present system has not yet been observed. To confirm superfluidity explicitly, one must check whether or not the circulation around a vortex line, generated by rotation, is quantised in units of K defined by Eq. (1.2). For example, it is expected that a single quantised vortex line appears in the condensate at angular frequency fici, which corresponds to Hc\ in a type 2 superconductor, and one can then observe the change in density distribution of the condensate associated with it. We also expect that there is a phenomenon similar to the Josephson effect when two condensates, separated spatially, are weakly coupled. To close this brief review we should note that attempts are being made to extract a coherent atom pulse, that is, a pulsed atom laser from the trapped condensate (see [H8] for example).
Appendix 2 Recent developments in research on high temperature superconductors
A2.1 Pair structure of high temperature superconductors and Josephson effects It is current opinion that the pair in a copper oxide superconductor is not spinsinglet swave type but has the symmetry of a spinsinglet dwave pair. It is considered, from the temperature dependence of the specific heat, the penetration depth, nuclear magnetic relaxation rate and so on, that the energy gap vanishes on points or lines on the Fermi surface (see Section 7.2). Recent experiments using angular resolution photoelectron emission revealed that the gap is vanishingly small in the diagonal directions, fcx = \ky\. These facts may be explained if the order parameter A(k) in momentum space takes the dwave form A(k) = (cos kx  cos ky) A
(A2.1)
with the /cdependence shown in Fig. A2.1(a). Here the system is regarded as twodimensional and the x and yaxes are taken as in Fig. 7.7. Let us recall that A is a complex number and the spatial variation of its phase x produces the supercurrent. The above experiments can also be accounted for by swave pairing with quite a large anisotropy as shown in Fig. A2.1(b). Theorists are of the opinion that antiferromagnetic fluctuations, which result in dwave pairing, are important in copper oxides, although there is no direct evidence for the claim so far. From 1993 onwards, there have been several experiments making use of the Josephson effect to determine the structure of the pairing. These experiments have produced interesting results that will be outlined below. If the pairing takes the form shown in Fig. A2.1(a), then the order parameter changes sign, in other words, the phase changes by n depending whether k is directed towards the aaxis or the fcaxis in the CuC>2 plane. One may 189
190
Recent developments in HTSC research ky
ky
Fig. A2.1. (a) The amplitude and signature of the dwave pairing on the Fermi surface, (b) The amplitude of the anisotropic swave pairing.
conclude that the pairing is not swave but dwave if this phase difference is detected experimentally. The simplest experiment employs the tunnelling device shown in Fig. A2.2, see [H9]. Here a loop is made of the tunnelling junctions of an swave superconductor such as Pb attached to the faces a and b of a single crystal of a highT c superconductor (YBCO in this experiment). We expect that electron pairs whose momenta (k, —k) are perpendicular to the face of the junction mainly tunnel through (although it seems that for the present this claim is not clearly founded on microscopic theory). If this is the case, the phase of the pair tunnelling through the side a into YBCO is different by n from the phase of that through b. In other words, the phase of a pair when it goes around the loop changes by n. As a consequence, the loop must carry current. In the limit of a large selfinductance, this current produces a stable state with a flux 0o/2 (0o = hc/2e) even without an external magnetic field. One would like to detect this flux but in practice this is not easy, due to problems associated with residual magnetic flux or flux due to the measurement current. Accordingly the method employing the interference effect, introduced in Section 3.4, is used, see [H10]. One may assume that variation in the phase % takes place only at the two tunnelling junctions in the loop of Fig. A2.2 as assumed in Section 3.4. Then it holds that =
2TT,
(A2.2)
where is the flux through the loop in the unit of <£o The parameter 5 is + 1 if the phase change n (7rshift) is associated with YBCO in the right side (R) of the junction, while d = 0 if the order parameter of R is of swave type. Let us assume for simplicity that the two junctions have the same
A2.1 Pair structure of HTSC and Josephson effects y
YBCO single crystal
191
SNS Josephson tunnelling junction
Pb thin film
Fig. A2.2. A loop with 7rshift. (From [H9].)
characteristics. The bias current / from left to right in this case is given by
where Ic is the critical current of each junction and Xo
=
If S = 0, one reproduces the result I /Ic = 2sinxocos7r0
(A2.4)
obtained in Section 3.4, while if 8 = +1 one has I/Ic = 2 cos #o sin 7T0.
(A2.5)
/ for S = 0, from which Figure 3.10 shows I/Ic as a function of the flux <> we see maximal values occur when <> / is an integer. In contrast, it takes a maximal value when <\> is a halfodd integer if b = + 1 . Thus the difference shown in Fig. A2.3 must occur. In other possible experiments we measure with the help of another SQUID the magnetic flux produced by the current circulating in the loop when the bias current is kept at zero; see [Hll]. We will not go into details of the experimental results here. Although most results favour dwave pairing, there is a report [H12] in which the 7rshift has not been observed. The above Josephson circuit is symmetric with respect to timereversal transformation. A state with the bias current / and the magnetic flux dfo is mapped to a state with reversed current —/ and reversed flux — 8(j)o under time reversal. If a circuit is made of an ordinary superconductor, a state with S = 0 is mapped to itself, while a state with the 7ishift is necessarily mapped to a different state. For example, a state with n = 1 is mapped to
192
Recent developments in HTSC research s wave
321
0
1 2
3 d wave
 3  2  1 0 1 2 3 Fig. A2.3. The critical current as a function of the flux through the loop. that with n = — 1, see [H13]. Note also that superconductivity with such a complex order parameter as A(jfc) = (kl — k2)A\ + \kxkyA2 or A(k) = (k2xk2y)
A,+iAs
does not have this symmetry (unless A2 —> — A2 and As > —A s under time reversal). This observation may be one of the clues to identify the symmetry of the pair. So far we have discussed the spatial structure of the order parameter, that is, the ^dependence of the pair wave function. On the other hand, the codependence of A as mentioned in Chapter 4 is also interesting in HTSC. However the experiment seems to be difficult in HTSC since the coherence length is extremely small. A2.2 High temperature superconductor in a magnetic field The characteristics of a high temperature superconductor in a magnetic field have been studied in Section 7.2, where it was pointed out, in conjunction with its peculiar layered structure, that fluctuations are quite important and that there is a possibility that an ordinary Abrikosov lattice melts to form a vortex liquid state. This unique physics, realised for the first time due to the discovery of HTSC, has been actively studied since then and interesting
A2.2 High temperature superconductor in a magnetic
field
193
results obtained. Although this can be observed in YBCO, most studies have used a typical HTSC, BSCCO (Bi2Sr2CaCu2O8). The latter has a strong anisotropy and the effect of fluctuations is far more important. An ordinary type 2 superconductor undergoes a second order phase transition at a temperature T determined by H = HC2(T) in the presence of an external field H and is in the Abrikosov vortex lattice state below that temperature. In contrast with this, there does not exist such a phase transition in HTSC when a magnetic field is applied parallel to the oaxis. Rather it undergoes continuous transition from the normal state to the vortex liquid state. A vortex lattice state should appear, however, as the temperature is further lowered. Then it is conjectured that, in an ideal system without such effects as a pinning, there exists a clearcut thermodynamic phase transition between the vortex liquid and the lattice. It is also likely that the transition is of the first order, like an ordinary liquidgas transition, since the transition from the normal state is pushed down to low temperatures by the effect of fluctuations. These predictions have been based mainly on the temperature dependence of the electrical resistivity in a magnetic field. Recently they were confirmed directly by thermodynamic measurements and quite interesting facts have come to light. In [H14], an external field H(\\ c) was applied to a planar BSCCO crystal (T c = 90 K) perpendicular to the caxis and the magnetic flux density B at the sample surface was measured with precision making use of the Hall effect of the twodimensional electron system in GaAs. Figure A2.4 shows the sharp jump in the flux density B observed as the temperature is lowered, while Fig. A2.5 is the phase diagram in the temperaturemagnetic field plane. This is the first order phase transition, since B has a jump, and B is larger on the liquid side where the vortex density is larger, as in the waterice transition. The jump in Fig. A2.4 corresponds to an entropy jump AS = 0.3/CB per vortex line whose length is the interlayer distance. Note that the melting curve Bm(T) is far below HC2(T) in BSCCO. What is more interesting is that this melting curve looks as if it ends at the critical point (T = 37 K and B = 380 G). In other words, the jump in B disappears there. It may be possible that the phase transition is of the second order beyond this point due to the effect of randomly distributed defects. How is the phase transition between the vortex liquid and the vortex lattice reflected in the electrical resistance? Let us note that a similar first order phase transition is also observed in a clean YBCO. Figure A2.6 shows the temperature dependence of the electrical resistance along with the jump in magnetisation, see [H15]. It can be seen from this that the resistivity suddenly disappears as the
Recent developments in HTSC research
194
44.4 :
o 44.2
:
44.0
81.75
81.80 81.85 T (K)
81.90
Fig. A2.4. A jump in the magnetic flux density B observed as the temperature is lowered with an external magnetic field of 53 Oe (note that 1 G = 10~4 T). (From [H14].) 500 400
\
ou 40 20
\
Q 300 200
critical point ^5
40
50
60
. . .,
1 •


>
:
s •s n
100 0
•
AH
•
•
•
I
80
70
•
i
i
. •
85
80
90 ;
90
T (K) Fig. A2.5. Phase diagram showing the phase boundary between the vortex lattice and the vortex liquid in BSCCO. (From [H14].)
vortex liquid solidifies. It is considered as the origin of this behaviour that the pinning mechanism starts to work as the vortices form a lattice with stiffness and the decay of current due to vortex motion is then forbidden. It is also shown in Fig. A2.7 that the changes of if and T and the measurement of p all give the same melting curve. The jump disappears if the sample is irradiated by an electron beam to create defects, after which p(T) approaches zero as T is lowered. It seems that the pinning mechanism does not work efficiently in BSCCO and the discontinuous change in p has not been observed. Another possible origin of the phase transition, which is not considered above, is that the links of the vortex lines in different layers may collectively
^42.2 High temperature superconductor in a magnetic field 1 0
0.8
1
• :
5.6
4.2 2.9 1.8T
195
'' '
HWc
'•
1 0.4 ': 5 0.2
"
"
K
8
I
/

0 60 50 ;
1 40
Js=0.65 A/cm2 //lie
d so
>
•v 1
~a 20 10
wa'.' '
%
•5.6! 4.21 2.911.8/
0 80
85
r(K)
0.4/0.2IOT95
90
Fig. A2.6. The jump in magnetisation and disappearance of the electrical resisitivity p in YBCO. The numbers in the figure denote the magnitude of the external field (H ~ M). (From [H15].) A Hm obtained from M{H\ o Tm obtained from M(T) obtained from p(T) •
86 88 T(K)
92
Fig. A2.7. The melting curve of the vortex lattice in YBCO obtained from magnetisation and resistivity measurements. disappear. It may also be expected that the vortex glass state appears in a disordered crystal. So far the theories related to these problems are either phenomenological or based on simulations. It is interesting to analyse theoretically how the phase correlation between order parameters at two points
196
Recent developments in HTSC research
H
Fig. A2.8. CuO2 sheets coupled through Josephson junctions.
separated by R and the correlation of the positions of the vortex centres change as R increases. The former is the very parameter that characterises superconductivity and superfluidity. These correlations should, of course, behave differently in a clean system and in a disordered system. It seems that the entire picture of the physics of the vortex state in HTSC is yet to be clarified. A2.3 Supplement to research in highTc superconductors 1. It was reported in Chapter 7 that the superconductor with the highest Tc was Bi2Sr2CaCu2O8 with Tc = 125 K. Shortly after this discovery, it was found that a group of materials with similar structure but incorporating mercury becomes superconducting (1992). Among others, HgBa 2 Ca2Cu 3 08x is found to have Tc ~ 135 K (~ 150 K under pressure). This record is not broken at the moment (see [H16]). Unfortunately this material is unstable and a good sample cannot be prepared. Thus its properties are seldom studied. 2. It was found recently that Sr2RuC>4, which has a layered perovskite structure like La2CuO4 with Cu substituted by Ru in the platinum group, becomes superconducting below Tc ~ IK, see [H17]. This material has a structure shown in Fig. 7.6(a) with La substituted by Sr and Cu by Ru and shows strong twodimensionality even without doping (see [H18]), in contrast with La2CuO4, which becomes conducting only when La is substituted by Sr by doping. The low Tc ~ I K suggests that what is important for highT c superconductivity is not simply a layered structure but the existence of the CuC>2 sheets.
A2.3 Supplement to research in highTc superconductors
197
3. HTSC has a strong twodimensionality due to the layered structure. It has been considered in particular that the superconducting properties may be explained by regarding the system as weakly coupled CuC>2 sheets. If this is the case, it may be possible to observe the Josephson effect due to the microscopic structure itself. Recently, as microfabrication technology has advanced, a sample with a few tens of microns edge size and less than 100 CuC>2 sheets has been made and the d.c. and a.c. Josephson effects were indeed observed. Figure A2.8 shows the schematic diagram of the system. The current / = IC(H) is measured in the d.c. mode. This effect is also observed in both BSCCO and YBCO with weaker interlayer coupling made by reducing oxygen atoms, see [H18].
References and bibliography
Books on manybody problem and related subjects [Al] A.A. Abrikosov, L.E. Dyaloshinskii and L.P. Gor'kov: Methods of Quantum Field Theory in Statistical Physics (Dover, New York 1963). A typical textbook on the manybody problem based on the Green's functions. Fermi liquids, superfluidity of Bose systems and superconductivity are treated in detail. [A2] A.A. Abrikosov: Fundamentals of the Theory of Metals (NorthHolland, Amsterdam 1988). A thick book with 630 pages. The first half (Part I) is devoted to the Fermi liquid theory of metals while the second half (Part II) covers the theory of superconductivity. [A3] P.W. Anderson: Basic Notions of Condensed Matter Physics (Benjamin, Menlo Park 1983). Unique expositions and a collection of original papers on symmetry breaking, Fermi liquid theory and other subjects. [A4] N.W. Ashcroft and N.D. Mermin: Solid State Physics (Holt, Rinehart and Winston, Saunders College, Philadelphia 1976). Chapter 35 provides an introduction to superconductivity. [A5] A. Fetter and J.D. Walecka: Quantum Theory of ManyParticle Systems (McGrawHill, New York 1971). A textbook similar to but easier to understand than [Al]. [A6] K. Yamada: Electron Correlation in Metals (Cambridge University Press, Cambridge, to be published). Books on superfluidity [Bl] K.H. Benneman and J.B. Ketterson: The Physics of Liquid and Solid Helium, Parts I and II (WileyInterscience, New York 1976). 198
References and bibliography
199
A collection of excellent expositions on superfluid 4He, normal and superfluid 3He. [B2] R J . Donnelly: Experimental Superfluidity (University of Chicago Press, Chicago 1967). The most easily understood book on superfluid 4He. [B3] R J Donnelly: Quantized Vortices in Helium II (Cambridge University Press, Cambridge 1991). An excellent book on the physics of superfluid 4He, which is only briefly treated in the present book. [B4] W.E. Keller: Helium3 and Helium4 (Plenum Press, New York 1969). A book covering the general aspects of helium systems, although slightly out of date. [B5] I.M. Khalatnikov: Introduction to the Theory of Superfluidity (Benjamin, New York 1965). ; The theory of superfluids with emphasis on hydrodynamic aspects. tB6] F. London: Superfluids (John Wiley, New York Vol. I 1950, Vol. II 1954). Vol. I is on superconductivity while Vol. II is on superfluidity of liquid 4He. These classics are worth reading, even today, [B7] D. Vollhardt and P. Wolfe: The Superfluid Phases of Helium 3 (Taylor and Francis, London 1990). An exposition of more than 600 pages exclusively on the research on superfluid 3He as of the end of the 1980s. [B8] H. Yukawa and T. Matsubara (eds.): Solid State Physics I (2nd edn) (Iwanami Series on Foundation of Contemporary Physics, Vol. 6, in Japanese) (Iwanami, Tokyo 1978). Chapter 3 'Physics of Helium System' and Appendix A 'Superfluid 3He' by the present author serve as moderate introductions. [B9] K. Yamada and T. Ohmi: Superfluidity (New Physics Series 28, in Japanese) (Baifukan, Tokyo 1995). An excellent book on superfluid helium published recently. Books on superconductivity [Cl] P. de Gennes: Superconductivity of Metals and Alloys (Benjamin, New York 1966), (Reprint, AddisonWesley, Reading 1989). A unique textbook, which contains a detailed account of the Bogoliubovde Gennes theory and the GL theory. [C2] R.D. Parks (ed.): Superconductivity, Vols. I & II (Marcel Dekker, New York 1969). A handbook of research in superconductivity as of the end of the 1960s. Contribu
200
References and bibliography
tions to these volumes are repeatedly cited when one discusses such topics as the strong coupling theory.
[C3] J.R. Schrieffer: Theory of Superconductivity (revised edn) (AddisonWesley, Reading 1983). An excellent textbook on the Green's function formulation of superconductivity and electronphonon interaction. [C4] M. Tinkham: Introduction to Superconductivity (McGrawHill, New York 1975). A wellpresented textbook. A detailed account of the Josephson effect is given. [C5] S. Nakajima: Introduction to Superconductivity (New Physics Series 9, in Japanese) (Baifukan, Tokyo 1971). Basic concepts are well explained. Although this book is meant to be an introduction, it is rather advanced. [C6] Japanese Physical Society (ed.): Superconductivity (in Japanese) (Maruzen, Tokyo 1979). A collection of expositions from foundations to applications. [C7] P.F. Dahl: Superconductivity (American Institute of Physics, 1992). A history from Onnes to HTCS.
Monographs on selected topics in superconductivity
[Dl] A. Barone and G. Paterno: Physics and Applications of the Josephson Effect (John Wiley, New York 1982). This book can be recommended as a detailed exposition on the Josephson effect. [D2] G. Grimvall: The ElectronPhonon Interaction in Metals (NorthHolland, Amsterdam 1981). A detailed account of electronphonon interaction in both normal and superconducting states. [D3] D.H. Douglass (ed.): Superconductivity in d andfBand Metals (Plenum Press, New York 1976). [D4] W. Buckel and W. Weber (eds.): Superconductivity in d and fBand Metals (Kernforschungszentrum, Karlsruhe 1982). The above two books give detailed accounts of superconductivity in transition metals and intermetallic compounds. [D5] B. Deaver and J. Ruvald (eds.): Advances in Superconductivity (Plenum Press, New York 1983). [D6] D. Saint James, G. Sarma and E. Thomas: Type II Superconductors (Clarendon, Oxford 1969). These are slightly oldfashioned textbooks on type 2 superconductors.
References and bibliography
201
[D7] D.N. Langenberg and A.I. Larkin (eds.): Nonequilibrium Superconductivity (NorthHolland, Amsterdam 1986). [D8] R. Tidecks: Nonequilibrium Phenomena in Superconductors (SpringerVerlag, Berlin 1990). The above two books explain such topics as TDGL, CarlsonGoldman mode and PSO in detail. [D9] V.L. Ginzburg and D.A. Kirzhnits (eds.): HighTemperature Superconductivity (English edn.) (Consultant Bureau, 1982). We list only the above book on HTSC research before the discovery of copper oxide highTc superconductors. [D10] T. Ishiguro and K. Yamaji: Organic Superconductors (SpringerVerlag, Berlin 1990). An uptodate review on organic superconductors. [Dll] J.C. Phillips: Physics of High Temperature Superconductors (Academic Press, London 1989). This book provides a good explanation of the physics of highTc superconductors, although from a restricted point of view. [D12] Proceedings of the 19th International Conference on Low Temp. Physics, Part III, Physica B169 (1991). [D13] S. Maekawa and M. Sato (eds.): Physics of HighTemperature Superconductors (SpringerVerlag, Berlin 1991). [D14] Proceedings of the International Conference on Materials and Mechanisms of Superconductivity, High Temperature Superconductors III, Part 1, Physica C189 (1991). The above three proceedings provided excellent coverage on the present status of research on highTc superconductors and heavy electron systems. [D15] K.S. Bedell, M. Inui and D.E. Meltzer (eds.): Phenomenology & Applications of High Temperature Superconductors (AddisonWesley, Reading 1992). [D16] High Temperature Superconductors, special issue in Solid State Physics (in Japanese) 25 (1990) 617. The above references contain convenient reviews for further, detailed study of HTSC. Further reading
The following references are listed to supplement the main text and to cover those topics that are not considered therein. [El] D.E. MacLaughlin: Magnetic Resonance in the Superconducting State, in Solid State Physics 31, edited by H. Ehrenreich, F. Seitz and D. Turnbull (Academic Press, London 1976).
202
References and bibliography
[E2] AJ. Leggett, S. Chakravarty, A.T. Dorsey, M.P.A. Fisher, A. Garg and W. Zwerger: Dynamics of the Dissipative Twostate System, Rev. Mod. Phys. 59 (1987) 1. [E3] P.B. Allen and B. Mitrovic: Theory of Superconducting Tc, in Solid State Physics 37, edited by H. Ehrenreich, F. Seitz and D. Turnbull (Academic Press, London 1982). [E4] WJ. Skocpol and M. Tinkham: Fluctuations near Superconducting Phase Transitions, in Report on Progress in Physics 38 Part 3, (1975). [E5] M.M. Salomaa and G.E. Volovik: Quantized Vortices in Superfluid 3 He, Rev. Mod. Phys. 59 (1987) 533. [E6] A.L Larkin and Yu.N. Ovchinikov: Pinning in Type II Superconductors, J. Low. Temp. Phys. 34 (1979) 409. [E7] G.E. Volovik and L.P. Gor'kov: Superconducting Classes in HeavyFermion Systems, Sov. Phys. JETP 61 (1985) 843. [E8] M. Sigirist and K. Ueda: Phenomenological Theory of Unconventional Superconductivity, Rev. Mod. Phys. 63 (1991) 239. [E9] M. Ozaki, K. Machida and T. Ohmi: Classification of superconducting pair function by symmetry, Solid State Physics (in Japanese) 23 (1988) 879. [E10] J. A. Sauls: The order parameter for the superconducting phases of UPt 3 , Adv. in Phys. 43 (1994) 113. [Ell] E. Hanamura: Quantum Optics (SpringerVerlag, Berlin, to be published). Collections of original papers (Circulated only in Japan) [Fl] Superconductivity, Collected Papers in Physics 153 (Japanese Physical Society, Tokyo 1966). [F2] Quantum Fluids, Collected Papers in Physics: New Edition 43 (Japanese Physical Society, Tokyo 1970). [F3] Superfluid 3 He, Collected Papers in Physics 190 (Japanese Physical Society, Tokyo 1975). [F4] Physical Properties of Organic Superconductors, Collected Papers in Physics I (Japanese Physical Society, Tokyo 1992). References in text [Gl] J.G. Bednorz and K.A. Muller: Z. Phys. B 64 (1986) 189. [G2] H.F. Hess, R.B. Robinson, R.C. Dynes, J.M. Valles, Jr. and J.V. Waszczak: Phys. Rev. Lett. 62 (1989) 214. [G3] A.D.B. Woods and R.A. Cowley: Canad. J. Phys. 49 (1971) 177.
References and bibliography
203
[G4] V. Fock: Z.fur Physik, 98 (1936) 145. [G5] N.E. Phillips: Phys. Rev. 114 (1959) 676. [G6] R.W. Morse and H.V. Bohm: Phys. Rev. 108 (1957) 1094. [G7] G.J. Dick and F. Reif: Phys. Rev. 181 (1969) 774. [G8] R.H. Hammond and G.M. Kelly: Phys. Rev. Lett. 18 (1967) 156. [G9] Y. Masuda and A.G. Redfield: Phys. Rev. 125 (1962) 159. [G10] L.C. Hebel and C.P. Slichter: Phys. Rev. 113 (1959) 1504. [Gll] W.H. Parker, D.N. Langenberg, A. Denenstein and B.N. Taylor: Phys. Rev. Ill (1969) 639. [G12] J. Kwo and T.H. Geballe: Phys. Rev. B23 (1981) 3230. [G13] R.P. Groff and R.D. Parks: Phys. Rev. 176 (1968) 567. [G14] A.A. Abrikosov: Soviet PhysicsJETP 5 (1957) 1174. [G15] J.D. Meyer: Appl. Phys. 2 (1973) 303. [G16] R.J. WattsTobin, Y. Krahenbuhl and L. Kramer: J. Low Temp. Phys. 42 (1981) 459. [G17] W.P. Halperin, C.N. Archie, F.B. Rasmussen, T.A. Alvesalo and R.C. Richardson: Phys. Rev. B13 (1976) 2124. [G18] J.E. Berthold, R.W. Giannetta, E.N. Smith and J.D. Reppy: Phys. Rev. Lett. 37 (1976) 1138. [G19] A.I. Ahonen, T.A. Alvesalo, M.T. Haikala, M. Krustus and M.A. Paalanen: Phys. Lett. 51A (1975) 279. [G20] M.M. Salomaa and G.E. Volovik: Rev. Mod. Phys. 59 (1987) 533. [G21] V.P. Mineev, M.M. Salomaa and O.V. Lounasmaa: Nature 324 (1986) 333. [G22] K. Shimizu, N. Tamitani, N. Takeshita, M. Ishizuka, K. Amaya and S. Endo: J. Phys. Soc. Jpn. 61 (1992) 3853. [G23] W. Little: Phys. Rev. 134 (1964) A1416. [G24] A.W. Sleight, J.L. Gillson and P.E. Bierstedt: Solid State Commun. 17 (1975) 27. [G25] K. Kadowaki, J.N. Li and J.J.M. Franse: Physica C170 (1990) 298. [G26] Y.J. Uemura: Physica B169 (1991) 99. [G27] T. Hasegawa: Proc.USJapan Seminar on the Electronic Structure and Fermiology of HTSC, 1992. [G28] Y. Kitaoka, K. Ishida, S. Ohsugi, K. Fujiwara and K. Asayama: Physica C185189 (1991) 98. [G29] J.N. Li, K. Kadowaki, M.J.V. Menken, A.A. Menovsky and J.J.M. Franse: Physica C161 (1989) 313. [G30] H.R. Ott, H. Rudigier, T.M. Rice, K. Ueda, Z. Fisk and J.L. Smith: Phys. Rev. Lett. 52 (1984) 1915.
204
References and bibliography
[G31] Y. Kohori, T. Kohara, H. Shibai, Y. Oda, Y. Kitaoka, K. Asayama: J. Phys. Soc. Jpn. 57 (1988) 395. [G32] K. Hasselbach, L. Taillefer and J. Flouquet: Phys. Rev. Lett. 63 (1989) 93. [G33] H.Tou, Y. Kitaoka, K. Asayama et al: Phys. Rev. Lett. 77 (1996) 1374. References in appendices [Hl] M.H. Anderson, J.R. Ensher, M.R. Matthews, C.E. Wieman and E.A. Cornell: Science 269 (1995) 198. [H2] K.B. Davis, M.O. Mewes, M.R. Andrews el al: Phys. Rev. Lett. 75 (1995) 3969. [H3] M.O. Mewes, M.R. Andrews, N.J. van Druten, D.M. Kurn, D.S. Durfee, and W. Ketterle: Phys. Rev. Lett. 11 (1996) 416. [H4] A. Griffin, D.W. Snoke and S. Stringari: BoseEinstein Condensation (Cambridge University Press, Cambridge 1995). [H5] D.S. Jin, J.R. Ensher, M.R. Matthews, C.E. Wieman, E.A. Cornell: Phys. Rev. Lett. 11 (1996) 420. [H6] M.O. Mewes, M.R. Andrews, N.J. van Druten, D.M. Kurn, D.S. Durfee and W. Ketterle: Phys. Rev. Lett. 11 (1996) 988. [H7] S. Stringari: Phys. Rev. Lett. 11 (1996) 2360. [H8] M.O. Mewes, M.R. Andrews, D.M. Kurn, D.S. Durfee, C.G. Townsend and W. Kettlerle: Phys. Rev. Lett. 78 (1997) 582. [H9] D.A. Wollman, D.J. Van Harlingen, W.C. Lee, D.M. Ginsberg and A.J. Leggett: Phys. Rev. Lett. 71 (1993) 2134. [H10] J.H. Miller, Jr., Q.Y. Ying, Z.G. Zou et al: Phys. Rev. Lett. 74 (1995) 2347. [Hll] A. Mathai, Y. Gim, R.C. Black, A. Amar and EC. Wellstood: Phys. Rev. Lett. 74 (1995) 4523. [H12] R. Chaudhari and S.Y. Lin: Phys. Rev. Lett. 72 (1994) 1084. [H13] M. Sigirist, D.B. Bailey, R.B Laughlin: Phys. Rev. Lett. 74 (1995) 3249. [H14] E. Zeldov, D. Majer, M. Konczykowski, V.B. Geshkenbein, V.M. Vinokur and H. Shtrikman: Nature 375 (1995) 373. [Hl5] U. Welp, J.A. Fendrich, W.K. Kwok, G.W. Crabtree and B.W. Veal: Phys. Rev. Lett. 76 (1996) 4809. [H16] E.V. Antipov, S.N. Putilin, E.M. Kopnin et al: Physica C235240 (1994) 21. [H17] Y Maeno, H. Hashimoto, K. Yoshida et al.: Nature 372 (1994) 532.
References and bibliography
205
[H18] See, for example, M. Rapp, A. Murk, R. Semerad and W. Prusseit: Phys. Rev. Lett. 11 (1996) 928 and Yu.L Latyshev and J.E. Nevelskaya: Phys. Rev. Lett. 11 (1996) 932.
It should be remarked that the above list is compiled with the author's prejudice and is not meant to exhaust all the important works.
Index
d vector, 135 /vector, 135
upper—, 4 critical region, 125
A phase, 127 Ai phase, 127 Ai state, 137 a.c. Josephson effect, 62 A15 superconductor, 164 ABM state, 135 AbrikosovGor'kov theory, 96 AharonovBohm effect, 11 Andreev scattering, 65 antiferromagnetism, 168, 180
dwave, 189 density of states, 19 depairing, 66 di Gamma function, 34 dilute Bose gas, 8
B phase, 127 Bogoliubov transformation, 26, 31, 64, 187 BogoliubovAnderson mode, 51 Bogoliubovde Gennes equation, 64, 113 BoseEinstein condensation, 7, 185 boundary energy, 104 BW state, 134 CarlsonGoldman mode, 117 charge density, 36 circulation quantum, 6 Clogston (Pauli) limit, 44 coherence factor, 46 coherence length, 35, 170 coherent state, 12 collective mode, 51, 145 compressibility —of 3 He, 130 condensate, 7, 185 dynamics of—, 186 Cooper pair, 21 copper oxide superconductor, 165 Coulomb interaction, 86 —parameter, 89 Josephson term, 59 quasiparticle term, 58 critical current, 103 critical magnetic field, 4, 39 lower—, 4
effective interaction, 129 effective mass, 73, 131, 178 Einstein phonon, 83 electrical conductivity, 123 electronphonon interaction, 72 Eliashberg equation, 80 energy gap, 33, 139 excitonic mechanism, 163 Fermi liquid effect, 143 Fermi liquid theory, 129 fluctuations in a superconductor, 122, 174 flux quantum, 5 free energy density, 148 fullerene, 165 gap equation, 28 gapless state, 97 gauge invariance, 51 Ginzburg criterion, 125, 175 GinzburgLandau equation, 102 GinzburgLandau theory, 100, 148 GL parameter, 102, 171 Gor'kov equations, 68 gradient energy, 148 Green's function, 67 group theoretical classification, 182 healing distance, 9, 186 heavy electron system, 177 highTc superconductor, 164 Hubbard model, 168 impurity effect, 94
207
208
Index
interference effect, 61, 190 intrinsic angular momentum, 138 isotope effect, 92
planar state, 137 polar state, 137 proximity effect, 70
jellium model, 77 Josephson effect, 13, 56, 60, 189, 197 dwave—, 189
quasiparticle lifetime, 77, 96
Knight shift, 53, 173 Kondo effect, 98 Korringa equation, 55 Landau criterion, 14 Landau parameter, 130 London equation, 49 London limit, 49, 152 London penetration depth, 10, 102, 171 lower critical magnetic field, 4, 107 magnetic dipole interaction, 134, 144 magnetic free energy (GL theory), 149 mass enhancement parameter, 77 McMillan's formula, 92 meanfield approximation, 23 Meissner effect, 4 melting curve, 193 Migdal's theorem, 79 momentum density, 149 Mott insulator, 168 NambuGoldstone mode, 51, 117 neutron matter, 134 neutron star, 1 nonunitary pair, 25 nonlinear fluctuation, 176 normal component, 4 nuclear magnetic resonance (NMR), 145 shift in the resonance frequency, 146 nuclear spin relaxation, 172 nuclear spin relaxation time, 53 order parameter, 12, 100 organic superconductor, 165 pair —amplitude, 23 Cooper—, 21 dwave—, 189 unitary—, 25 pairing interaction, 132 paramagnon, 151 Pauli (Clogston) limit, 44 perfect diamagnetism, 4 perovskite type, 164 phase —slip centre (PSC), 121 —slip oscillation (PSO), 119 phase diagram —of superfluid 3 He, 127 superconductor—, 4 phonon, roton excitation, 14 pinning, 119
retardation, 80 rotating system, 156 semiclassical approximation, 70 Shapiro step, 63 Sommerfeld constant, 39, 177 specific heat, 140 —anomaly, 2 jump of—, 40 spectral density, 58, 59 spin dynamics, 145 spin fluctuation, 150 spin paramagnetism, 43 spinsinglet state, 24 spintriplet pwave pairing, 132 spintriplet state, 24 SQUID, 62 strong coupling theory, 80 strongcoupling effect, 89, 150 superconductivity, 1 superconductor copper oxide—, 165 highTc—, 164 type 1— 4, 107 type 2— 4, 107 supercurrent, 40 superfluid component, 4, 42, 140 superfluidity, 1 susceptibility, 131, 177 symmetry breaking, 12, 152 TDGL equation, 115 texture, 152 thermal conductivity, 50 tunnelling characteristics, 89 tunnelling junction, 56 twocomponent model, 4 type 1 superconductor, 4, 107 type 2 superconductor, 4, 107 ultrasound absorption, 47 unitary pair, 25 upper critical magnetic field, 4, 109 vortex lattice, 110, 176, 193 sliding of—, 118 vortex line core of—, 109 quasiparticle excitation associated with—, 113 vortex liquid, 176, 192 vortex structure —with a core, 153 continuous—, 154 weak coupling limit, 85